This book uses asymptotic methods to obtain simple approximate analytic solutions to various problems within mechanics,

*265*
*66*
*12MB*

*English*
*Pages 250
[251]*
*Year 2021*

- Author / Uploaded
- Igor V. Andrianov
- Jan Awrejcewicz
- Vladyslav Danishevskyy

*Table of contents : CoverHalf TitleTitle PageCopyright PageDedicationContentsPrefacePermissionsChapter 1: Models and Methods to Study Elastic Waves 1.1. Brief literature overview 1.2. Small “tutorial" 1.3. Analytical and numerical solutions in the theory of composite materials 1.4. Some general results of the homogenization theoryChapter 2: Waves in Layered Composites: Linear Problems 2.1. One-dimensional (1D) dynamic problem 2.2. Higher-order homogenization method 2.3. The Bloch-Floquet method and exact dispersion equation 2.4. Numerical resultsChapter 3: Waves in Fiber Composites: Linear Problems 3.1. Two-dimensional (2D) dynamic problem 3.2. Method of higher-order homogenization 3.3. The Bloch-Floquet method and solution based on Fourier series 3.4. Numerical results 3.5. Shear waves dispersion in cylindrically structured cancellous viscoelastic bonesChapter 4: Longitudinal Waves in Layered Composites 4.1. Fundamental relations of nonlinear theory of elasticity 4.2. Input boundary value problems 4.3. Macroscopic wave equation 4.4. Analytical solution for stationary waves 4.5. Analysis of solution and numerical resultsChapter 5: Antiplane ShearWaves in Fiber Composites with Structural Nonlinearity 5.1. Boundary value problem for imperfect bonding conditions 5.2. Macroscopic wave equation 5.3. Analytical solution for stationary waves 5.4. Analysis of solution and numerical resultChapter 6: Formation of Localized Nonlinear Waves in Layered Composites 6.1. Initial model and pseudo-spectral method 6.2. The Fourier-Pade approximation 6.3. Numerical modeling of non-stationary nonlinear wavesChapter 7: Vibration Localization in 1D Linear and Nonlinear Lattices 7.1. Introduction 7.2. Monatomic lattice with a perturbed mass 7.3. Monatomic lattice with a perturbed mass – the continuous approximation 7.4. Diatomic lattice 7.5. Diatomic lattice with a perturbed mass 7.6. Diatomic lattice with a perturbed mass – the continuous approximation 7.7. Vibrations of a lattice on the support with a defect 7.8. Nonlinear vibrations of a lattice 7.9. Effect of nonlinearity on pass bands and stop bandsChapter 8: Spatial Localization of Linear Elastic Waves in Composite Materials with Defects 8.1. Introduction 8.2. Wave localization in a layered composite material: transfer-matrix method 8.3. Wave localization in a layered composite material: lattice approach 8.4. Antiplane shear waves in a FIBER compositeChapter 9: Nonlinear Vibrations of Viscoelastic Heterogeneous Solids of Finite Size 9.1. Introduction 9.2. Input problem and homogenized dynamical equation 9.3. Discretization procedure 9.4. Method of multiple time scales 9.5. Numerical simulation of the modes coupling 9.6. Concluding remarksChapter 10: Nonlocal, Gradient and Local Models of Elastic Media: 1D Case 10.1. Introduction 10.2. A chain of elastically coupled masses 10.3. Classical continuous approximations 10.4. “Splashes” 10.5. Envelope continualization 10.6. Intermediate continuous models 10.7. Using of Pade approximations 10.8. Normal modes expansion 10.9. Theories of elasticity with couple-stresses 10.10. Correspondence between functions of discrete arguments and approximating analytical functions 10.11. The kernels of integro-differential equations of the discrete and continuous systems 10.12. Dispersive wave propagation 10.13. Green’s function 10.14. Double- and triple-dispersive equations 10.15. Toda lattice 10.16. Discrete kinks 10.17. Continualization of b-FPU lattice 10.18. Acoustic branch of a-FPU lattice 10.19. Anti-continuum limit 10.20. 2D lattice 10.21. Molecular dynamics simulations and continualization: handshake 10.22. Continualization and discretization 10.23. Possible generalization and applications and open problemsChapter 11: Regular and Chaotic Dynamics Based on Continualization and Discretization 11.1. Introduction 11.2. Integrable ODE 11.3. Continualization with Pade approximants 11.4. Numerical resultsReferencesIndex*

Linear and Nonlinear Waves in Microstructured Solids

Linear and Nonlinear Waves in Microstructured Solids Homogenization and Asymptotic Approaches Igor V. Andrianov

([email protected])

Jan Awrejcewicz

([email protected])

Vladyslav Danishevskyy

([email protected])

First edition published 2021 by CRC Press 6000 Broken Sound Parkway NW, Suite 300, Boca Raton, FL 33487-2742 and by CRC Press 2 Park Square, Milton Park, Abingdon, Oxon, OX14 4RN © 2021 Igor V. Andrianov, Jan Awrejcewicz and Vladyslav Danishevskyy CRC Press is an imprint of Taylor & Francis Group, LLC The right of Igor V. Andrianov, Jan Awrejcewicz and Vladyslav Danishevskyy to be identified as authors of this work has been asserted by them in accordance with sections 77 and 78 of the Copyright, Designs and Patents Act 1988. Reasonable efforts have been made to publish reliable data and information, but the author and publisher cannot assume responsibility for the validity of all materials or the consequences of their use. The authors and publishers have attempted to trace the copyright holders of all material reproduced in this publication and apologize to copyright holders if permission to publish in this form has not been obtained. If any copyright material has not been acknowledged please write and let us know so we may rectify in any future reprint. Except as permitted under U.S. Copyright Law, no part of this book may be reprinted, reproduced, transmitted, or utilized in any form by any electronic, mechanical, or other means, now known or hereafter invented, including photocopying, microfilming, and recording, or in any information storage or retrieval system, without written permission from the publishers. For permission to photocopy or use material electronically from this work, access www.copyright. com or contact the Copyright Clearance Center, Inc. (CCC), 222 Rosewood Drive, Danvers, MA 01923, 978-750-8400. For works that are not available on CCC please contact [email protected] Trademark notice: Product or corporate names may be trademarks or registered trademarks and are used only for identification and explanation without intent to infringe. Library of Congress Cataloging‑in‑Publication Data ISBN: [9780367704124] (hbk) ISBN: [9781003146162] (ebk) Typeset in Minion by KnowledgeWorks Global Ltd.

Dedication This is a modest contribution dedicated to the work and virtue of Professor Leonid I. Manevitch (02.04.1938 - 20.08.2020), a prominent figure in Dynamics and Mechanics of Composite Materials

Contents Preface.......................................................................................................................xi Permissions ............................................................................................................xvii Chapter 1

Models and Methods to Study Elastic Waves.................................. 1 1.1 1.2 1.3 1.4

Chapter 2

Waves in Layered Composites: Linear Problems .......................... 23 2.1 2.2 2.3 2.4

Chapter 3

3.4 3.5

Two-dimensional (2D) dynamic problem............................. 39 Method of higher-order homogenization.............................. 40 The Bloch-Floquet method and solution based on Fourier series ........................................................................ 46 Numerical results .................................................................. 48 Shear waves dispersion in cylindrically structured cancellous viscoelastic bones ..................................................... 50

Longitudinal Waves in Layered Composites ................................. 63 4.1 4.2 4.3 4.4 4.5

Chapter 5

One-dimensional (1D) dynamic problem ............................. 23 Higher-order homogenization method.................................. 24 The Bloch-Floquet method and exact dispersion equation... 29 Numerical results .................................................................. 34

Waves in Fiber Composites: Linear Problems............................... 39 3.1 3.2 3.3

Chapter 4

Brief literature overview ......................................................... 1 Small “tutorial”....................................................................... 7 Analytical and numerical solutions in the theory of composite materials .................................................................... 19 Some general results of the homogenization theory............. 20

Fundamental relations of nonlinear theory of elasticity ....... 63 Input boundary value problems ........................................... 65 Macroscopic wave equation ................................................. 66 Analytical solution for stationary waves .............................. 72 Analysis of solution and numerical results........................... 76

Antiplane Shear Waves in Fiber Composites with Structural Nonlinearity.......................................................................................... 81 5.1

Boundary value problem for imperfect bonding conditions. 81

vii

viii

Contents

5.2 5.3 5.4 Chapter 6

Formation of Localized Nonlinear Waves in Layered Composites ............................................................................................... 101 6.1 6.2 6.3

Chapter 7

7.4 7.5 7.6 7.7 7.8 7.9

Introduction......................................................................... 111 Monatomic lattice with a perturbed mass........................... 112 Monatomic lattice with a perturbed mass – the continuous approximation .............................................................. 114 Diatomic lattice................................................................... 115 Diatomic lattice with a perturbed mass .............................. 117 Diatomic lattice with a perturbed mass – the continuous approximation .................................................................... 121 Vibrations of a lattice on the support with a defect ........... 123 Nonlinear vibrations of a lattice ......................................... 123 Effect of nonlinearity on pass bands and stop bands .......... 126

Spatial Localization of Linear Elastic Waves in Composite Materials with Defects......................................................................... 129 8.1 8.2 8.3 8.4

Chapter 9

Initial model and pseudo-spectral method.......................... 101 The Fourier-Pad´e approximation ........................................ 103 Numerical modeling of non-stationary nonlinear waves .... 106

Vibration Localization in 1D Linear and Nonlinear Lattices ...... 111 7.1 7.2 7.3

Chapter 8

Macroscopic wave equation.................................................. 84 Analytical solution for stationary waves .............................. 92 Analysis of solution and numerical result ............................ 96

Introduction......................................................................... 129 Wave localization in a layered composite material: transfer-matrix method ....................................................... 130 Wave localization in a layered composite material: lattice approach....................................................................... 136 Antiplane shear waves in a FIBER composite.................... 137

Nonlinear Vibrations of Viscoelastic Heterogeneous Solids of Finite Size ....................................................................................... 141 9.1 9.2 9.3 9.4 9.5 9.6

Introduction......................................................................... 141 Input problem and homogenized dynamical equation........ 142 Discretization procedure..................................................... 145 Method of multiple time scales........................................... 147 Numerical simulation of the modes coupling..................... 149 Concluding remarks............................................................ 151

ix

Contents

Chapter 10

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case153 10.1 Introduction......................................................................... 153 10.2 A chain of elastically coupled masses ................................ 155 10.3 Classical continuous approximations ................................ 157 10.4 “Splashes”........................................................................... 159 10.5 Envelope continualization .................................................. 161 10.6 Intermediate continuous models ........................................ 162 10.7 Using of Pad´e approximations............................................ 164 10.8 Normal modes expansion ................................................... 167 10.9 Theories of elasticity with couple-stresses ......................... 169 10.10Correspondence between functions of discrete arguments and approximating analytical functions ................... 170 10.11The kernels of integro-differential equations of the discrete and continuous systems.............................................. 171 10.12Dispersive wave propagation .............................................. 175 10.13Green’s function.................................................................. 176 10.14Double- and triple-dispersive equations ............................. 176 10.15Toda lattice.......................................................................... 179 10.16Discrete kinks ..................................................................... 181 10.17Continualization of β -FPU lattice ...................................... 183 10.18Acoustic branch of α-FPU lattice ...................................... 186 10.19Anti-continuum limit ......................................................... 186 10.202D lattice............................................................................. 186 10.21Molecular dynamics simulations and continualization: handshake................................................ 189 10.22Continualization and discretization .................................... 190 10.23Possible generalization and applications and open problems..................................................................................... 190

Chapter 11

Regular and Chaotic Dynamics Based on Continualization and Discretization............................................................................... 193 11.1 11.2 11.3 11.4

Introduction......................................................................... 193 Integrable O∆E ................................................................... 195 Continualization with Pad´e approximants .......................... 196 Numerical results ................................................................ 197

References ............................................................................................................. 207 Index...................................................................................................................... 229

Preface Wave propagation in heterogeneous materials and structures is characterized by a number of significant phenomena, which can never be observed in homogeneous solids. In recent years, intensive studies have been devoted to phononic band gaps, negative refraction, dynamic anisotropy and waves focusing, acoustic diodes, acoustically invisible cloaks, waves localization in structures with defects. All these remarkable effects and properties have a great practical importance for a large variety of applications in physics, engineering, biomechanics, and many other areas. Composite materials, metamaterials and acoustic crystals, consisting of several components with different physical and mechanical properties, are widely used in modern civil and mechanical engineering, aircraft and rocketry industries. Examples of composites are reinforced plastics, concrete, laminated wood, plywood and many other materials. In recent years, technologies for creating nanocomposites have been intensively developed, in which reinforcing particles (fullerenes, nanotubes) have a characteristic size from 1 nm to 100 nm. Unlike ordinary substances, in the nanoparticles most of the atoms are placed on the surface, which leads to their extremely high stiffness and strength. Due to this, nanocomposites are characterized by special mechanical properties that significantly exceed the properties of traditional materials. From the point of view of mechanics, the main feature of modeling and calculation of composite materials is to take into account the heterogeneity of their internal structure. Therefore, models and methods of the theory of composites can also be used to study spatially heterogeneous structures, such as beams with attached masses, layered, ribbed, perforated plates and shells, pile foundations, and many others. The propagation of elastic strain waves in composite materials is accompanied multiple reflections and refractions of the signal on the nonhomogeneities of the internal structure, which lead to dispersion of the wave field and scattering of mechanical energy. The influence of nonlinearity, on the contrary, leads to the concentration of energy and to the generation of higher harmonics. In the case of a balance between the effects of dispersion and nonlinearity, the formation of stationary nonlinear waves (periodic or solitary) is possible, which propagate without changing the shape and speed. The properties of linear and nonlinear strain waves propagating in an nonhomogeneous medium substantially depend on the characteristics of the microstructure. Studying the processes of formation and propagation of waves, one can get detailed information about the internal structure and defects of the composite material. Localized nonlinear waves accumulate a significant amount of mechanical energy, which can lead to local destruction of structures. Therefore, the consideration of nonlinear effects is necessary when developing new, refined criteria for dynamic strength. The special properties of nonlinear waves (such as dispersion, localization, the dependence of the shape and propagation velocity on the amplitude) can be used to xi

xii

Preface

create various types of acoustic instruments and devices: vibration dampers, filters, receivers, transmitters and waveguides. Linear and nonlinear elastic waves in solids have been investigated by many authors. In most studies, homogeneous materials and structures were considered when the dispersion phenomenon is caused by geometric factors (the presence of bending forces, reflection of waves from the side surfaces of the waveguide, etc.). The propagation of strain waves in composite materials has been much less studied. Many approaches are phenomenological in nature; therefore, the numerical values of the coefficients in the wave equations are often not defined. It is assumed that they can be found experimentally. However, for many real materials, the exact values of the phenomenological parameters remain unknown. Therefore, the critical problem is the development of new methods for modeling linear and nonlinear waves in composite materials and finding solutions that would allow taking into account the influence of the internal structure of the medium on the processes of wave propagation at the macrolevel. This monograph can be treated as extension/continuation of our previous monograph [19]. In the mentioned book we considered the static problems of the theory of composites using asymptotic approaches. In the present book these approaches are generalized to the dynamic case. The same asymptotic methods are employed, i.e. the homogenization approach, singular and regular asymptotics, as well as one- and multi-point Pad´e approximations. In the first chapter of the book, we illustrate and discuss the mathematical models and the methods devoted to study elastic waves propagating in nonlinear and nonhomogeneous materials. First, a brief literature overview is presented highlighting various effects of the wave evolution including nonlinearity, dispersion and dissipation features. The nonlinearly exhibited by a solid body may include geometric, physical and structural components. Then the state-of-the art of the analytical/numerical approaches is presented with an emphasis to scale effects studied with the help of the asymptotic homogenization method. Namely, it is known that when the wavelength of a travelling wave signal becomes comparable with characteristic size of heterogeneities, reflections and refractions of the wave may generate polarization, dispersion and attenuation effects on both micro and macro level. In addition benefits given by asymptotic methods and with the homogenization method are outlined. The second chapter is aimed on the study of waves in layered materials from perspective of a linear analysis. First, 1D dynamic problem with a help of the BlochFloquet method is considered. The use of higher-order homogenization method is described. Next, the solution to the exact dispersion equation is compared with that obtained through the Bloch-Floquet method. Two numerical examples are presented. The similar like methodology is presented in Chapter 3 where waves in fiber composites are investigated in frame of linear statement. First, the 2D dynamical problem is considered. Then the method of higher-order homogenization is employed to solve the problem. The comparison of solutions yielded by the Bloch-Floquet method and

Preface

xiii

by the standard Fourier series approximation is carried out based on numerical investigations. Moreover, the shear waves dispersion in cylindrically structured cancellous viscoelastic bones are modeled and analyzed. Longitudinal waves in layered composite materials exhibiting both physical and geometric nonlinearity are analyzed in Chapter 4. In beginning, the fundamental relations of nonlinear theory of elasticity are introduced. Then, a solution to the macroscopic wave equation is derived. Furthermore, analytical solution for stationary waves propagation constant velocity and form is obtained including the case of soft and hard nonlinearity. Numerical examples validating the obtained solutions are provided. Chapter 5 is devoted to the antiplane shear waves in fiber composite with an account of a structural nonlinearity. Boundary value problem for imperfect bounding conditions is defined first. Then the microscopic wave equation is solved using the method of homogenization. Analytical solution governing stationary wave propagation is derived including soft and hard nonlinearity effects. Formation and propagation of localized nonlinear waves in composite materials are considered in Chapter 6. The model of longitudinal waves propagating in a layered composite in a direction perpendicular to the layers arrangement is derived and solved using the pseudo-spectral method and the Fourier-Pad´e approximation. Moreover, the numerical analysis of formation and propagation of non-stationary nonlinear waves is carried out including three cases: (i) generation of a single localized wave; (ii) generation of a train of localized waves; (iii) scattering of an initial impulse of tension. Localization of vibrations in 1D linear and nonlinear lattices based on the developed discrete and continuous model is analyzed in Chapter 7. First, a monatomic lattice with a perturbed mass is studied based on lumped-mass approximation. Then the same problem is solved based on the continuous approximation of mass distribution. Then, the same methodology is employed to study of a diatomic lattice. The problem of vibration of a lattice on the support with a defect is solved. Moreover, the problem governed by a set of second-order ODEs with the Duffing-type nonlinearity governing vibration of a lattice is solved. The effects of nonlinearity on pass bands and stop bands are outlined. Chapter 8 deals with spatial localization of linear elastic waves in composite materials with defects. We begin with a simple problem of an elastic composite material consisting of two alternating layers which is solved by the transfer-matrix method. Then, the problem of localization in a layered composite material based on lattice approach is solved. Moreover, antiplane shear waves in a fiber 2D composite are analyzed. The aim of the Chapter 9 is to study how viscous damping influences mode coupling in nonlinear vibrations of microstructured solids. Natural longitudinal vibrations of a layered composite are considered. The macroscopic dynamic equation is obtained by asymptotic homogenization. The input continuous problem is analyzed using a spatial discretization procedure. An asymptotic solution is developed by the method of multiple time scales and the fourth-order Runge-Kutta method is

xiv

Preface

employed for numerical simulations. Internal resonances and energy transfers between the vibrating modes are predicted and analyzed. The conditions for possible truncation of the original infinite system are discussed. The obtained numerical and analytical results are in good agreement. Chapter 10 focuses on continuous models derived from a discrete microstructure. Various continualization procedures that approximately take into account the nonlocal interaction between variables of the discrete media are analyzed. Theories of elasticity with couple-stresses are also under consideration. Continualizations of FPU lattice are analyzed. Relations between molecular dynamics simulations and continualization as well as between continualization and discretization are also described. In Chapter 11 we study various variants of Verhulst-like ODE and ordinary difference equations. Usually Verhulst ODE serves as an example of a deterministic system and discrete logistic equation is a classic example of a simple system with very complicated (chaotic) behavior. We present examples of deterministic discretization and chaotic continualization. Continualization procedure is based on Pad´e approximants. To correctly characterize the dynamics of obtained ODE we measured such characteristic parameters of chaotic dynamical systems as the Lyapunov exponents and the Lyapunov dimensions. It is assumed that the reader has knowledge of basic calculus as well as the elementary properties of ODEs and PDEs, strength of materials and theory of elasticity and oscillation theory. Our previous monograph contains a voluminous tutorial, which we do not repeat in this book but recommends for a quick acquaintance with the applied technique. Further development of the book described in this monograph can go in the following directions: 1. The solution of specific tasks important for practice, for example, the study waves in viscoelastic composites with imperfect bonding between components, wave propagation in layered composites with degraded matrices at locations of imperfect bonding, etc. [30, 31]. 2. Calculation of dynamics of composite materials of finite size [21, 24]. Perhaps, it is more efficient to apply spectral or pseudo-spectral methods from the very beginning to study these systems. In this case, methods for overcoming of the Wilbraham-Gibbs phenomenon require further development. In particular, previous results show that the combination of Pad´e approximants and filter function improve converges of used series better. 3. The use of short-wave homogenization methods [126, 130, 133] seems promising. 4. Most of the real composites possess random microstructures. For analysis of this composites a lot of homogenization techniques can be found in literature such as ensemble averaging [459]. Example calculations demonstrate that “effective modulus” and “effective density” are operators, nonlocal in space and time [313, 460, 461].

Preface

xv

Hence, in order to obtain the exact homogenized solution, one needs, generally speaking, an infinite set of correlation functions, which are intended to provide a statistical description of the microgeometry of the composite. Naturally, in many cases such a description is not available. On the other hand, various methods give a possibility to estimate bounds for the effective properties using only a limiting amount of microstructural information. As it were shown, in many cases a regular composite possesses the extreme effective properties among the corresponding random structures [75, 76, 252, 477]. Therefore, a solution for the perfectly regular composite can be considered as bounds on the effective coefficient of random ones, at least for the shaking-geometry random structures [33]. The limitation of the analytical approaches motivated their usage of the finite element model of the unit cell. The numerical homogenization not being bound to certain geometries for the structure of the unit cell [7, 312]. Numerical solutions are important not only on their own, but they also give possibillity to evaluate the applicability of analytical solutions and refine them. At the same time, analytic solutions can be used as benchmark results for numerical ones. They also are impotant for solving of optimization problems and as the first approximation for numerical approaches. We would like to acknowledge A.L. Kalamkarov, V.I. Malyi, L.I. Manevitch, V.V. Mityushev, A.V. Porubov, G.A. Starushenko, H. Topol, D. Weichert for the helpful and inspiring exchanges of ideas, fruitful collaboration, stimulating discussions, encouraging remarks and thoughtful criticism we have received over the years. In addition, let us acknowledge that some results presented in this monograph have been supported by (i) the German Research Foundation (Deutsche Forschungsgemeinschaft), grant no. WE736/30-1 (I.V. Andrianov), (ii) Alexander von Humboldt Foundation (grant no.3.4-Fokoop-UKR/1070297) and European Union Horizon 2020 Research and Innovation Programme (Maria Sklodowska-Curie grant no. 655177) (V.V. Danishevskyy), and (iii) Polish Natonal Science Centre under the grant OPUS14 No. 2017/27/B/ST8/01330 (J. Awrejcewicz). We are aware of the fact that the book may contain controversial statements, too personal or one-sided arguments, inaccuracies and typographical errors. Any of remarks, comments and criticisms regarding the book are appreciated.

Aachen, Germany Lodz, Poland Dnipro, Ukraine

Igor V. Andrianov Jan Awrejcewicz Vladyslav V. Danishevskyy

Permissions Figures 4.3–4.8 is reprinted from the paper “Dynamic homogenization and wave propagation in a nonlinear 1D composite material” authored by I. Andrianov, V. Danishevs’kyy, O. Ryzhkov, D. Weichert, Wave Motion, vol. 50, pages 271–281, 2013. Copyright 4913751111215 (2020), with permission from Elsevier. Figures 5.4–5.12 is reprinted from the paper “Anti-plane shear waves in a fiberreinforced composite with a non-linear imperfect interface” authored by V. Danishevs’kyy, J. Kaplunov, G. Rogerson, International Journal of Non-linear Mechanics, vol. 76, pages 223–232, 2015. Copyright 4915481459476 (2020), with permission from Elsevier. Figures 6.1–6.9 is reprinted from the paper “Numerical study of formation of solitary strain waves in a nonlinear elastic layered composite material” authored by I.V. Andrianov, V.V. Danishevs’kyy, O.I. Ryzhkov, D. Weichert, Wave Motion, vol. 51, pages 405–417, 2014. Copyright 4913760036534 (2020), with permission from Elsevier. Text and figures of Chapter 7 are reprinted from the paper “Vibration localization in one-dimensional linear and nonlinear lattices: discrete and continuum models” authored by I.V. Andrianov, V. Danishevs’kyy, A.L. Kalamkarov, Nonlinear Dynamics, vol. 72 (1-2), pages 37–48, 2013. Copyright 4915400154694 (2020), with permission from Springer Nature. Text and figures of Chapter 8 are reprinted from the paper “Spatial localization of linear elastic waves in composite materials with defects” authored by I.V. Andrianov, V.V. Danishevs’kyy, Ie.A. Kushnierov, ZAMM, vol. 94, pages 1001–1010, 2014. Copyright 4914180424490 (2020), with permission from John Wiley and Sons. Text and figures of Chapter 9 are reprinted from the paper “Internal resonances and modes interactions in non-linear vibrations of viscoelastic heterogeneous solids” authored by I.V. Andrianov, V.V. Danishevskyy, G. Rogerson, vol. 433, pages 55– 64, 2018, Journal of Sound and Vibration. Copyright 4914141333640 (2020), with permission from Elsevier.

xvii

and Methods to 1 Models Study Elastic Waves in Nonlinear and Nonhomogeneous Materials In this chapter problems of wave propagation in heterogeneous materials and structures and existing approaches for their effective solutions are analyzed. The main features which must be taken into account are dispersion, dissipation and nonlinearity. They are caused by polarization, reflections and refraction at the microinhomoneinities, as well as geometric, physical and structural nonlinearities. The existing methods of analysis are mainly based on the homogenization and Bloch-Floquet approaches. General ideas of higher- order homogenization are described based on a simple case study. The papers and books dealing with analytical and numerical solutions are also reviewed. Relations between numerical and analytical solutions are analyzed. Advantages of analytical approaches are outlined. General results yielded by the homogenization theory are presented and discussed.

1.1

BRIEF LITERATURE OVERVIEW

Composite materials are materials consisting of several components with different physical and mechanical characteristics. By the special choice of their volume fractions and geometric shapes, it is possible to create new structural materials with valuable properties like those having high strength and stiffness with low weight, materials with improved heat and electrical conductivity, materials characterized by resistance to aggressive environments, etc. Consider the characteristic scale l of the internal structure of the composite (the size of the reinforcing particle or grain) is small in comparison to the size of the structure. At the same time, it is assumed that l is much larger than an interatomic distance. In this case, the physical behavior of the composite material can be described using equations of continuum mechanics. Literature dedicated to the statics of composite materials is thoroughly analyzed in [19]. In this monograph, we focus on the dynamic problems. Generally, in the problems of dynamics, one of the manifestations of the scale effect stands for the dispersion of waves in composites caused by local reflections and refractions of the signal on the nonhomogeneities of the medium. Boutin [89–91], Boutin and Auriault 1

2

Linear and Nonlinear Waves in Microstructured Solids

[92], Bakhvalov and Eglit [53, 54], Fish and Chen [120, 170, 171] using the higherorder homogenization method obtained solutions suitable for long waves analysis (η 0,

(1.27)

at y < 0,

m

−E ) c(E −E ) where A1 = − (1−c)(E , B1 = (1−c)E in +cE m , C1 = −B1 ; c is the inclusions’ vol(1−c)E in +cE m ume fraction, c = 2a/L . Terms containing ua2 are eliminated using condition (1.23). As the result, we derive the macroscopic equilibrium equation of the order O(η 0 ):

hEi0 where hEi0 =

∂ 2 u0 = −X + hλ i u0 , ∂ x2

E in E m , (1 − c) E in + cE m

hλ i = (1 − c)λ m + cλ in

(1.28)

(1.29)

are the O(η 0 ) order effective modulus. Expression (1.29) coincides with a well-known formula for the effective elastic modulus of the laminated composite material obtained by simple arithmetical averaging of the components’ compliances: c 1 − c −1 hEi0 = + . (1.30) E in Em This is so-called Reuss averaging, and it is known that it gives lower bound for real effective parameter. Solution of the cell problem (1.13), (1.18), (1.21), (1.25) is: at y > 0: 2 1 λ in hEi0 2 1 ∂ u0 in 1 + 2A1 − y + A2 Ly , u2 = − hλ i E in 2 4 ∂ x2 (1.31) 2 1 λ m hEi0 2 1 1 m 2 ∂ u0 u2 = − 1 + 2B1 − y + B2 Ly + C2 L , hλ i E m 2 4 8 ∂ x2

13

Models and Methods to Study Elastic Waves

at y < 0: 2 1 λ in hEi0 2 1 d u0 = − 1 + 2A1 − y − A2 Ly , hλ i E in 2 4 dx2 2 1 λ m hEi0 2 1 1 2 ∂ u0 m , 1 + 2B1 − y − B2 Ly + C2 L u2 = − hλ i E m 2 4 8 ∂ x2 uin 2

where A2 = −

c (1 − c) E m E in λ in − E m λ m

, (1.32) [(1 − c) λ m + cλ in ] [(1 − c) E in + cE m ]2 2 (1 − c) (1 + 2c) λ in − 2cλ m E in − B2 = c [(1 − c) λ m + cλ in ] [(1 − c) E in + cE m ]2 n o 1 − 3c + 4c2 λ m − 4c2 λ in E in E m + 2c (1 − c) λ m + cλ in (E m )2 , c [(1 − c) λ m + cλ in ] [(1 − c) E in + cE m ]2 2 (1 − c) λ in − λ m E in 2 C2 = −c − [(1 − c) λ m + cλ in ] [(1 − c) E in + cE m ]2 m in E in E m − (1 − c) λ m + cλ in (E m )2 2 (1 − 2c) λ + 2cλ . c [(1 − c) λ m + cλ in ] [(1 − c) E in + cE m ]2 Substituting expressions (1.31) into equation (1.14) and performing the homogenization we obtain that all integrals in the homogenizing operator vanish. Therefore, in the problem under consideration, the displacement components ua2 do not contribute to the macroscopic equation. Solution of the cell problem (1.14), (1.19), (1.21), (1.25) is: at y > 0: 3 1 λ in hEi0 3 1 1 ∂ u0 2 2 = uin 2 + 3A + (A − 2) y − A Ly + A L y , 1 1 2 3 3 hλ i E in 6 4 24 ∂ x3 1 λ m hEi0 3 1 λ m hEi0 = um 2 + 3B + (B − 2) y − B +C −C Ly2 + 1 1 2 1 1 3 hλ i E m hλ i E m 6 4 3 1 1 2 3 ∂ u0 B3 L y + C3 L , 24 48 ∂ x3 (1.33) at y < 0: 3 1 λ in hEi0 3 1 1 ∂ u0 2 2 in 2 + 3A1 + (A1 − 2) y + A2 Ly + A3 L y , u3 = hλ i E in 6 4 24 ∂ x3 λ m hEi0 3 1 λ m hEi0 1 2 + 3B1 + (B1 − 2) y + B +C −C Ly2 + um 2 1 1 3 = hλ i E m hλ i E m 6 4 3 1 1 2 3 ∂ u0 B3 L y − C3 L , 24 48 ∂ x3

14

Linear and Nonlinear Waves in Microstructured Solids

where A3 =

c (1 − c) E m E in λ in − E m λ m

(1 − c) E in − cE m

, (1.34) [(1 − c) λ m + cλ in ] [(1 − c) E in + cE m ]3 3 (1 − c) 3c2 λ m + (1 − c) (1 + 3c) λ in E in B3 = c − [(1 − c) λ m + cλ in ] [(1 − c) E in + cE m ]3 h 2 1 + c + 4c2 − 9c3 λ m + c (1 − c) (2 + 9c) λ in E in E m − c [(1 − c) λ m + cλ in ] [(1 − c) E in + cE m ]3 m 2 2 in E in (E m )2 + c (1 − c) λ m + cλ in (E m )3 2 1 − 2c + 9c λ − 9c λ , c [(1 − c) λ m + cλ in ] [(1 − c) E in + cE m ]3 3 (1 − c) cλ m + (1 − c) λ in E in C3 = −c2 − [(1 − c) λ m + cλ in ] [(1 − c) E in + cE m ]3 h 2 1 + c − 3c2 λ m + (1 − c) (1 − 3c) λ in E in E m + c2 [(1 − c) λ m + cλ in ] [(1 − c) E in + cE m ]3 (1 − c) λ m + cλ in (E m )3 3 . c [(1 − c) λ m + cλ in ] [(1 − c) E in + cE m ]3 Applying the homogenizing operator to equations (1.13), (1.15) and combining the results we come to the macroscopic equilibrium equation of the order O(η 2 ): hEi0 where

∂ 4 u0 ∂ 2 u0 2 2 hEi + η L = −X + hλ i u0 , 2 ∂ x2 ∂ x4

2 2 1 c2 (1 − c) E in E m E in λ in − E m λ m hEi2 = 48 [(1 − c) ρ m + cρ in ]2 [(1 − c) E in + cE m ]3

(1.35)

(1.36)

can be treated as the O(η 2 ) order effective modulus. If we suppose λ in = λ m , then 2 1 c2 (1 − c) E in E m E in − E m hEi2 = 48 [(1 − c) E in + cE m ]3

2 .

(1.37)

The second term on the left-hand side of equation (1.35) represents the influence of the microstructural scale effect on the macroscopic material’s behavior. It can be easily seen that the scale effect disappears in the case of a homogeneous material (c = 0, c = 1 or E in = E m ). Analysis of the ratio of the second-to-first constitutive terms in equation (1.35) allows to estimate the range of applicability of the homogenization procedure. Now, let us consider a dynamic problem for the laminated composite material governed by the following PDEs: Ea

∂ 2 ua ∂ 2 ua = ρa 2 , 2 ∂x ∂t

(1.38)

15

Models and Methods to Study Elastic Waves

where ρ a are the mass densities of the components. Conditions of the perfect bonding between the matrix and inclusions are introduced by equations (1.5) and (1.6). Following the algorithm presented above we introduce the small parameter η (1.7), slow x and fast y co-ordinates (1.7), and search the displacements as the asymptotic expansion (1.8). Splitting of equation (1.38) with respect to η yields: at η −2 : ∂ 2 u0 E a 2 = 0, (1.39) ∂y at η −1 : 2 ∂ u0 ∂ 2 ua1 + = 0, Ea 2 ∂ x∂ y ∂ y2

(1.40)

at η 0 : E

a

E

a

∂ 2 ua1 ∂ 2 ua2 ∂ 2 u0 + 2 + ∂ x2 ∂ x∂ y ∂ y2

∂ 2 ua2 ∂ 2 ua3 ∂ 2 ua1 + 2 + ∂ x2 ∂ x∂ y ∂ y2

∂ 2 ua3 ∂ 2 ua4 ∂ 2 ua2 + 2 + ∂ x2 ∂ x∂ y ∂ y2

= ρa

∂ 2 u0 , ∂t 2

(1.41)

= ρa

∂ 2 ua1 , ∂t 2

(1.42)

= ρa

∂ 2 ua2 ∂t 2

(1.43)

at η 1 :

at η 2 : E

a

and so on. The set of equations (1.16)–(1.20) as well as equations (1.21)–(1.26) remain the same as in the static case. In the dynamic problem the macroscopic boundary conditions (1.26) should be accompanied by certain initial conditions, for example ∂ u0 (1.44) u0 = U3 |t=0 , = U4 . ∂t t=0 Equations (1.16) and (1.39) are satisfied trivially since ∂ u0 /∂ y = 0. The firstorder cell problem is defined by equations (1.17), (1.21), (1.25), (1.40) and thus coincides with the first-order cell problem of the static case. The solution for ua1 is given by expressions (1.27). Substituting ua1 into equation (1.41) and applying the homogenizing operator Z Z (·)dy L−1 , (1.45) (·)dy + Ωin 0

Ωm 0

we derive the macroscopic equation of motion of the O(η 0 ) order: hEi0

∂ 2 u0 ∂ 2 u0 hρi = , ∂ x2 ∂t 2

(1.46)

16

Linear and Nonlinear Waves in Microstructured Solids

where hEi0 is the O(η 0 ) order effective modulus determined by formula (1.29), hρi is the homogenized mass density of the composite material, hρi = (1 − c)ρ m + cρ in . Solution of the cell problem (1.18), (1.21), (1.25), (1.41) is: at y > 0: 2 1 ρ in hEi0 2 1 ∂ u0 in u2 = − , 1 + 2A1 − y + A2 Ly in hρi E 2 4 ∂ x2 (1.47) 2 ρ m hEi0 2 1 1 1 m 2 ∂ u0 1 + 2B1 − y + B2 Ly + C2 L , u2 = − hρi E m 2 4 8 ∂ x2 at y < 0: 2 1 ρ in hEi0 2 1 d u0 = − 1 + 2A1 − y − A2 Ly , in hρi E 2 4 dx2 2 ρ m hEi0 2 1 1 1 2 ∂ u0 um = − 1 + 2B − y − B Ly + C L , 1 2 2 2 hρi E m 2 4 8 ∂ x2 uin 2

where A2 = −

c (1 − c) E m E in ρ in − E m ρ m

, (1.48) [(1 − c) ρ m + cρ in ] [(1 − c) E in + cE m ]2 2 (1 − c) (1 + 2c) ρ in − 2cρ m E in B2 = c − [(1 − c) ρ m + cρ in ] [(1 − c) E in + cE m ]2 1 − 3c + 4c2 ρ m − 4c2 ρ in E in E m + 2c (1 − c) ρ m + cρ in (E m )2 c , [(1 − c) ρ m + cρ in ] [(1 − c) E in + cE m ]2 2 (1 − c) ρ in − ρ m E in 2 C2 = −c − [(1 − c) ρ m + cρ in ] [(1 − c) E in + cE m ]2 m in E in E m − (1 − c) ρ m + cρ in (E m )2 2 (1 − 2c) ρ + 2cρ . c [(1 − c) ρ m + cρ in ] [(1 − c) E in + cE m ]2 Substituting expressions (1.47) into equation (1.42) and performing the homogenization we obtain that all integrals in the homogenizing operator vanish. Therefore, in the problem under consideration, the displacement components ua2 do not contribute to the macroscopic equation. However, Boutin and Auriault [92] have shown that such contribution do take place in dynamic problems for anisotropic composite materials, where the O(η 1 ) order macroscopic equation describes the phenomenon of polarization. Solution of the cell problem (1.19), (1.21), (1.25), (1.42) is:

17

Models and Methods to Study Elastic Waves

at y > 0: 3 1 1 ∂ u0 ρ in hEi0 3 1 in 2 2 u3 = y − A2 Ly + A3 L y , 2 + 3A1 + (A1 − 2) in hρi E 6 4 24 ∂ x3 1 ρ m hEi0 3 1 ρ m hEi0 um = y − Ly2 + 2 + 3B + (B − 2) B +C −C 1 1 2 1 1 3 hρi E m hρi E m 6 4 3 1 ∂ u0 1 B3 L2 y + C3 L3 , 24 48 ∂ x3 (1.49) at y < 0: 3 ρ in hEi0 3 1 1 ∂ u0 1 2 2 2 + 3A + (A − 2) y + A Ly + A L y , = uin 1 1 2 3 3 hρi E in 6 4 24 ∂ x3 1 ρ m hEi0 3 1 ρ m hEi0 um = 2 + 3B + (B − 2) y + B +C −C Ly2 + 1 1 2 1 1 3 hρi E m hρi E m 6 4 3 1 1 2 3 ∂ u0 , B3 L y − C3 L 24 48 ∂ x3 where

c (1 − c) E m E in ρ in − E m ρ m

(1 − c) E in − cE m

, [(1 − c) ρ m + cρ in ] [(1 − c) E in + cE m ]3 3 (1 − c) 3c2 ρ m + (1 − c) (1 + 3c) ρ in E in B3 = c − [(1 − c) ρ m + cρ in ] [(1 − c) E in + cE m ]3 h 2 1 + c + 4c2 − 9c3 ρ m + c (1 − c) (2 + 9c) ρ in E in E m c − [(1 − c) ρ m + cρ in ] [(1 − c) E in + cE m ]3 m 2 2 in E in (E m )2 2 1 − 2c + 9c ρ − 9c ρ − c [(1 − c) ρ m + cρ in ] [(1 − c) E in + cE m ]3 (1 − c) ρ m + cρ in (E m )3 3 , c [(1 − c) ρ m + cρ in ] [(1 − c) E in + cE m ]3 3 (1 − c) cρ m + (1 − c) ρ in E in 2 + C3 = −c [(1 − c) ρ m + cρ in ] [(1 − c) E in + cE m ]3 h 2 1 + c − 3c2 ρ m + (1 − c) (1 − 3c) ρ in E in E m 2 c − [(1 − c) ρ m + cρ in ] [(1 − c) E in + cE m ]3 1 − c − 3c2 ρ m + 3c2 ρ in E in (E m )2 2 + c [(1 − c) ρ m + cρ in ] [(1 − c) E in + cE m ]3 (1 − c) ρ m + cρ in (E m )3 3 c . [(1 − c) ρ m + cρ in ] [(1 − c) E in + cE m ]3 A3 =

(1.50)

18

Linear and Nonlinear Waves in Microstructured Solids

Applying the homogenizing operator to equations (1.41), (1.43) and combining the results we come to the macroscopic equation of motion of the O(η 2 ) order: hEi0 where

∂ 2 u0 ∂ 2 u0 ∂ 4 u0 2 2 hEi hρi + η L = , 2 ∂ x2 ∂ x4 ∂t 2

2 2 1 c2 (1 − c) E in E m E in ρ in − E m ρ m hEi2 = 48 [(1 − c) ρ m + cρ in ]2 [(1 − c) E in + cE m ]3

(1.51)

(1.52)

is the O(η 2 ) order effective modulus in the dynamic case. The second term in equation (1.51) represents the influence of the microstructural scale effect, which leads to the phenomenon of dispersion on macro level. If the impedances of the components are identical (E in ρ in = E m ρ m ) then hEi2 vanishes and the macroscopic equation (1.51) turns to the non-dispersive form (1.46). From the physical point of view, this means that there are no reflections of the waves at the components’ interfaces. Assuming ρ in = ρ m yields (1.37). Expression (1.52) also coincides with those obtained in [120, 170, 171, 399]. Also, as shown in section 2.3, the first terms of the expansion of the solution of the exact dispersion equation (which can be obtained for the problem under consideration) in a series in a small parameter η, coincide with those obtained with the asymptotic homogenization method. In [399], a solution of equation (1.52) was compared with a numerical solution of the original problem. Gaussian initial disturbance was chosen. The discrepancy between the numerical solution of exact and the homogenized problems becomes sufficiently large only at very large times. Surprisingly, some mathematicians call the representation of the form (1.51) “criminal algorithm”, because it mixed different powers of small parameter in one higher-order homogenized equations [10,269,399]. At the same time, it is noted that such equations have a higher degree of approximation [10]. Solution (1.52) shows that in this case the homogenization approach gives an upper bound estimation for the eigenvalues. Since it stands for a constructive estimate, it is interesting to trace what is known about a priori estimations. In the general case, the problem of constructing such estimations can be formulated as follows. For many problems, the eigenvalues are the minima of some quadratic functionals. Moreover, often the initial formulation of the problem exhibits a symmetry, while the variable coefficients of quadratic forms are asymmetric. A study of the behavior of the minima of such functionals with a change in the degree of asymmetry of the coefficient was carried out in [207, 473, 475]. In [475], it was shown that for a wide range of problems, the natural vibration frequencies do not decrease when the density is symmetrized. In [207, 473] this result was generalized to symmetrization of the stiffnesses of the original system.

Models and Methods to Study Elastic Waves

1.3

19

ANALYTICAL AND NUMERICAL SOLUTIONS IN THE THEORY OF COMPOSITE MATERIALS “The speed of computation as a limiting factor in simulating physical systems has largely been replaced by the difficulty of extracting useful information from large data sets”. J. Guckenheimer [191]

We live in the era of Big Data and AI, ANNs and powerful commercial codes. Large datasets are becoming increasingly available and important in science and technology. However, our ability to understand the ongoing processes, as before, is based on simple models [35]. Like 50 years ago, “The purpose of computing is insight, not numbers” [200]. In our opinion, there is no question of “asymptotic or computer (numerical) modeling”. Both of these scientific directions are equally important [14, 15]. As shown in [13], without a clear understanding of the asymptotic nature of any model of applied mathematics, it is impossible to correctly determine its place in the hierarchy of describing various aspects of the phenomenon. In addition, the more powerful numerical algorithms become, the more the role of a successful zero approximation increases. All these algorithms require a suitable initial seed values to start the approximation. For essentially nonlinear problems, it is important to know in the vicinity of which we construct the solution. Otherwise, the most advanced numerical algorithm will be unstable, the solution may diverge, or we will get a parasitic solution. Asymptotic solutions often allow finding such suitable initial seed values. “When we bundle exacting algorithms into libraries and wrap them into packages to facilitate easy use, we create de facto standards that make it easy to ignore numerical analysis. We regard the existing base as static and invest in the development of problem-solving environments and high-level languages. This is needed, but we also need to maintain our investment in continuing research on algorithms themselves” [192]. An increase of the number of program packages developed on the basis of unknown for users’ principles results in an increase of chance of omitting the existence of their limitations and principal systematic errors. From this point of view, asymptotic methods are not only a useful analysis tool, but also provide important and useful benchmark solutions. A possibility of getting information has significantly increased in recent years. This implies high quality tools for its safe keeping and a transformation in a manner to be understandable by a human being. The last requirement is related to: a) construction of low dimensional models; b) aggregation of high dimensional information; c) extraction of the most important singularities in a system’s behaviour (for instance, the bifurcation points), and so on. The most suitable tools to realize the mentioned requirements are related to analytical, and in particular, to asymptotic methods. Discrete numerical solution refers to applications of the finite elements and difference methods. These methods are powerful and their application is reasonable when the geometry and the physical parameters are fixed. Many experts perceive a pris-

20

Linear and Nonlinear Waves in Microstructured Solids

tine computational block (package) as an exact formula: just substitute data and get the result! However, a sackful of numbers is not as useful as an analytical formula. Pure numerical procedures can fail as a rule for the critical parameters and analytical matching with asymptotic solutions can be useful even for the numerical computations [457]. Moreover, numerical packages sometimes are presented as a remedy from all deceases. It is worth noting again that numerical solutions are useful if we are interested in a fixed geometry and fixed set of parameters for engineering purposes. Analytical formula are useful to specialists developing codes for composites, especially for optimal design. We are talking about the creation of highly specialized codes, which enable to solve a narrow class of problems with exceptionally high speed. “It should be emphasized that in problem of design optimization the requirements of accuracy are not very high. A key role plays the ability of the model to predict how the system reacts on the change of the design parameters. This combination of requirements opens a road to renaissance of approximate analytical and semi-analytical models, which in the recent decades have been practically replaced by “universal codes” [169]. Asymptotic approaches allow us to define really important parameters of the system. The important parameters in a boundary value problem are those that, when slightly perturbed, yield large variations in the solutions. In other words, asymptotic methods make it possible to evaluate the sensitivity of the system. There is no need to recall that in real problems the parameters of composites are known with a certain (often not very high) degree of accuracy. This causes the popularity of various kinds of assessments in engineering practice. In addition, the fuzzy object oriented (robust in some sense) model is useful to the engineer. Multiparameter models rarely have this quality. “You can make your model more complex and more faithful to reality, or you can make it simpler and easier to handle. Only the most naive scientist believes that the perfect model is the one that represents reality” [186]. It should also be remembered that for the construction of multiparameter models it is necessary to have very detailed information on the state of the system. Obtaining such information for an engineer is often very difficult for a number of objective reasons, or it requires a lot of time and money. It should be emphasized that the most natural way of constructing sufficiently accurate low-parametric models is based on the use of the asymptotic methods.

1.4

SOME GENERAL RESULTS OF THE HOMOGENIZATION THEORY

For the past years’ homogenization methods have proven to be powerful techniques for the study of heterogeneous media. Homogenization approach can be used for local and integral functionals [338]. For analysis of ODEs and PDEs the classical tools include multiple-scale expansions [70] or Bakhvalov’s ansatz [55, 345] usually used. An approach based on Fourier analysis was proposed in [128]. This method works in the following way. First, original operator is transformed into an equivalent operator in the Fourier space. The standard Fourier series is used to expand the coefficients of the operator and a Fourier transform is used to decompose the integrals. Next, the

Models and Methods to Study Elastic Waves

21

Fourier transforms of the integrals are expanded using a suitable two-scale expansion, and the homogenized problem is finally derived by neglecting higher-order terms in the above expansions when moving to the limit as the period tends to zero. Another use of Fourier analysis for homogenization of ODEs and PDEs was proposed in [34]. This variant of homogenization is strongly based on Vishik amd Lyusternik asymptotic results for ODEs and PDEs with rapidly changing coefficients and boundary conditions [451]. We also mention papers on homogenization using nonsmooth transformations [365, 366]. G- and Γ-variational convergences theories [132, 338] are used to identify the asymptotic limit for the integral functionals. In our book we deal with local operators, i.e. PDEs and ODEs with rapidly oscillating or periodically discontinuous coefficients and we use homogenization method, based on multiple-scale expansions. Mathematical homogenization method gives possibility to obtain many general results useful for problems considered in our book [48–52, 56, 149, 150]. An important issue is the variational formulation of the problems in the theory of composites. In [48], the following two problems are solved. (1) It is shown that for a certain interpretation of the the Euler equation for a stationary point of a periodic functional in the approximation of any order of accuracy with respect to a small microinhomogeneity parameter, the Euler equation corresponds to a certain “averaged” functional. (2) Let the periodic medium be such that for some processes there exists an energy integral in it. In this case, the homogenized equation also has an energy integral. An important question is whether the occurrence of dissipation in a composite composed of components without dissipation is possible. For composites of a periodic structure, dissipation does not occur [48]. In random composites viscosity, and hence dissipation, occurs even if it is absent in all components [50]. Homogenization problems for mixtures are mathematically rigorously considered in [51, 56]. The averaged equations that describe the propagation of small long-wave disturbances in a strongly inhomogeneous mixture of weakly viscous liquids and gases are substantiated. Such equations were previously constructed and justified for mixtures of solids. Under some additional restrictions on the determining parameters of the medium, the averaged equations are justified for mixtures of a random structure, and under these conditions the averaged equations turn out to be the same as for the periodic case. The equations of dynamics of composites of periodic or random structures composed of weakly compressible elastic components were considered in [49]. Under certain restrictions on the determining parameters (the ratio of the linear scale of inhomogeneities to the linear scale of disturbances and the ratio of the Lam´e coefficients), the averaged equations are justified. These equations are written explicitly and describe, in particular, the effect of reducing the speed of sound in composites composed of substantially heterogeneous materials. Let us dwell on the curious “paradox” described in [52]. The following cases are considered. In the first case, homogenization is used for media with voids. In the sec-

22

Linear and Nonlinear Waves in Microstructured Solids

ond case, homogenization procedure is employed for media with soft inclusions, and then in the homogenized expressions the characteristics of inclusions were assumed to be zero. The corresponding homogenized systems do not coincide.

in Layered 2 Waves Composites: Linear Problems One-dimensional propagation of linear waves in nonhomogeneous media is studied. Higher-order homogenization method is employed for spatially infinite domain. Then, the Bloch-Floquet method is used and the dispersion equation is derived analytically. A few of limiting cases are investigated. Two numerical example are given and the results are presented graphically in the form of dispersion curves and the wave attenuation coefficients for the composites of steel-aluminium and CE plasticsteel.

2.1

ONE-DIMENSIONAL (1D) DYNAMIC PROBLEM

Processes of propagation of waves in homogeneous and nonhomogeneous medium are qualitatively different. In composite materials the local reflection and refraction on the boundaries of the components separation implies the waves dispersion on the microlevel. The latter phenomenon can be described with a help of the homogenization method of a higher order, and hence reliable solution of the problem can be obtained for the long wave analysis. If the wave length is decreased and becomes compared with a size of internal structure, the pass and stop bands appear, and hence the composite material plays the role of a wave filter. The mentioned phenomenon can be described with a help of the piecewise homogeneous models, in particular, by employment of the Bloch-Floquet method [82, 176]. We consider the problem of elastic waves propagation in the layered composite consisting of the components Ω(1) and Ω(2) (Fig. 2.1). Let a longitudinal wave is propagated in the direction perpendicular to the layers plane and let the stresses depend on co-ordinate x. The governing equations take the following form E (a)

∂ 2 u(a) ∂ 2 u(a) = ρ (a) . 2 ∂x ∂t 2

(2.1)

Ideal contact on the boundaries of the components ∂ Ω is assumed, i.e. we take n o u(1) = u(2) , (2.2) ∂Ω

( E

(1) ∂ u

(1)

∂x

=E

) ∂x

(2) (2) ∂ u

.

(2.3)

∂Ω

23

24

Linear and Nonlinear Waves in Microstructured Solids

Figure 2.1 Layered composite.

The 1D problem (2.1)–(2.3) allows to find an exact dispersive equation. Therefore, it can be considered as an benchmark example for investigation of the area of applicability of the higher-order homogenization method. The practical advantage of the homogenization approach is displayed in the cases when the exact dispersion equations are not known (2D and 3D problems, nonlinear composites, etc.).

2.2

HIGHER-ORDER HOMOGENIZATION METHOD

We begin with the introduction of a small parameter η = l/L , where l stands for the periodicity cell size, and L describes the wave length. Let us introduce “slow” x and “fast” y = η −1 x variables, then ∂ /∂ x = ∂ /∂ x + η −1 ∂ /∂ y.

(2.4)

The being searched solution is presented in the form of the following series (a)

(a)

u(a) = u0 (x) + ηu1 (x, y) + η 2 u2 (x, y) + · · · , (a)

(2.5)

(a)

where ui (x, y) = ui (x, y + L), i = 1, 2, 3, .... Assuming that the components properties have the same order: E (2) /E (1) = O(η 0 ), ρ (2) /ρ (1) = O(η 0 ), we carry out the splitting of the boundary value problem (2.1)–(2.3) with regard to η. In result, one gets a sequence of the boundary value problems on a cell including the microscopic equations of motion: ! 2 u(a) 2 (a) 2 u(a) 2 u(a) ∂ ∂ ∂ i−1 i−2 (a) ∂ ui−2 (a) i +2 + =ρ , (2.6) E ∂ x2 ∂ x∂ y ∂ y2 ∂t 2 (a)

where u−1 = 0, as well as the microscopic conditions of an ideal contact n o (1) (2) ui = ui , ∂Ω

(2.7)

25

Waves in Layered Composites: Linear Problems (1)

( E

(1)

∂ ui−1 ∂ u(1) + i ∂x ∂y

(2)

! =E

(2)

∂ ui−1 ∂ u(2) + i ∂x ∂y

!)

.

(2.8)

∂Ω (a)

In the case of the space-infinite composite, the periodicity conditions for ui can be replaced by zeroth boundary conditions in the cell center and on the cell boundary (Fig. 2.2)

Figure 2.2 Cell of periodicity (with respect to co-ordinate y).

n o (2) ui = 0

y=0

,

n o (1) ui = 0

y=± L2

.

(2.9)

Algorithm of the homogenization procedure is as follows. A solution to i-th (a) boundary value problems (2.6)–(2.9) allows to determine the term ui . Knowing R (a) ui , we employ to the (i + 1)-th equation (2.6) the averaging operator l −1 Ω0 (·)dy (1)

(2)

along the cell area Ω0 = Ω0 + Ω0 . (a)

The terms ui+1 are cancelled based on boundary condition (2.8), which with a (a)

help of periodicity ui+1 in y gives E

(1)

Z

(1) Ω0

(1) (2) Z (2) (1) ∂ 2 ui+1 ∂ 2 ui+1 ∂ 2 ui ∂ 2 ui (2) + dy + E + dy = 0. ∂ x∂ y ∂ y2 ∂ x∂ y ∂ y2 (2) Ω0

(2.10)

26

Linear and Nonlinear Waves in Microstructured Solids

In result, the following homogenized equation of order η i−1 is obtained E (1)

Z

(1) (2) Z ∂ 2 ui−1 ∂ 2 u(1) ∂ 2 ui−1 ∂ 2 u(2) (2) i i + + dy + E dy = ∂ x2 ∂ x∂ y ∂ x2 ∂ x∂ y

(1)

(2)

Ω0

ρ (1)

Z (1)

Ω0

Ω0

(2) (1) Z ∂ 2 ui−1 ∂ 2 ui−1 (2) dy + ρ dy. ∂t 2 ∂t 2

(2.11)

(2)

Ω0

Unite equations (2.11) for i = 1...n, one obtains the macroscopic wave equation of order η n . Here we carry out the computations up to the value of n = 3. The exact analytical solutions on the cell are as follows for y > 0 ∂ u0 1 ∂ u0 (2) (1) u1 = A1 y , u1 = B1 y + C1 L , ∂x 2 ∂x # " ! ρ (2) E0 ∂ 2 u0 1 1 (2) 2 1 + 2A1 − A Ly , u2 = − y + 2 (2.12) 2 ρ0 E (2) 4 ∂ x2 " ! # 2 1 ρ (1) E0 1 1 (1) 2 2 ∂ u0 u2 = − 1 + 2B1 − y + B Ly + C L , 2 2 2 ρ0 E (1) 4 8 ∂ x2 ) # ( " ρ (2) E0 1 ∂ 3 u0 1 1 2 2 3 , 2 + 3A1 + (A1 − 2) A Ly + A L y y − = 2 3 6 ρ0 E (2) 4 24 ∂ x3 ( " # 1 ρ (1) E0 (1) u3 = y3 − 2 + 3B1 + (B1 − 2) 6 ρ0 E (1) ! ) 3 1 ρ (1) E0 1 1 2 2 3 ∂ u0 B2 +C1 −C1 Ly + B L y + C L , 3 3 4 ρ0 E (1) 24 48 ∂ x3 (2) u3

for y < 0 1 ∂ u0 ∂ u0 (2) (1) , u1 = B1 y − C1 L , u1 = A1 y ∂x 2 ∂x " ! # 1 ρ (2) E0 1 d 2 u0 (2) 2 u2 = − 1 + 2A1 − A Ly , y − 2 2 ρ0 E (2) 4 dx2 " ! # 2 1 ρ (1) E0 1 1 (1) 2 2 ∂ u0 u2 = − 1 + 2B1 − y − B2 Ly + C2 L , (1) 2 ρ0 E 4 8 ∂ x2

(2.13)

27

Waves in Layered Composites: Linear Problems

( " # ) 1 ρ (2) E0 1 1 ∂ 3 u0 3 2 2 = , 2 + 3A1 + (A1 − 2) y + A2 Ly + A3 L y (2) 6 ρ0 E 4 24 ∂ x3 # ( " ρ (1) E0 1 (1) y3 + 2 + 3B1 + (B1 − 2) u3 = 6 ρ0 E (1) ) ! 3 1 ρ (1) E0 1 1 2 3 ∂ u0 2 B L y − C L . B2 +C1 −C1 Ly + 3 3 4 ρ0 E (1) 24 48 ∂ x3 (2) u3

The coefficients Ai , Bi , Ci follow A1 = − 1 − c(2) E (2) − E (1) /D , B1 = c(2) E (2) − E (1) /D , C1 = −B1 , D = 1 − c(2) E (2) + c(2) E (1) , h nh i o A2 = − 1 − c(2) 1 − c(2) ρ (1) + 2c(2) ρ (2) E0 + ρ0 E (1) E (2) + 2 (2) (2) (1) c ρ E E0 / ρ0 E (2) D , h i B2 = c(2) E (1) c(2) ρ (2) − 2ρ (1) E0 − 2ρ0 E (1) + 2 E (2) 1 + 2c(2) ρ0 E (1) − 1 − c(2) ρ (1) E0 / ρ0 E (1) D , 2 n C2 = c(2) ρ0 E (1) + 1 − c(2) ρ (1) E (2) E0 − E (1) ρ0 E (2) + h i o c(2) ρ (2) + ρ (1) 1 − 2c(2) E0 / ρ0 E (1) D , 2 2 2 3 (2) (2) (1) (2) (2) ρ E E0 + 1 − c E ρ (1) E0 1 − c(2) − A3 = − c i n h i o ρ0 E (1) + 3E0 1 − c(2) c(2) ρ (2) + 1 − c(2) ρ (1) − ρ0 E (1) × o c(2) E (1) E (2) / ρ0 E (2) D2 , h i 2 (2) (2) (2) (1) (2) (2) (2) B3 = c E0 5c ρ + 3ρ 1 − 4c − 2cρ0 E 1 − 3c × 2 2 E (1) + E (1) E (2) ρ0 E (2) 1 − c(2) 1 + 3c(2) + 3 c(2) E0 × 3 io 2 h − 3 c(2) ρ0 E (1) + ρ (2) 1 − c(2) − ρ (1) 4 − 5c(2) 2 2 (1) (2) (2) (2) ρ E E0 1 − c 1 + c − 5 c(2) / ρ0 E (1) D2 , (2.14)

28

Linear and Nonlinear Waves in Microstructured Solids

2 n h io C3 = c(2) E (1) ρ0 E (2) 1 − 2c(2) − c(2) E0 2c(2) ρ (2) + 3ρ (1) 1 − 2c(2) − 2 + E (1) E (2) ρ0 E (2) 1 − c(2) + ρ (1) E0 1 − 6c(2) + 6 c(2) 3 2 c(2) ρ0 E (1) + ρ (1) E (2) E0 1 − c(2) 1 − 2c(2) / ρ0 E (1) D2 . In the reported formulas h i−1 E0 = c(2) /E (2) + 1 − c(2) /E (1)

(2.15)

stands for the effective elasticity modulus of the layered composite in the quasihomogeneous cases (for η = 0), ρ0 = 1 − c(2) ρ (1) + c(2) ρ (2) (2.16) is the averaged density, and c(2) = l2 /l = 2A/L is the volume fraction of the component Ω(2) , A = l2 /(2η) . Macroscopic wave equation of order η 2 takes the following form E0

∂ 2 u0 ∂ 4 u0 ∂ 2 u0 2 2 4 + η L E + O(η ) = ρ , 2 0 ∂ x2 ∂ x4 ∂t 2

(2.17)

where the coefficient 2 3 E (2) ρ (2) − E (1) ρ (1) E 2 2 0 1 (2) E2 = c 1 − c(2) 2 12 ρ 2 E (1) E (2)

(2.18)

0

can be interpreted as the effective elastic modulus of order η 2 . The second term on the left hand side of equation (2.17) exhibits the dispersion effect of the wave scattering on the microinhomogeneties of the composite. The coefficient E2 is equal to zero and the dispersion vanishes in the case of (a) homogeneous material (c(2) = 0, c(2) = 1) and (b) under equality of the acoustic impedance of the components (E (2) ρ (2) = E (1) ρ (1) ), where local reflections on the boundary of separation ∂ Ω are absent. Consider a harmonic wave u0 = U exp(iµx) exp(iωt)

(2.19)

with the amplitude U, frequency ω and the wave number µ = 2π/L . Substituting (2.19) into (2.17), the following dispersion relation is obtained 4 2 E2 2 2 2 η + O(η ) , (2.20) ω = ω0 1 − 4π E0

Waves in Layered Composites: Linear Problems

29

p where η = l/L = µl/(2π) , ω0 = µv0 is frequency and v0 = E0 /ρ0 stands for velocity in the quasi-homogeneous case. Phase v p and group vg velocities are governed by the following equations, respectively 2 ω 4 2 2 2 E2 2 + O(η ) , (2.21) = v0 1 − 4π η vp = µ E0 2 1 − 8π 2 η 2 E2 /E0 dω 2 v2g = + O(η 4 ). (2.22) = v20 dµ 1 − 4π 2 η 2 E2 /E0 Asymptotic solution (2.20)–(2.22) describes the long-wave approximation. Decreasing the wave length L (and increasing the frequency ω) implies decrease of the group velocity vg . The condition vg = 0 defines a bound of the first stop band. The upper frequency limit ωmax can be found based on equations (2.20), (2.22) 2 ωmax =

hEi20 + O(η 4 ). 4l 2 hEi2 hρi

(2.23)

It should be noticed that the given homogenization procedure is developed for the spatially infinite domain. It allowed for defining the dispersive relations as the selfcharacteristic of the composite material independently on the kind of the boundary conditions on the macrolevel. If one considers composite structure of the finite size then the homogenized solution must be supplemented by the macroscopic boundary conditions. The formal transition of the results obtained for the infinite domain into the case of a composite of finite size can produce errors in the boundary conditions on the macro level.

2.3

THE BLOCH-FLOQUET METHOD AND EXACT DISPERSION EQUATION

A solution suitable for short waves can be found using the Bloch-Floquet approach [82, 176]. Owing to the given method, let us write the ansatz governing propagation of the harmonic wave in the piece-wise medium u(a) = F (a) (x) exp(iµx) exp(iωt),

(2.24)

where F (a) (x) is periodic function taking into account of the material microstructure, F (a) (x) = F (a) (x + l). Periodicity of F (a) (x) implies u(a) (x + l) = u(a) (x) exp(iµl). Substituting ansatz (2.24) into the wave equation (2.1) yields h i h i (a) (a) F (a) (x) = F1 exp(i µ (a) − µ x) + F2 exp(−i µ (a) + µ x), where: µ (a) = ω

p ρ (a) /E (a) stands for the wave complex number.

(2.25)

(2.26)

30

Linear and Nonlinear Waves in Microstructured Solids

Figure 2.3 Periodicity cell (with respect to co-ordinate x). (a)

(a)

In order to define the coefficients F1 , F2 , we need to employ the conditions (2.2), (2.3). Let us consider the cell of periodicity shown in Fig. 2.3. On the boundary x = 0 we have ) ( n o (2) (1) (2) ∂ u (1) (2) (1) ∂ u =E (2.27) u =u E . , ∂x ∂x x=0 x=0

Displacements and stresses on the boundaries x = −l1 can be linked with a help of equation (2.25) in the following way u(2) = u(1) exp(iµl), x=l2 x=−l1 (2.28) (2) (1) (2) ∂ u (1) ∂ u E =E exp(iµl). ∂x ∂x x=l2

x=−l1

Substituting ansatz (2.24), (2.26) into boundary conditions (2.27), (2.28), the following four linear algebraic equations are obtained (1)

(1)

(2)

(2)

F1 + F2 − F1 − F2

= 0,

(1) (1) (2) (2) F1 z1 − F2 z1 − F1 z2 + F2 z2 = 0, h i h i (1) (1) F1 exp −i(µ (1) − µ)l1 + F2 exp i(µ (1) + µ)l1 −

h i h i (2) (2) F1 exp i(µ (2) − µ)l2 − F2 exp −i(µ (2) + µ)l2 = 0, h i h i (1) (1) F1 z1 exp −i(µ (1) − µ)l1 − F2 z1 exp i(µ (1) + µ)l1 − i h i h (2) (2) F1 z2 exp i(µ (2) − µ)l2 + F2 z2 exp −i(µ (2) + µ)l2 = 0,

(2.29)

Waves in Layered Composites: Linear Problems

31

p where z(a) = E (a) ρ (a) stands for the components impedance. System (2.29) has non-trivial solution only if the determinant of the matrix composed of its coefficients is equal to zero. The given condition allows to write the dispersion equation in the explicit analytical form cos(µl) = cos(µ (1) l1 ) cos(µ (2) l2 )− ! 1 z(1) z(2) + sin(µ (1) l1 ) sin(µ (2) l2 ). 2 z(2) z(1)

(2.30)

Exact equation (2.30) allows for investigation of numerous simplified cases. The limiting transitions l2 → 0, ρ (2) l2 → m, ρ (1) → 0, E (1) /l1 → C yields the known dispersive relations for the oscillating chain of masses m, coupled by springs of stiffness C mω 2 . (2.31) cos(µl) = 1 − 2C Employing l2 → 0, ρ (2) l2 → m, ρ (1) = ρ, E (1) = E, yields the dispersive equation of the rod with the attached masses longitudinal vibrations r r ρ mω ρ cos(µl) = cos ωl − √ sin ωl . (2.32) E 2 Eρ E In the case of long waves one may consider the frequency ω in the η series, where η = l/L = µl/(2π) → 0. The coefficients of the latter series are computed from equation (2.30), and first two of them coincide with the first two coefficients of the asymptotic series (2.20), obtained with the help of homogenization method. Let us consider the material to be made up of layers of equal travel time. Such a material is known as the Goupillaud medium in geophysics [189]. In this case T (1) = T (2) = T,

(2.33)

p

where T (a) = ρ (a) /E (a) la . Condition (2.33) provided that (2.30) is solved exactly q 2 2 2z(1) z(2) cos(µl) + (z(1) ) + (z(2) ) 1 . ω = ± arccos T z(1) + z(2)

(2.34)

In the case when the components of the composite have the high contrast parameters, z(2) 0) and anomalous (dω/dµ < 0) dispersion has been investigated in reference [272]. In mechanics of materials the physically important is one mode regime where for a given harmonic (2.24) there is preserved unique dependence between ω and µ [60,272,408,409]. The corresponding branches of the spectrum are denoted by solid curves in Fig. 2.4, whereas the remaining branches are marked by dashed curves. The branches choice has been validated through an asymptotic transition from solution of the piece-wise homogenous medium to the solution of the corresponding homogenous medium: equality of the components impedance (z(2) /z(1) → 1) implies decrease of the stop bands and solid branches tend to coincide with a straight line (ω → ω0 = µv0 ). The coefficient µI is associated with symmetric pair of positive and negative roots (Fig. 2.5). Positive values µI (solid curves) describe the attenuation effect. Negative values µI (dashed curves) should correspond to the exponential increase of a signal which has no physical interpretation in the case of the considered conservative system. Solution behavior can be described in the following way. For low frequencies ω the dispersion curve is close to the straight line, ω ≈ ω0 , phase velocity v p = ω/µ and group velocity v p = dω/dµ are close to each other and do not depend on ω, v p ≈ vg ≈ v0 . The so considered case is referred to as quasi-homogenous. Increase of frequency, angle of inclination of the dispersive curve is decreased. Both phase and group velocities are decreased though the group velocity decreases more fast v p > vg . On the boundary of the stop band the group velocity tends to zero vg = 0, and the composite exhibits a standing wave. In the successive pass bands the group velocity changes from zero on the boundaries up to maximum values in the center.

34

2.4

Linear and Nonlinear Waves in Microstructured Solids

NUMERICAL RESULTS

As the first case we consider low contrast composite consisting of aluminium (E (1) = 70 GPa, ρ (1) = 2700kg/m3 ) and steel (E (2) = 210 GPa, ρ (2) = 7800kg/m3 ). Dispersion curves and the wave attenuation coefficient are reported in Fig. 2.6 and Fig. 2.7, respectively. In order to decrease the figures size, the spectrum branches are shown in interval 0 ≤ µR l ≤ π. Fig. 2.8 presents the dispersion curve in the first pass band (acoustic branch) found with a help of homogenization method (formula (2.20)), which is compared with the numerical results of solution to the dispersion equation (2.30) (we have fixed c(2) = 0.3). The employed method of homogenization allows to account of the dispersion effect through the high accuracy only for low values of the frequency ω. The general structure of the pass and stop bands versus the volume fraction c(2) is shown in Fig. 2.9.

Figure 2.6 Dispersion curves of composite “steel-aluminium”.

As the second example we consider the high-contrast composite composed of carbon-epoxide (CE) plastic (E (1) = 8.96 GPa, ρ (1) = 1600 kg/m3 ) and steel (E (2) = 210 GPa, ρ (2) = 7800 kg/m3 ). Dispersion curves are reported in Fig. 2.10, whereas the attenuation coefficient is shown in Fig. 2.11. The results obtained for the acoustic branch using the homogenization method coincide well with the exact solution (Fig. 2.12). The computations have been carried out for fixed c(2) = 0.5. Structure of the pass and stop bands is shown in Fig. 2.13.

Waves in Layered Composites: Linear Problems

Figure 2.7 Wave attenuation coefficient of composite “steel-aluminium”.

Figure 2.8 Acoustic branched of composite “steel-aluminium”.

35

36

Linear and Nonlinear Waves in Microstructured Solids

Figure 2.9 Pass and stop bands of composite “steel-aluminium”.

Figure 2.10 Dispersion curves of composite “CE plastic-steel”.

Waves in Layered Composites: Linear Problems

Figure 2.11 Wave attenuation coefficient of composite “CE plastic-steel”.

Figure 2.12 Acoustic branch of composite “CE plastic-steel”.

37

38

Linear and Nonlinear Waves in Microstructured Solids

Figure 2.13 Pass and stop bands of composite “CE plastic-steel”.

in Fiber 3 Waves Composites: Linear Problems Two-dimensional linear elastic waves propagation in the fiber composite material are investigated. Higher-order homogenization method is employed. The obtained solutions realibility is numerically validated. Effective moduli in the case of strong fibers interaction are obtained. Then the Bloch-Floquet method is used as well as the Fourier series approach to get a solution to the studied problem. Numerical results allowed to estimate dispersive curves and acoustic branches of the composite “nickel-aluminium” and “carbon-epoxide plastic”. Moreover, shear wave dispersion in cylindrically structured cancellous viscoelastic bones is analyzed.

3.1

TWO-DIMENSIONAL (2D) DYNAMIC PROBLEM

If displacements and stresses in composite material depend on two space coordinates x1 , x2 , then the problem of propagation of elastic waves is splitted into two independent problems with regard to plane and antiplane deformation. In what follows we consider the antiplane problem which deals with a shear wave propagating in plane x1 x2 in the fiber composite with the cylindrical inclusions (see Fig. 3.1).

Figure 3.1 Fiber composite material.

39

40

Linear and Nonlinear Waves in Microstructured Solids

The governing wave equation takes the following form ∇x · (G∇x u) = ρ

∂ 2u , ∂t 2

(3.1)

where u is the displacement in x3 direction and ∇x = e1 ∂ /∂ x1 + e2 ∂ /∂ x2 . Since we have the nonhomogeneous medium, the shear modulus G and density ρ are discontinuous functions of the co-ordinates G(x) = G(a) ,

ρ(x) = ρ (a) (x) for x ∈ Ω(a) ,

a = 1, 2.

(3.2)

Equation (3.1) can be presented in equivalent form G(a) ∇2xx u(a) = ρ (a)

∂ 2 u(a) , ∂t 2

(3.3)

where ∇2xx = ∂ 2 /∂ x12 + ∂ /∂ x22 . On the boundary ∂ Ω, separating the composite component, we account of the following ideal contact conditions ( ) n o (1) (2) (1) (2) (1) ∂ u (2) ∂ u u =u G =G (3.4) , . ∂n ∂n ∂Ω ∂Ω

It should be emphasized that the boundary value problem (3.1)–(3.4) allows for various physical interpretations. Beside considered here the example of elastic shear wave, considered problems describe processes of propagation of the electromagnetic waves in composites with dielectric inclusions.

3.2

METHOD OF HIGHER-ORDER HOMOGENIZATION

In order to construct a long-wave approximation we employ the asymptotic method of homogenization, see Sections 1.2, 2.2. The recurrent system of boundary value problems on a cell takes the following form: (a) ∂ 2 ui−2 (a) (a) (a) = ρ (a) G(a) ∇2xx ui−2 + 2∇2xy ui−1 + ∇2yy ui , ∂t 2 n o (1) (2) ui = ui ,

(3.5) (3.6)

∂Ω

(1)

( (1)

G

where i = 1, 2, 3, ..., ∂ /∂ y22 .

∂ ui−1 ∂ u(1) + i ∂n ∂m (a) u−1

= 0,

∇2xy

(2)

! (2)

=G

∂ ui−1 ∂ u(2) + i ∂n ∂m

= ∂ 2 /(∂ x1 ∂ y1 )

!)

+ ∂ 2 /(∂ x2 ∂ y2 ) ,

,

(3.7)

∂Ω

∇2yy = ∂ 2 /∂ y21 +

41

Waves in Fiber Composites: Linear Problems

In the case of spatially infinite composite we change the periodicity conditions by zeroth boundary conditions in the cell center and its external boundary ∂ Ω0 n o n o (2) (1) (3.8) ui = 0 x = 0 , ui = 0 . ∂ Ω0

y=0 (a)

After defining the ui term from the i-th boundary value problem (3.5)–(3.8) we employ the averaging operator S0−1

ZZ

(·)dS,

(3.9)

Ω0

where dS = dy1 dy2 . (a) The terms ui+1 are removed with the help of Gauss-Ostrogradsky’s theorem after integration with regard to the cell area ZZ ZZ (1) (1) (2) (2) G(1) ∇2xy ui + ∇2yy ui+1 dS + G(2) ∇2xy ui + ∇2yy ui+1 dS = 0. (3.10) (1)

(2)

Ω0

Ω0

The homogenized equation of motion of η i−1 order has the following form ZZ ZZ (1) (1) (2) (2) G(1) ∇2xx ui−1 + ∇2xy ui dS + G(2) ∇2xx ui−1 + ∇2xy ui dS = (1)

(2)

Ω0

ρ

(1)

ZZ (1)

Ω0

Ω0 (1)

(3.11)

(2)

ZZ 2 ∂ 2 ui−1 ∂ ui−1 (2) dS + ρ dS. 2 ∂t ∂t 2 (2)

Ω0

Adding the equations (3.11) for i = 1, ..., n, one gets the macroscopic wave equation of order η n . In order to solve boundary value problems on cell (3.5)–(3.8), one may employ various approaches. As a rule, the largest computational problems appear in the case of strong interaction of the inclusions when significant oscillations on the microlevel are exhibited. Let us consider the asymptotic solution using nondimensional width of the clearance between the neighboring fibers ν = 2(1 − A/L ) (Fig. 3.2). Let ν > 1. In zeroth approximation O(ν 0 ) for the zones dΩ1 , dΩ2 the following estimations hold (1)

(1)

∂ 2 ui ∂ 2 ui >> ∂ y21 ∂ y22 (1)

for y ∈ dΩ1 , (3.12)

(1)

∂ 2 ui ∂ 2 ui 0 ∂ u0 1 ∂ u0 (2) (1) u1 = A1,s ys , u1 = B1,s ys + C1,s L , ∂ xs 2 ∂ xs " # ! 1 ρ (2) G0 1 ∂ 2 u0 (2) 2 u2 = − 1 + 2A1,s − y + A Ly , s 2,s s 2 ρ0 G(2) 4 ∂ xs2 " ! # 2 1 1 ρ (1) G0 1 (1) 2 2 ∂ u0 u2 = − 1 + 2B1,s − ys + B2,s Lys + C2,s L , (1) 2 ρ0 G 4 8 ∂ xs2

43

Waves in Fiber Composites: Linear Problems

( " # 1 ρ (2) G0 = 2 + 3A1,s + (A1,s − 2) y3 − 6 ρ0 G(2) s 3 1 ∂ u0 1 A2,s Ly2s + A3,s L2 ys , 4 24 ∂ xs3 ( " # 1 ρ (1) G0 (1) u3 = 2 + 3B1,s + (B1,s − 2) y3 − 6 ρ0 G(1) s ! ρ (1) G0 1 Ly2s + B2,s +C1,s −C1,s 4 ρ0 G(1) 3 1 ∂ u0 1 B3,s L2 ys + C3,s L3 , 24 48 ∂ xs3 (2) u3

(3.14)

and for ys < 0 1 ∂ u0 ∂ u0 (1) , u1 = B1,s ys − C1,s L , = A1,s ys ∂ xs 2 ∂ xs " # ! 1 ρ (2) G0 ∂ 2 u0 1 (2) 2 u2 = − , 1 + 2A1,s − A Ly y − s 2,s s 2 ρ0 G(2) 4 ∂ xs2 # ! " 2 ρ (1) G0 1 1 1 (1) 2 ∂ u0 2 , 1 + 2B1,s − B Ly + C L y − u2 = − s 2,s 2,s s 2 ρ0 G(1) 4 8 ∂ xs2

(2) u1

(3.15)

( " # 1 ρ (2) G0 = 2 + 3A1,s + (A1,s − 2) y3 + 6 ρ0 G(2) s 3 1 1 ∂ u0 , A2,s Ly2s + A3,s L2 ys 4 24 ∂ xs3 # ( " ρ (1) G0 1 (1) 2 + 3B1,s + (B1,s − 2) y3 + u3 = 6 ρ0 G(1) s ! ) 3 ρ (1) G0 1 1 1 2 2 3 ∂ u0 B2,s +C1,s −C1,s Lys + B3,s L ys − C3,s L . (1) 4 ρ0 G 24 48 ∂ xs3 (2) u3

Here G0 stands for the effective shear modulus in thequasi-homogeneous case (it is yielded by equation (3.11) for i = 1); ρ0 = 1 − c(2) ρ (1) + c(2) ρ (2) stands for the averaged density, whereas c(2) = πA2 /L2 stands for the volume fraction of fibers, (2) (2) 0 ≤ c(2) ≤ cmax , cmax = π/4 = 0.7853...

44

Linear and Nonlinear Waves in Microstructured Solids

The coefficients Ai,s , Bi,s , Ci,s follow A1,s = −(1 − χs ) G(2) − G(1) /Ds ,

B1,s = χs G(2) − G(1) /Ds ,

C1,s = −B1,s , Ds = (1 − χs ) G(2) + χs G(1) , h nh i o A2,s = − (1 − χs ) (1 − χs ) ρ (1) + 2χs ρ (2) G0 + ρ0 G(1) G(2) + i χs2 ρ (2) G(1) G0 / ρ0 G(2) Ds , n h i B2,s = χs G(1) χs ρ (2) − 2ρ (1) G0 − 2ρ0 G(1) + h io G(2) (1 + 2χs ) ρ0 G(1) − 1 − χs2 ρ (1) G0 / ρ0 G(1) Ds , 2 n C2,s = χs ρ0 G(1) + (1 − χs ) ρ (1) G(2) G0 − G(1) ρ0 G(2) + h i o χs ρ (2) + ρ (1) (1 − 2χs ) G0 / ρ0 G(1) Ds , 2 2 h A3,s = − χs3 ρ (2) G(1) G0 + (1 − χs ) G(2) ρ (1) G0 (1 − χs )2 − i n h i o ρ0 G(1) + 3G0 (1 − χs ) χs ρ (2) + (1 − χs )ρ (1) − ρ0 G(1) × o χs G(1) G(2) / ρ0 G(2) D2s , hn h i o B3,s = χs2 G0 5χs ρ (2) + 3ρ (1) (1 − 4χs ) − 2χs ρ0 G(2) (1 − 3χs ) × 2 n G(1) + G(1) G(2) ρ0 G(2) (1 − χs ) (1 + 3χs ) + 3χs2 G0 × h io 3 ρ (2) (1 − χs ) − ρ (1) (4 − 5χs ) − 3χs2 ρ0 G(1) +

(3.16)

2 ρ (1) G(2) G0 (1 − χs ) 1 + χs − 5χs2 / ρ0 G(1) D2s , 2 n h io C3,s = χs G(1) ρ0 G(2) (1 − 2χs ) − χs G0 2χs ρ (2) + 3ρ (1) (1 − 2χs ) − h i G(1) G(2) ρ0 G(2) (1 − χs ) + ρ (1) G0 1 − 6χs + 6χs2 + 3 2 (1) (1) (2) χs ρ0 G +ρ G G0 (1 − χs ) (1 − 2χs ) / ρ0 G(1) D2s , r r (2) (2) 2 (2) 2 where χ1 = c /cmax 1 − y2 /A , χ2 = c(2) /cmax 1 − y21 /A2 . The macroscopic wave equation of order η 2 takes the following form G0 ∇2xx u0 + η 2 L2 G2 ∇41 u0 + O(η 4 ) = ρ0

∂ 2 u0 , ∂t 2

(3.17)

Waves in Fiber Composites: Linear Problems

45

where ∇41 = ∂ 4 /∂ x14 + ∂ /∂ x24 , and the coefficient G2 presents the effective modulus of order η 2 (it is computed from equation (3.11) for i = 3). In the order to check reliability of the obtained solution, we consider numerical results for the nondimensional effective shear modulus λ0 = G0 /G(1) . Fig. 3.3 presents λ0 in the case of strong interaction of the neighboring fibers (λ (2) = G(2) /G(1) → ∞, (2) c(2) → cmax ). Owing to the mathematical analogy between the problems of conductivity and longitudinal shear, the obtained solution (solid curves) are compared with those obtained through the asymptotic formula (dashed curves) which have been obtained for two highly conducted cylinders approaching a contact [358]. The estimations (3.12) are valid only in the case of a high contrast composite material with large volume fraction of inclusions. Yet, the obtained solution exhibits high accuracy for arbitrary values of the parameters 1 ≤ λ (2) < ∞ and 0 ≤ c(2) ≤ (2) cmax . This statement is illustrated in Fig. 3.4, where the results obtained for λ0 (solid curves) are compared with the results reported in [358] (circles).

Figure 3.3 Effective modulus in the case of strong interaction of the neighboring fibers; a) (2)

λ (2) → ∞, c(2) = 0.784, b) λ (2) = ∞, c(2) → cmax .

Consider the following harmonic wave u0 = U exp(iµ · x) exp(iωt),

(3.18)

where U is the amplitude, ω stands for the frequency, µ = µ1 e1 + µ2 e2 is wave vector, µ ≡ |µ| = 2π/L stands for the wave number. Projections of the vector µ on the axis of co-ordinates are as follows: µ 1 = µ cos φ , µ 2 = µ sin φ , where φ stands for the angle between the axis x1 and direction of the wave propagation, φ = (e1 , µ). Substituting of ansatz (3.18) into equation (3.17), the following dispersion relation is obtained G2 2 η + O(η 4 ) , (3.19) ω 2 = ω02 1 − 4π 2 sin4 ϕ + cos4 ϕ G0

46

Linear and Nonlinear Waves in Microstructured Solids

Figure 3.4 Effective modulus for different values of the fibers stiffness; a) λ (2) = ∞, b) λ (2) = 5, 10, 20, 50.

p where η = l/L = µl/(2π) , ω0 = µv0 is the frequency and v0 = G0 /ρ0 stands for the velocity in the quasi-homogenous case. Phase v p and group vg wave velocities are governed by the following equations: v2p v2g

=

2

=

ω µ

2

dω dµ

G2 2 4 2 4 4 η + O(η ) , 1 − 4π sin φ + cos φ G0

(3.20)

2 1 − 8π 2 η 2 sin4 φ + cos4 φ G2 /G0 + O(η 4 ). 1 − 4π 2 η 2 sin4 φ + cos4 φ G2 /G0

(3.21)

= v20

= v20

Asymptotic solution (3.19)–(3.21) is obtained for the case when the wave length is essentially larger than the characteristic size of internal composite structure. The upper frequency limit ωmax , which corresponds to the beginning of the stop band, is defined from the condition vg = 0: 2 ωmax =

G20 + O(η 4 ). 4l 2 G2 ρ0 sin4 φ + cos4 φ

(3.22)

In the quasi-homogeneous case the considered fiber composite is transversallyisotropic; the solution for G0 , v0 , ω0 does not depend on the direction of wave propagation in plane x1 x2 . The higher-order approximations allow to detect the anisotropic effects of the problem. Namely, beginning with the terms of order η 2 , the relations (3.19)–(3.21) depend on direction φ of the wave vector.

3.3

THE BLOCH-FLOQUET METHOD AND SOLUTION BASED ON FOURIER SERIES

Owing to the Bloch-Floquet method, a solution to the wave equation (3.1) is searched in the following form u = F(x) exp(iµ · x) exp(iωt), (3.23)

Waves in Fiber Composites: Linear Problems

47

where F(x) is periodic functions of co-ordinates, F(x) = F(x + l p ), l p = p1 l1 + p2 l2 , p1 , p2 = 0, ±1, ±2, ..., l1 , l2 are translations vectors of the square lattice. We present the function F(x) and properties of components G(x), ρ(x) in the form of Fourier series ∞ ∞ 2π F(x) = ∑ ∑ An1 n2 exp i (n1 x1 + n2 x2 ) , l n1 =−∞ n2 =−∞ ∞ ∞ 2π G(x) = ∑ ∑ Bn1 n2 exp i (n1 x1 + n2 x2 ) , (3.24) l n1 =−∞ n2 =−∞ ∞ ∞ 2π ρ(x) = ∑ ∑ Cn1 n2 exp i (n1 x1 + n2 x2 ) , l n1 =−∞ n2 =−∞ where the coefficients Bn1 n2 , Cn1 n2 are defined in the following way ZZ 2π 1 G(x) exp −i (n1 x1 + n2 x2 ) dS, Bn1 n2 = S0 l Ω0 ZZ 1 2π Cn1 n2 = ρ(x) exp −i (n1 x1 + n2 x2 ) dS, S0 l

(3.25)

Ω0

RR

and the operator Ω0 (·)dS denotes integration along the cell area Ω0 , dS = dx1 dx2 , S0 = l 2 stands for the cell area. Substituting relations (3.23), (3.24) into equation (3.1) and comparing the coefficients standing by the terms exp i2πl −1 ( j1 x1 + j2 x2 ) , j1 , j2 = 0, ±1, ±2, ..., we obtain the infinite system of linear algebraic equations for unknowns An1 n2 ∞ ∞ 2π 2π A B n + µ j + µ j −n , 1 1 1 1 + ∑ ∑ n1 n2 j1 −n1 l l n1 =−∞ n2 =−∞ 2 2 (3.26) 2π 2π 2 n2 + µ2 j2 + µ2 −C j1 −n1 , ω = 0. l l j2 −n2 The condition for existence of solution to the system (3.26) is defined by equating to zero the determinant of the matrix composed of their coefficients. It gives the dispersive relation for ω and µ. It should be emphasized that the given method does not employ boundary conditions (3.4) in the explicit form. Condition of ideal contact between fibers and matrix are “hidden” in equation (3.1) and in development (3.24) for F(x), where the fields of displacements and stresses are implicitly treated as continuous. In the case of the numerical studies reported below, the dispersive relations are computed on a basis of truncation of system (3.26) assuming − jmax ≤ j1 , j2 ≤ jmax . The number of employed equations is equal to (2 jmax + 1)2 . The introduced truncation has physical interpretation: we neglect high frequencies. In order to illustrate the effect of wave filtering, let us split the problem (3.23) into real µ R and imaginary part µ I of the vector µ = µ R + iµ I u = F(x) exp(−µ I · x) exp(iµ R · x) exp(iωt).

(3.27)

48

Linear and Nonlinear Waves in Microstructured Solids

The imaginary part µI ≡ |µ I | of the wave number presents the attenuation coefficient. The values µI = 0 correspond to pass band, whereas µI 6= 0 correspond to stop band. q Boundaries of the pass and stop bands are defined through condition

µl = πn/ sin4 φ + cos4 φ , n = 1, 2, 3, .... The corresponding length of waves are q defined by the formula L = (2l/n ) sin4 φ + cos4 φ .

3.4

NUMERICAL RESULTS

In order to compare solutions obtained with a help of the Fourier series with result obtained by other authors, we consider the non-homogeneous material composed of the matrix with properties G(1) = 1, ρ (1) = 1 and with voids, G(2) = 0, ρ (2) = 0, A/L = 0.4, c(2) ≈ 0.503.

Figure 3.5 Dispersive curves of composite with voids.

Dispersive curves are shown in Fig. 3.5. The dashed lines correspond to computations for jmax = 1, whereas the solid lines correspond to jmax = 2; circles refer to the results reported in work [376] and obtained by the Rayleigh method. The dispersive diagram is composed of two parts separated by the vertical dashed line. The first part corresponds to the orthogonal (φ = 0), and left part corresponds to the diagonal (φ = π/4 ) direction of the wave propagation. In the quasi-homogenous case (ω → 0) the solution is isotropic and does not depend on the angle φ . However, with increase of the frequency ω the composite exhibits anisotropic properties. Brown color refers to the full stop band, where the signal propagation is not possible in any of directions. Increase of jmax increases accuracy of the numerical results. As an example of the low-contrast composite we consider material with aluminium matrix (G(1) = 27.9

Waves in Fiber Composites: Linear Problems

49

Figure 3.6 Dispersive curves of the composite “nickel-aluminium”.

GPa, ρ (1) = 2700 kg/m3 ) and nickel fibers (G(2) = 75.4 GPa, ρ (2) = 8936 kg/m3 , c(2) = 0.35). The related dispersive curves are shown in Fig. 3.6. The results obtained for jmax = 1 (dashed curves) and for jmax = 2 (solid curves) are close to each other which confirm the fast convergence of the solution. As it follows from computation of the acoustic branch of spectrum (Fig. 3.7), the homogenization method allows to account of the dispersion effect, though the good accuracy is achieved only on the interval of low frequencies.

Figure 3.7 Acoustic branch of the composite “nickel-aluminium”, φ = 0.

In the case of high-contrast composite (epoxy matrix with G(1) = 1.53 GPa, ρ (1) = 1250 kg/m3 and carbon fibers with G(2) = 86 GPa, ρ (2) = 1800 kg/m3 ,

50

Linear and Nonlinear Waves in Microstructured Solids

Figure 3.8 Acoustic branch of the carbon-epoxide plastic, φ = 0.

c(2) = 0.5), the solution based on the Fourier series converges more slowly (Fig. 3.8). The homogenization q method yields qualitatively correct results up to the first stop band (for µR l = π/ sin4 φ + cos4 φ we get vg ≈ 0).

3.5

SHEAR WAVES DISPERSION IN CYLINDRICALLY STRUCTURED CANCELLOUS VISCOELASTIC BONES

Animal and human bones are heterogeneous materials with a complicated hierarchical structure. Bone tissues occur in the two main forms: as a dense solid (cortical or compact bone) and as a porous media filled by a viscous marrow (trabecular or cancellous bone) [219, 458] (Fig. 3.9). The basic mechanical discrepancy between these two types consists in their relative densities. Both types can be found in the bones of the body. A classical example of the macroscopic bone structure can be given by the long bones (e.g., humerus, femur, and tibia). They include an outer shell of the dense cortical tissue surrounding an inner core of a porous cancellous tissue. The microstructure of cancellous bones is often described by two- or three-dimensional mesh of interconnected rods and plates [180]. The microstructure of cancellous bones is often described by two- or threedimensional theory of viscoelasticity [432]. Lakes [215, 268] used nonlocal theory of elasticity for dynamical study of couple stress effects in human compact bone. Cortical bone can be also modeled as a composite material with hierarchical structure [185]. Williams and Lewis [458] modeled the structured of a 2D section of trabecular bone using the plane strain FEMs to predict transversally isotropic elastic constant. An investigation has been made of the source and magnitude of anisotropic material properties of cancellous bone in the proximal epiphysis of the human tibia. Results are reported for stiffness measurements made in three orthogonal directions on 21 cubes of cancellous bone before testing to failure along one of the three principal axes. The structure is approximately transversely isotropic. Strength and stiff-

Waves in Fiber Composites: Linear Problems

51

Figure 3.9 Scanning micrograph of a cylindrically structured cancellous bone [458] [by courtesy of the ASME].

ness are linear with area fraction for loading along the isotropic axis. Strength is proportional to stiffness for all directions. A FEM is proposed, based on experimental observations, which enables one to predict the elastic constants of cylindrically structured cancellous bone in the tibia from morphological measurements in the transverse plane. In order to take into account the influence of bone marrow, Kasra and Grynpas [233] performed suitable numerical calculation using FEM. Many authors applied the homogenization theory to investigation of mechanical behaviour of the structures modeling trabecular bones [210]. Parnell and Grimal [352] investigate the influence of mesoscale porosity on the induced anisotropy of the material using asymptotic homogenization and new solution of the cell problem. Despite the obvious simplicity, such idealized models may provide a satisfactory agreement between theoretical predictions and experimental results for the mechanical properties of real bones. Here we deal with a two-dimensional model of cylindrically structured cancellous bones. A challenging problem consists in the detection of the bone structure using noninvasive measurements. The inverse homogenization approach (“dehomogenization procedure”) [122] can help to derive information about the microgeometry of the bone tissue from the values of effective moduli. Another possibility is to extract this information from a dynamic response of the bone, measuring velocity and attenuation of ultrasonic waves of different frequencies. Acoustic waves propagating through cancellous bones undergo dispersion and damping. There are two different physical effects influencing on the dynamic properties of the bone: (i) transmission of mechanical energy to heat due to the viscosity of the marrow (viscoelastic damping and dispersion) [215] and (ii) successive reflections and refractions of local waves at the trabecula-marrow interfaces (Bloch dispersion) [98]. From the theoretical standpoint, both effects are realized simultaneously. However, their intensities are very frequency dependent. For many real materials the effects of viscoelastic damping and Bloch dispersion are observed in a rather distant frequency ranges. In such a case they can be analyzed separately. We study transverse antiplane shear waves propagating in the (x1 , x2 ) plane

52

Linear and Nonlinear Waves in Microstructured Solids

Figure 3.10 Cancellous structure under consideration

through a regular cancellous structure consisting of a spatially infinite elastic matrix (trabeculae) Ω(1) and viscous inclusions (marrow) Ω(2) (Fig. 3.10). The governing two-dimensional wave equation is: ∇x · (G∇x w) = ρ

∂ 2u , ∂t 2

(3.28)

where G is the complex shear modulus, ρ is the mass density, u is the longitudinal displacement (in the x3 direction), ∇x = e1 ∂ /∂ x1 + e2 ∂ /∂ x2 , e1 , e2 are the unit Cartesian vectors. Due to the heterogeneity of the medium the physical properties G and ρ are represented by piece-wise continuous functions of co-ordinates: ρG(x) = G(a) (x),

(x) = ρ (a) (x)

f or

x ∈ Ω(a) ,

x = x1 e1 + x2 e2 .

(3.29)

Here and in the sequel the superscript (a) denotes different components of the structure, a = 1, 2. In Eq. (3.29), G(1) is the real shear modulus of the elastic matrix, G(2) = iων (2) , where ω is the frequency of a harmonic wave, ν (2) is the viscosity of the marrow. Because Eq. (3.28) contains delta functions, below we deal with the generalized solution of this equation [275]. Equation (3.28) can be written in the equivalent form: G(a) ∇2xx u(a) = ρ (a) n o u(1) = u(2)

∂Ω

( ,

∂ 2 u(a) , ∂t 2

(1) (1) ∂ u

G

∂n

(3.30) ) ∂n

(2) (2) ∂ u

=G

,

(3.31)

∂Ω

where ∇2xx = ∂ 2 /∂ x12 + ∂ /∂ x22 and ∂ /∂ n is the normal derivative to the contour ∂ Ω.

53

Waves in Fiber Composites: Linear Problems

From the physical standpoint, Eq. (3.31) mean the perfect bonding conditions at the trabeculae-marrow interface ∂ Ω. We start with the case, when the wavelength L is essentially larger than the internal size l of the cancellous structure, l 0 and E2 > 0 (hard nonlinearity). The third term in equation (4.22) describes the dispersion effect caused by energy dissipation on the medium nonhomogenuities. The coefficient E3 is equal to zero and dispersion vanishes: (i) in the case of homogeneous material (c(1) = 1, c(2) = 0 or c(1) = 0, c(2) = 1) and (ii) in the case of equality of the acoustic impedances of the components (z(1) = z(2) ), when local reflections of the signal on the separation boundary ∂ Ω are absent (it follows from formulas (4.25), E3 ≥ 0). Therefore, occurence of microstructure implies negative (normal) dispersion which yields decrease of the phase velocity under increase of the frequency. The given conclusion holds only in frame of the long-wave approximation governed by equation (4.22). For the high frequencies, when the wave length is comparable with the size of the periodicity cell, the nonhomogeneous materials may exhibit either normal or anomalous dispersion. It should be mentioned that the homogenized model (4.22) is obtained for the case of spatially infinite medium. If one considers structure of the finite size, then solutions depend on the boundary conditions defined on the macrolevel. The mentioned

71

Longitudinal Waves in Layered Composites

dependence will introduce occurrence of the additional correcting terms in formulas (4.23)–(4.25). Therefore, the formal transition of the results obtained for the infinite medium for the case of finite size may introduce errors in the boundary conditions. The macroscopic wave equation (4.22) has the asymptotic origin and is useful when the wave length L is larger then the characteristic size l of the microstructure such that η = l/L < 1. In order to estimate the area of applicatibility of this model we compare the dispersive dependence which is obtained from equation (4.22) with the exact solution found for the linear case with the help of the Floquet-Bloch theory. We consider the linear wave (E2 = 0): u = Uexp (ikx) exp (iωt) ,

(4.26)

where k is the wave number, k = 2π/L; ω is the frequency. We substitute (4.26) into equation (4.22), and obtain the asymptotic formula for the dispersive dependence 4 2 2 2 E3 2 η +O η , (4.27) ω = ω0 1 − 4π E1 where: ω0 = v0 k; η = l/L = kl/ (2π). The formula (4.27) describes the acoustic branch of the dispersive curve. Keeping the larges number of terms we may increase the numerical accuracy of the solution. However, in principle it is impossible to model the successive branches in the upper spectrum part. With decreasing the wave length (increasing the frequency) in the composite material the pass and stop bands appear [98]. If a frequency goes into the stop band, there appears standing wave, the group velocity of which is equal to zero. Following theory of Floquet-Bloch [98], the exact dependence between ω and k can be found by solving the transcendent equation of the following form cos (kl) = cos k(1) l (1) cos k(2) l (2) − ! (4.28) 1 z(1) z(2) (1) (1) (2) (2) − sin k l sin k l , 2 z(2) z(1) where k(n) = ω/v(n) .

Table 4.2 Properties of the components of the composite materials. Material Steel Helca 37 Aluminium D16T Carbonplastic

λ [GPa] 111 57 5.18

µ [GPa] 82.1 27.6 3.45

ρ [kg/m3 ] 7800 2700 1600

ν [m/s] 5940 6450 2750

z · 10−6 46.3 17.4 4.40

72

Linear and Nonlinear Waves in Microstructured Solids

Figure 4.3 Acoustic branches of the dispersive curves in linear case: (a) steel-aluminium; (b) steel-carboplastic [reprinted with permission from Elsevier].

Fig. 4.3 presents the acoustic branches of the dispersive curves localized in the intervals of the first pass band 0 < η < 1/2. The threshold value η = 1/2 (L = 2l) corresponds to the first stop band. The dashed curves correspond to the asymptotic formula (4.27), whereas solid curves represent the exact solution (4.28). The computations have been carried out for the cases of low-contrast “steel-aluminium” and high-contrast “steel-carboplastic” composite materials. Properties of the components are shown in Table 4.2, based on references [286, 370]; volume fractions of components are the same, c(1) = c(2) = 0.5. The obtained results show that the convergence of the asymptotic solution (4.27) depend on the material properties. In the considered examples the homogenized wave equation (4.22) guarantees the efficient accuracy for η = l/L < 0.4.

4.4

ANALYTICAL SOLUTION FOR STATIONARY WAVES

We consider the stationary wave propagating with a constant velocity without changing of its form. In the latter case the solution satisfies the following conditions u (x,t) = u (ξ ) ,

(4.29)

where: ξ is the running wave variable, ξ = x − vt, v is the phase velocity. We introduce the following non-dimensional deformation of the wave profile: f=

du . dξ

Substituting relations (4.29), (4.30) into equation (4.22) one gets v2 d f E2 d f E3 2 d 3 f + f + l = 0. 1− 2 v0 dξ E1 dξ E1 dξ 3

(4.30)

(4.31)

Integration with respect to the variable ξ yields the following equations of the harmonic oscillator with squared nonlinearity d2 f + a f + b f 2 + c = 0, dξ 2

(4.32)

73

Longitudinal Waves in Layered Composites

where: a = E1 1 − v2 /v20 / E3 l 2 , b = E2 / 2E3 l 2 , c is the constant of integration. A few researchers did not take into account the constant c while investigating the propagation of nonlinear waves in solid media [158]. The obtained results were erroneous from the physical standpoint. It is clear that the displacements u cannot increase unboundedly. It means that the average deformation with regard to the wave period should be equal zero: 1 L

ZL

f (ξ ) dξ = 0.

(4.33)

0

Condition (4.33) allows to find constant c. In order to find the exact analytical solution, we multiply equation (4.32) by d f /dξ , and after integration one gets 1 df 2 a 2 b 3 + f + f + f = W0 . 2 dξ 2 3

(4.34)

Relation (4.34) can be interpreted as the energy conservation principle of the anharmonic oscillator. The integration constant W0 presents the initial total energy of the system, W0 > 0; Wk = (1/2) (d f /dξ )2 is the kinetic energy; Wp = (a/2) f 2 + (b/3) f 3 + f is the potential energy; W0 = Wk +Wp . Equation (4.34) can be recast to the following form: √ df 2dξ = q . W0 − c f − a2 f 2 − b3 f 3

(4.35)

A solution exists if the kinetic energy satisfies the following inequality Wk = W0 −Wp = W0 − c f −

a 2 b 3 f − f > 0. 2 3

(4.36)

The cubic term W0 − c f − (a/2) f 2 − (b/3) f 3 , depending on the values of the coefficients, is responsible either for one or three real roots. Since the case of one real root corresponds to the unbounded solution it is not further considered, the solution is bounded and periodic if the function Wk = W0 − c f − (a/2) f 2 − (b/3) f 3 takes values on the interval between its real roots. Let us present the polynom W0 − c f − (a/2) f 2 − (b/3) f 3 through its roots f1 , f2 , f3 : a b b W0 − c f − f 2 − f 3 = − ( f − f1 ) ( f − f2 ) ( f − f3 ) , (4.37) 2 3 3 where 3a 3c f1 + f2 + f3 = − , f1 f2 + f2 f3 + f1 f3 = , 2b b (4.38) 3W0 f1 f2 f3 = . b

74

Linear and Nonlinear Waves in Microstructured Solids

Figure 4.4 Kinetic energy of the oscillator with square nonlinearity: (a) b < 0, (b) b > 0 [reprinted with permission from Elsevier].

Equation (4.35) is recast to the following form r 2 df . − bdξ = p 3 ( f − f1 ) ( f − f2 ) ( f − f3 )

(4.39)

Assume the following order of the roots: f1 ≥ f2 ≥ f3 . Form of the graph of the kinetic energy function depends on the soft (E2 < 0, b < 0) or hard (E2 > 0, b > 0) nonlinearity of the composite material (Fig. 4.4). In what follows we briefly consider both cases. Soft nonlinearity. If b < 0, then the periodic solution exists for f2 ≥ f ≥ f3 . Let us carry out the following change of the variables g2 =

f − f3 , f2 − f3

0 ≤ g2 ≤ 1,

f2 − f3 , 0 ≤ s2 ≤ 1. f1 − f3 Equation (4.39) takes the following form: r b dg − ( f1 − f3 )dξ = p . 2 6 (1 − g ) (1 − s2 g2 ) s2 =

Integration of equation (4.42) yields r Zg b dg − ( f1 − f3 )ξ = p . 2 6 (1 − g ) (1 − s2 g2 )

(4.40) (4.41)

(4.42)

(4.43)

0

We carry out inversion of the elliptic integral occurring on the right hand side of equation (4.43) [2]: "r # b 2 f = f3 + ( f2 − f3 ) sn − ( f1 − f3 )ξ , s . (4.44) 6

75

Longitudinal Waves in Layered Composites

p p Let us introduce the following notations: F = f2 − f3 , κ = 2 −b ( f1 − f3 ) /6 = −2bF/ (3s2 ), where F is the amplitude, F > 0, κ is the constant of propagation (analog of frequency). Solution (4.44) has the period L = 4K (s) /κ. Substituting (4.44) into condition (4.33) yields 1 − E (s) /K (s) , (4.45) f3 = −F s2 where K (s) and E (s) stand for complete elliptic integrals of the first and second kind, respectively [2]. Finally, we have E (s) 1 − E (s) /K (s) F , f2 = F + f3 = F 1 − , (4.46) f1 = 2 + f3 = F 2 s s K (s) s2 and solution (4.44) is recast to the following form f = −F

1 − E (s) /K (s) 2 κ + Fsn ξ , s . s2 2

(4.47)

Modulus s of the elliptic function stands for solution to the following transcendental equation FE2 s2 K(s)2 = − . (4.48) 48η 2 E3 The propagation constant κ is coupled with wave length L in the following way κ=

4K (s) . L

(4.49)

Velocity of the wave propagation is found from equation (4.38), and it reads v2 E3 = 1 − 16 3E (s) /K (s) − 2 + s2 K(s)2 η 2 . E1 v20

(4.50)

Hard nonlinearity. If b > 0, then the periodic solution exists for f1 ≥ f ≥ f2 . Instead of relations (4.40), (4.41), we introduce the following dependencies f1 − f , f1 − f2 f1 − f2 s2 = , f1 − f3 g2 =

0 ≤ g2 ≤ 1, (4.51) 0 ≤ s2 ≤ 1,

and we introduce the notation F = f1 − f2 > 0,

q p κ = 2 b ( f1 − f3 ) /6 = 2bF/ (3s2 ).

(4.52)

76

Linear and Nonlinear Waves in Microstructured Solids

Carrying out the transformations in a way analogous to the previous, we get f =F

1 − E (s) /K (s) 2 κ − Fsn ξ , s , s2 2

(4.53)

where modulus s is defined by the following transcendental equation s2 K(s)2 =

FE2 . 48η 2 E3

(4.54)

The relations (4.49), (4.50) are the same. Observe that the solutions (4.47), (4.48) in the case of soft nonlinearity (E2 < 0) and the solution (4.53), (4.54) in the case of hard nonlinearity (E2 > 0) get over to each other while changing the sign of coefficient E2 .

4.5

ANALYSIS OF SOLUTION AND NUMERICAL RESULTS

The value of parameter s estimates intensity of the nonlinear effects as well as allows to define how strong the nonlinear regime of the wave propagation differs from the linear one. Fig. 4.5 presents the form of nonlinear waves of deformation for different values of s. The computations have been carried out for the composite material with soft nonlinearity based on equation (4.47).

Figure 4.5 Forms of periodic nonlinear waves of deformation for E2 < 0 [reprinted with permission from Elsevier].

In the case of s = 0 the following limiting transitions take place: E (0) = π/2, K (0) = π/2, E (0) /K (0) ∼ 1 − s2 /2, sn (z, 0) = sin (z). The found solution describes the following harmonic wave 2π F 2π F f = − cos ξ for E2 < 0, f = cos ξ for E2 > 0, 2 L 2 L v2 E3 = 1 − 4π 2 η 2 . E1 v20

(4.55)

Longitudinal Waves in Layered Composites

77

In the case of s = 1, the periodic nonlinear wave is transformed into the localized wave of the bell-form (soliton) - see Fig. 4.6. Having in mind that: E (1) = 1, lim K (s) = ∞, sn(z, 1)2 = 1 − sech(z)2 , one gets s→1

12E3 ξ ∆2 =− for E2 < 0, f = −Fsech , ∆ l2 FE2 ξ 12E3 ∆2 f = Fsech2 = for E2 > 0, , 2 ∆ l FE2 2

(4.56)

E3 l 2 v2 = 1 + 4 , E1 ∆2 v20 where the parameter ∆ stands for the soliton width.

Figure 4.6 Localized nonlinear waves of deformations (solitons): (a) soft nonlinearity (E2 < 0); (b) hard nonlinearity (E2 > 0) [reprinted with permission from Elsevier].

Analysis of solution (4.56) allows to achieve important conclusions regarding properties of the localized nonlinear waves propagation in composite materials. Since F > 0, then in the case of soft nonlinearity (E2 < 0) we have f < 0. It means that in such material the localized waves of compression propagate. On contrary, in the case of hard nonlinearity (E2 > 0) we have f > 0, and consequently only localized waves of extension may exist. Increase of the soliton amplitude F yields decrease of its width ∆ and increase of its velocity v. Therefore, the “high” solitons have the small width and propagate faster than “low” solitons. The velocity of solitons is higher than the velocity of waves propagating in linear homogeneous medium: v > v0 . It is the ultrasonic regime. The analogous effect is observed while studying nonlinear waves of deformation in homogeneous solid [158, 398]. Further numerical examples is devoted to the case of the steel-aluminium composite. Properties of the components are the same: c(1) = c(2) = 0.5. Owing to the obtained solution (4.23)–(4.25), we compute the effective elastic coefficients: E1 = 160 GPa, E2 = −2385 GPa (soft nonlinearity) for E3 = 2.73 GPa.

78

Linear and Nonlinear Waves in Microstructured Solids

Figure 4.7 Phase velocity of the nonlinear wave of deformation [reprinted with permission from Elsevier].

Fig. 4.7 presents the results for the phase velocity v of the nonlinear wave. For s < s0 the super sonic (v < v0 ) regime is realized, whereas for s > s0 we deal with the ultrasonic regime (v > v0 ). Owing to relation (4.50) the threshold value s0 is defined by the following condition 3E (s0 ) − 2 + s20 = 0. K (s0 )

(4.57)

Solving numerically equation (4.57) yields s0 = 0.9803 . . .. It should be noticed that the given value is defined only by the character of the obtained analytical solutions and does not depend on the properties of the composite material. The obtained numerical results (Figs. 4.5, 4.7) yield conclusion that influence of nonlinearity on the form and velocity of the wave become important for s > 0.6 . . . 0.8. In the case of smaller values of s, the wave form almost does not differ from harmonic one, whereas the regime of propagation is very close to the linear regime. We consider how the value of parameter s depends on the wave amplitude F and on the ratio of the wave length L and the size of the material microstructure l. Note that the parameter η = l/L characterizes intensity of the effect of dispersion. The higher value η, the bigger is influence of the microstructure on the dissipation of the wave energy. The parametric dependencies of the modulus s on F and η are shown in Fig. 4.8 (they have been found by solving numerically equation (4.48)). The obtained data illustrate how phenomena of nonlinearity and dispersion compensate each other. Increase of the amplitude F(with constant η) implies increase of s which yields increase of intensity of the nonlinear effects. In contrary, decrease of the wave length and increase of η (with constant amplitude F) yields decrease of the parameter s; the solution becomes more close to its linear counterpart.

Longitudinal Waves in Layered Composites

79

Figure 4.8 Modulus s characterizing intensity of the nonlinear effects [reprinted with permission from Elsevier].

Analysis of the results presented in Fig. 4.8 allows to estimate areas of applibility of various approximate theories, which are employed for modeling of elastic waves propagating in solids. For the majority of materials used for mechanical constructions, the area of elastic deformations is bounded by the value of F ≤ 10−3 . Nonlinear effects are exhibited for s > 0.6 (in the latter case η < 0.13). Consequently, modeling of nonlinear waves can be carried out in the scope of the length wave linear approximation (for instance by employing of the higher order continuous or homogenize models). Occurrence of dispersion plays a key role when the wave length is close to the size of the internal structure of material, i.e. for η > 0.3 (see Fig. 4.3). Then we get s < 0.28, which means that the nonlinear effects can be neglected. Therefore, the problem of propagation of short and strongly dispersive waves can be analyzed in the scope of linear theory. The solution can be obtained with a help of the Floquet-Bloch method [98]. The so far given statements are not valid if the model allows for large values of elastic deformations (F > 10−2 . . . 10−1 ). In the latter case, the nonlinear and dispersive effects may appear simulteneously. They are exhibited by the rubber-type materials and elastomers, molecular and atomic chains, nano tubes, etc.

Shear Waves in 5 Antiplane Fiber Composites with Structural Nonlinearity The antiplane shear waves propagating in a fiber composite with an account of structural nonlinearity are studied. Boundary value problem for imperfect bonding conditions are given and discussed. Then, the macroscopic wave equation is derived and analytical solution for stationary waves is presented and analyzed in the case of soft and hard nonlinearities.

5.1

BOUNDARY VALUE PROBLEM FOR IMPERFECT BONDING CONDITIONS

We consider the fiber composite consisting of the matrix Ω(1) and the square lattice of cylindrical inclusions Ω(2) (Fig. 5.1). We assume that physical and geometric nonlinearity can be neglected, and the non-linear properties of the model are originated from imperfect contact conditions on the boundary of the components. The latter effect stands for the structural nonlinearity which is associated with nonhomogeneity of the internal structure of the composite material.

Figure 5.1 Fiber composite material.

We investigate the propagation of the elastic waves in plane perpendicular to the fibers axis. In this case the components of the stress-strain state depend only on 81

82

Linear and Nonlinear Waves in Microstructured Solids

two spatial co-ordinates x1 , x2 , and the system of equations of motion is split into two uncoupled problems governing propagation of plane waves and antiplane shear waves. Our further considerations are limited to consider only antiplane transverse waves. The governing wave equation has the following form: ! 2 (n) ∂ 2 u(n) ∂ 2 u(n) (n) ∂ u + = ρ (n) , (5.1) µ 2 2 ∂t 2 ∂ x1 ∂ x2 where: µ (n) is the Young’s modulus; u(n) is the displacement in direction x3 , n = 1, 2. We consider the model of imperfect contact between fibers and the matrix. We suppose the following bonding conditions concerning stresses σ ∗ = σ (1) = σ (2)

at

∂ Ω,

(5.2)

where: σ (n) = µ (n) (∂ u(n) /∂ n), ∂ /∂ n – derivation along normal n to the boundary ∂ Ω. The violation of the mechanical coupling between the fibers and the matrix supplies occurrence of discontinuities in the displacement fields. One of the most popular approach aimed on modeling of the imperfect contact consists of employment of the dependence between the displacements jump ∆u∗ = u(1) − u(2) and the stresses σ ∗ on the separation boundary: ∆u∗ = f (σ ∗ )

at

∂ Ω,

(5.3)

where f (σ ∗ ) stands for the function of adhesion. Problems of imperfect contact were investigated by numerous authors. In the simple cases the adhesion function is assumed to be linear, and the boundary of separation plays the role of a spring [5, 71, 202, 276, 332, 333, 336]. In [159, 160, 436, 437] a few kinds of more complex adhesion dependencies are considered. Owing to the employed models, weakness of the coupling between the matrix and inclusion σ ∗ increases with increase of ∆u∗ achieves a maximum, and then decreases up to zero, which corresponds to the destruction of the bonding. The latter approach has been successively used to describe scenarios of microscopic damage of composite materials. Bonds with nonlinear properties were investigated in [277–279]. Experimental investigations of the adhesion have been carried out in [428]. If the dependence (5.3) does not strongly differ from a linear one, it can be approximated by the following truncated series: " ∗ 3 # ∗ ∆u∗ 5 ∗ ∗ ∆u ∗ ∆u σ = µ1 + µ3 +O at ∂ Ω, (5.4) h h h where h stands for the thickness of the boundary of separation between the components. Deformation exhibits symmetry and hence the adhesion function is odd, i.e. we have f (σ ∗ ) = − f (−σ ∗ ), and only odd powers of the quantity ∆u∗ /h appear in the

Antiplane Shear Waves in Fiber Composites with Structural Nonlinearity

83

expression (5.4). The coefficients µ1∗ , µ3∗ represent the linear and nonlinear stiffness in the bonding of components, respectively. The series (5.4) yields " # σ∗ 5 ∆u∗ σ ∗ µ3∗ σ ∗ 3 +O at ∂ Ω. (5.5) = ∗− ∗ ∗ h µ1 µ1 µ1 µ1∗ In order to model effects of the imperfect contact, the following nondimensional adhesion parameters are introduced hu(1) α= , lu∗1

µ∗ β = 3∗ µ1

µ (1) µ1∗

!2 ,

(5.6)

where the thickness of the boundary h is rescaled with regard to the size of the cell of periodicity l, whereas the stiffnesses µ1∗ , µ3∗ are rescaled with respect to the modulus µ (1) . Let the thickness and stiffness of the bonding tends to zero: h → 0, µ1∗ → 0, µ3∗ → 0. Then in the asymptotic limit, depending on the values of parameters α and β , one may takes into account various kinds of adhesion between the components. Formula (5.5) is recast to the following form u(1) − u(2) = αl

∗ 3 σ∗ σ − αβ l µ (1) µ (1)

at ∂ Ω.

(5.7)

The value α = 0 corresponds to the ideal contact, whereas the transition α → ∞ stands for lack of the contact between fibers and the matrix. In the case β = 0 the elastic properties of the bonding are linear while increase of |β | implies increase of the nonlinearity. In the case β < 0 (β > 0) the nonlinearity is soft (hard). Relations (5.1), (5.2) and (5.6) present the input boundary value problem. The proposed model of the imperfect bonding is correct in the case of soft nonlinearity. Equation (5.6) has an asymptotic character and can be used if in its right hand side the ratio of the second to first term does not exceed 10−1 . The ratio of stress σ ∗ to the matrix stiffness µ (1) is approximately equal to the elastic deformation ε. Therefore, one gets the following estimation: |β |ε 2 ≤ 10−1 . The allowed values of β are presented in Table 5.1.

Table 5.1 Maximum allowed values of the adhesion parameter β vs. the values of elastic deformations ε. ε |β |

10−6 1011

10−5 109

10−4 107

10−3 105

84

Linear and Nonlinear Waves in Microstructured Solids

In the engineering practice the effect of the imperfect bonding can be caused by various reasons either through: defects and imperfection while fabricating the material, or via separation of a boundary in the exploitation process. Besides, there is a possibility when the adhesion between inclusions and the matrix is decreased, which implies decrease of the local stress concentrations. The proposed model of imperfect bonding does not depend on the physical circumstances causing damage of the coupling between components, and hence they can be used for description of a wide class of problems. There is only one requirement to be satisfied: weak nonlinear behavior of adhesion f (σ ∗ ) allows for employment of the truncated series (5.4). The parameters α and β have the phenomenological character. It is assumed that for real materials their values can be found experimentally [428]. The boundary value problem (5.1), (5.2), (5.7) stands for various physical interpretations. Besides of the considered example of the elastic wave, it can also describe processes of propagation of electromagnetic waves in the composites with the dielectric inclusions.

5.2

MACROSCOPIC WAVE EQUATION

Let us introduce the following nondimensional variables: u¯ =

u , U

n¯ =

n , L

x¯k =

xk , L

k = 1, 2,

U = max u.

(5.8)

Taking into account that σ ∗ = µ (1) (∂ u(1) /∂ n)

at

(5.9)

∂ Ω,

the boundary value problem (5.1), (5.2), (5.7) can be written in the following way ! 2 (n) ∂ 2 u¯(n) ∂ 2 u¯(n) (n) ∂ u¯ = ρ (n) L2 µ + , (5.10) 2 2 ∂t 2 ∂ x¯1 ∂ x¯2 µ (1) u¯

(1)

(2)

− u¯

∂ u¯(1) ∂ u¯(2) = µ (2) ∂ n¯ ∂ n¯

∂ u¯(1) − αηδ = αη ∂ n¯

at ∂ Ω, ∂ u¯(1) ∂ n¯

(5.11)

!3 at ∂ Ω,

(5.12)

where η = l/L, δ = β (U/L)2 stands for the small parameter. In the order to obtain the macroscopic wave equation, we employ the asymptotic method of homogenization. We introduce “slow” x¯k and “fast” yk = η −1 x¯k coordinates. The solution has the following asymptotic form (n)

(n)

(5.13)

i = 1, 2, 3, . . .

(5.14)

u¯(n) = u0 (x¯k ) + ηu1 (x¯k , yk ) + η 2 u2 (x¯k , yk ) + . . . , where

(n)

(n)

ui (x¯k , yk ) = ui (x¯k , yk ± 1) ,

Antiplane Shear Waves in Fiber Composites with Structural Nonlinearity

The recurrent system of boundary value problems on a cell takes the form ! (n) (n) (n) (n) 2 (n) ∂ 2 ui−2 ∂ 2 ui−1 ∂ 2 ui−1 ∂ 2 u(n) ∂ 2 ui (n) ∂ ui−2 i µ + +2 +2 + + = ∂ x¯1 ∂ y1 ∂ x¯2 ∂ y2 ∂ x¯12 ∂ x¯22 ∂ y21 ∂ y22

85

(5.15)

(n) ∂ 2 ui−2 ρ (n) L2 , ∂t 2 (1)

µ (1)

∂ ui−1 ∂ u(1) + i ∂ n¯ ∂m (1)

(1) (2) ui − ui

=α

(2)

! = µ (2)

∂ ui−1 ∂ u(1) + i ∂ n¯ ∂m

∂ ui−1 ∂ u(2) + i ∂ n¯ ∂m

!

(1)

!

∂ ui−1 ∂ u(1) + i ∂ n¯ ∂m

− αδ

at ∂ Ω,

(5.16)

!3 at ∂ Ω,

(5.17)

(n)

where: i = 1, 2, 3 . . . , u¯−1 = 0, and ∂ /∂ m is the derivative along the normal to ∂ Ω expressed in “fast” co-ordinates. The periodicity conditions (5.14) can be substituted by the condition of zero average value along the period ZZ

(1)

u dy1 dy2 + (1) i

Ω0

ZZ

(2)

(2)

Ω0

ui dy1 dy2 = 0.

(5.18)

The boundary value problems (5.15)–(5.18) can be considered in the interval of the separated cell of periodicity of the composite material (Fig. p 5.2). In “fast” coordinates the cell size is equal to unit, and the fiber radius is c(2) /π, where c(2) stands for the volume fraction of the fibers, and 0 ≤ c(2) ≤ π/4.

Figure 5.2 Cell of periodicity of the fiber composite material.

In order to find the approximate analytical solution we reduce the problem on cell into its axially symmetric form. For this purpose we replace the square cell by

86

Linear and Nonlinear Waves in Microstructured Solids

Figure 5.3 Simplification of the geometric form of the cell.

a circular one with the same area (Fig. 5.3). The accuracy of this approach increase with decreasing the volume fraction of fibers. The solution to the nonlinear problems on a cell can be approximated by the following expansion: (n) (n) (n) ui = ui0 + δ ui1 + O δ 2 . (5.19) The coefficients q of the series (5.19) are found using the polar system of co(n) ordinates r = y21 + y22 , tan θ = y2 /y1 . The term u1 is defined with accuracy of (n)

(n)

O (δ ), whereas the terms u2 and u3 keep accuracy of O(δ 0 ). Symbolic transformations were carried out using the Maple package, but they are omitted here due to their complexity. We employing the averaging operator (n) u¯4

R 2π R (4π)−1/2 0

0

(·) r dr dθ with respect to the

equation (5.15) for i = 4. The terms can be cancelled on the basis of the GaussOstrogradsky theorem with a help of conditions (5.14), (5.16). In result, the following macroscopic nonlinear wave equation is obtained " 2 ∂ 2 u0 ∂ u0 2 1 ∂ 2 u0 ∂ u0 2 ∂ u0 ∂ 2 u0 + + + + δ µ2 µ1 3 ∂ x¯12 ∂ x¯2 ∂ x¯12 ∂ x¯22 ∂ x¯12 ∂ x¯1 # 4 ∂ u0 ∂ u0 ∂ 2 u0 1 ∂ 2 u0 ∂ u0 2 ∂ 2 u0 ∂ u0 2 (5.20) + + + 3 ∂ x¯1 ∂ x¯2 ∂ x¯1 ∂ x¯2 3 ∂ x¯22 ∂ x¯1 ∂ x¯22 ∂ x¯2 4 ∂ u0 ∂ 4 u0 ∂ 2 u0 ∂ 4 u0 2 4 η2µ3 = ρ L2 2 . + 2 + + O δ + η 4 2 2 4 ∂t ∂ x¯1 ∂ x¯1 ∂ x¯2 ∂ x¯2

Antiplane Shear Waves in Fiber Composites with Structural Nonlinearity

87

Transition to dimensional variables u = u0U, xk = x¯k L allows for recasting equations (5.20) to the following form " 2 ∂ u ∂ 2u ∂ 2u ∂ u 2 1 ∂ 2u ∂ u 2 µ1 + + β µ2 + + 3 ∂ x12 ∂ x2 ∂ x12 ∂ x22 ∂ x12 ∂ x1 # 1 ∂ 2u ∂ u 2 ∂ 2u ∂ u 2 4 ∂ u ∂ u ∂ 2u (5.21) + + 2 + 3 ∂ x1 ∂ x2 ∂ x1 ∂ x2 3 ∂ x22 ∂ x1 ∂ x2 ∂ x2 4 ∂ u ∂ 2u ∂ 4u ∂ 4u 2 2 2 4 η L µ3 , = ρ + 2 + + O δ + η ∂t 2 ∂ x14 ∂ x12 ∂ x22 ∂ x24 where µ1 , µ2 , µ3 are effective moduli of stiffness, obtained analytically: 2 2 2 2 µ1 = µ (1) c(2) π 3/2 µ (2) + 2 c(2) π 3/2 µ (2) µ (1) − 4 2 4 2 µ (1) c(2) π 3/2 µ (2) + 2 c(2) π (3/2) µ (2) µ (1) − 4 3 2 3 c(2) π 3/2 µ (1) + c(2) π 3/2 µ (1) + 2 3/2 3/2 2 2µ (1) α µ (2) π 2 c(2) + 2α µ (2) π 2 c(2) µ (1) − 2 3 2 µ (1) α 2 µ (2) π 5/2 c(2) + µ (1) α 2 µ (2) c(2) π 5/2 + 2 7/2 7/2 2 (1) (2) 2 (2) (2) (2) 2 (1) 2µ α µ π c − 2α µ c π µ / 3/2 7/2 µ (1) + 2α µ (2) c(2) π 2 µ (1) − 2α µ (2) π 2 c(2) 2 3 2 (5.22) 2 µ (2) c(2) π 3/2 + 2 c(2) π 3/2 µ (2) µ (1) − 4 2 3/2 2 c(2) π 3/2 µ (2) µ (1) + 2α µ (2) π 2 c(2) + 2 3 2 2 7/2 α 2 µ (2) π 5/2 c(2) + α 2 µ (2) c(2) π 5/2 − 2α µ (2) π 2 c(2) + 2 2 3 2 c(2) π 3/2 + c(2) π 3/2 µ (2) + 2 µ (1) 2 2 4 2 2 4 c(2) π 3/2 µ (2) + c(2) π 3/2 µ (1) + c(2) π 3/2 µ (1) + 2 2 5/2 , 4α µ (2) π 2 c(2) µ (1) + 2α 2 µ (2) π 5/2 c(2) 5/2 4 µ2 = 36α µ (1) π c(2) µ (2) / 4 4 6 5 −4 c(2) π 1/2 µ (2) + c(2) π 1/2 µ (1) +

88

Linear and Nonlinear Waves in Microstructured Solids

4 4 3 4 2 4 6 c(2) π 1/2 µ (1) − 4 c(2) π 1/2 µ (2) + c(2) π 1/2 µ (1) + 6 4 3 2 2 c(2) π 1/2 µ (2) + 12c(2) µ (2) α 2 π 3/2 µ (1) + 6c(2) µ (2) α 2 π 3/2 µ (1) + 2 2 2 3 2 2 24 c(2) µ (2) α 2 π 3/2 µ (1) + 36 c(2) µ (2) α 2 π 3/2 µ (1) + 2 3 4 3 24 c(2) µ (2) α 2 π 3/2 µ (1) − 24 c(2) µ (2) α 2 π 3/2 µ (1) + 5 4 4 4 4 c(2) π 1/2 µ (1) + 6 c(2) π 1/2 µ (2) − 3 3 3 2 5 4 12 c(2) π 1/2 µ (1) µ (2) − 8 c(2) π 1/2 µ (1) µ (2) + 8 c(2) π 1/2 µ (2) µ (1) − 6 3 6 3 2 4 4 c(2) π 1/2 µ (2) µ (1) − 4 c(2) π 1/2 µ (2) µ (1) + c(2) π 1/2 µ (2) + 4 2 2 4 2 2 α 4 µ (2) π 5/2 + 6 c(2) π 1/2 µ (1) µ (2) + 24 c(2) µ (2) α 2 π 3/2 µ (1) − 5 2 2 5 3 µ (2) α 2 π 3/2 µ (1) + 12 c(2) µ (2) α 2 π 3/2 µ (1) + 6 c(2) 3 3/2 3 3/2 12 µ (2) πα c(2) µ (1) + 16 µ (2) π 2 α 3 c(2) µ (1) + 2 3/2 2 3/2 3 12 µ (2) πα c(2) µ (1) + 4µ (2) πα c(2) µ (1) + 3 9/2 2 9/2 2 4 µ (2) π 2 α 3 c(2) µ (1) − 24 µ (2) πα c(2) µ (1) + 9/2 3 3 5/2 16µ (2) πα c(2) µ (1) + 24 µ (2) π 2 α 3 c(2) µ (1) + 5/2 3 2 5/2 2 16µ (2) πα c(2) µ (1) + 24 µ (2) πα c(2) µ (1) + 11/2 3 2 11/2 2 4π µ (2) α c(2) µ (1) − 12π µ (2) α c(2) µ (1) + 3 11/2 3 7/2 12π µ (2) α c(2) µ (1) + 16 µ (2) π 2 α 3 c(2) µ (1) − 3 7/2 7/2 3 24 µ (2) πα c(2) µ (1) + 24µ (2) πα c(2) µ (1) + 4 3 6 2 3 5 8 c(2) π 1/2 µ (1) µ (2) + 6 c(2) π 1/2 µ (1) µ (2) + 4 c(2) π 1/2 µ (1) + 4 5 4 4 3 µ (2) α 2 π 3/2 + 6 c(2) µ (2) α 2 π 3/2 − 12 c(2) µ (2) α 2 π 3/2 + 6 c(2) 4 9/2 4 3/2 4 3/2 − 4 µ (2) π 2 α 3 c(2) + + 4 µ (2) πα c(2) 8 µ (2) π 2 α 3 c(2) 4 9/2 4 4 2 8 µ (2) πα c(2) + 4α 4 µ (2) π 5/2 c(2) + 6α 4 µ (2) π 5/2 c(2) + 4 5/2 4 4 4 3 − 4α 4 µ (2) π 5/2 c(2) + α 4 µ (2) π 5/2 c(2) − 8 µ (2) πα c(2) 4 7/2 2 3 4 11/2 + 4 c(2) π 1/2 µ (2) µ (1) + 4π µ (2) α c(2) − 8 µ (2) π 2 α 3 c(2)

89

Antiplane Shear Waves in Fiber Composites with Structural Nonlinearity

2 3 3 3 4 c(2) π 1/2 µ (2) µ (1) − 8 c(2) π 1/2 µ (1) µ (2) + 4 1/2 3 1/2 4π 2 µ (2) α 3 c(2) + 4π 2 µ (2) α 3 c(2) µ (1) . The values of the effective modulus µ3 were defined through numerical integration along the area of the cell of periodicity using the standard procedure of the Maple package. The obtained results are based on the simplification of the geometric form of the cell. In order to estimate accuracy of the proposed approximation, we consider the effective linear modulus µ1 in the case of the ideal contact between components (α = 0). The solution takes the following form: 1 − c(2) µ (1) + 1 + c(2) µ (2) . (5.23) µ1 = µ (1) 1 + c(2) µ (1) + 1 − c(2) µ (2) Observe that formula (5.23) can be obtained with a help of the self-consistent approach and coincides with the lower Hashin-Strickman bound [123]. A comparison of the analytical solution (5.23) with the theoretical results achieved in [358] with a help of the Rayleigh method for the composite with infinitely stiff fibers (µ (2) /µ (1) → ∞) is shown in Table 5.2. The given example is characterized by large concentrations of the local stresses, and hence the error of approximate analytical solution achieves a maximum. Decreasing of the fibers stiffness decreases the error.

Table 5.2 Effective linear shear modulus µ1 /µ (1) of the composite material with infinitely stiff fibers c(2) 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.74 0.76 0.77 0.78

Formula (5.23) 1.222 1.50 1.857 2.333 3.000 4.000 5.667 6.692 7.333 -

Data [358] 1.222 1.500 1.860 2.351 3.080 4.342 7.433 11.01 15.44 20.43 35.93

Error % 0.0 0.0 0.2 0.8 2.6 7.9 24.8 39.2 52.5 -

Formula (5.23) guarantees high accuracy for c(2) < 0.5. Error increases with increase of the volume fraction of fibers (c(2) > 0.6) when the distance between neighboring fibers is small. It is associated with occurrence of essential concentration of

90

Linear and Nonlinear Waves in Microstructured Solids

local stresses. In the latter case we need to take into account the space packing of fibers. It should be mentioned that for majority of real composite materials the volume fraction of the fibers does not achieve the value 0.4...0.5. It means that the obtained approximate solutions can be employed in real world situation. As a case study, we consider the composite material composed of the aluminum matrix (µ (1) = 27.9 GPa, ρ (1) = 2700 kg/m3 ) and nickel fibers (µ (2) = 75.4 GPa, ρ (2) = 8940 kg/m3 ). Figures 5.4–5.6 report the results obtained for the effective elastic moduli µ1 , µ2 , µ3 for different values of volume fractions of the fibers c(2) and the adhesion parameter α. Figure 5.4 presents a comparison of the obtained solution with the results obtained in [358] in the case of ideal contact (α = 0, circles) and in the case of material with voids (µ (2) = 0, dashed curve).

Figure 5.4 Effective linear shear modulus of the composite [reprinted with permission from Elsevier].

The effective moduli µ1 , µ3 take maximum values in the case of ideal contact of components (α = 0). The weakness of the coupling between fibers and the matrix (increase of the parameter α) yields decrease of µ1 and µ3 . The effective coefficient µ is equal zero for α = 0. It means that in the case of ideal contacting material the studied behavior is linear. In the interval α = 0.05...0.1 a rapid increase of µ2 is observed, and influence of nonlinearity achieves maximum. Further, decrease of the coupling between the components implies decrease of the coefficient µ2 and decrease of intensity of the nonlinear effects. On the other hand, on increase of volume fraction of inclusions c(2) (with fixed α) yields increase of the effective modulus µ2 . It can be explained in the following way: in the considered example nonlinear behavior of material is mainly governed by the properties on the separation boundary ∂ Ω. Therefore, increase of the area ∂ Ω implies increase of the nonlinearity. The effective modulus µ3 is characterized by intensity of the dispersion effect. For c(2) = 0 the material is homogeneous and there is no dispersion (µ3 = 0). In the case

Antiplane Shear Waves in Fiber Composites with Structural Nonlinearity

91

Figure 5.5 Effective nonlinear shear modulus of the composite material aluminum-nickel [reprinted with permission from Elsevier].

of the average values of the volume fraction of fibers we have c(2) = 0.25...0.45. It means that nonhomogeneity of the internal structure of composite is expressed strongly, and the coefficient µ3 achieves its maximum. Observe that the coefficients µ1 , µ2 and µ3 are always considered as positive. The macroscopic wave equation (5.21) holds for the case of long waves, when η = l/L < 1. In order to estimate the area of applicability of the homogenized model, we compare the dispersive dependences obtained based on equation (5.21) with the solution found with a help of the Floquet-Bloch approach. We consider the linear case (µ2 = 0). The harmonic wave is governed by the following equation u = U exp(ik · x) exp(iωt), (5.24) where: k is the wave vector, k = k1 e1 + k2 e2 ; e1 , e2 are the unit basis vectors in the rectangular system of co-ordinates; x = x1 e1 + x2 e2 . Projections of the vector k to the axes are as follows: k1 = qof the co-ordinates 2 2 kcosϕ, k2 = ksinϕ, where k = |k| = k1 + k2 = 2π/L, and ϕ stands for the angle between axes x1 and direction of the vector k. Substituting of ansatz (5.24) into equation (5.21) yields the following dispersive relation µ3 2 2 4 4 2 2 4 ω = ω0 1 − 4π sin ϕ + cos ϕ η + O(η ) , (5.25) µ1 where: ω0 = v0 k (v0pstands for the effective phase velocity in the linear homogeneous kl medium) and v0 = µ1 /ρ, η = Ll = 2π . Fig. 5.7 presents a comparison of the solution (5.25) (dashed curves) with the computational results obtained using a Floquet-Bloch method. The computations are carried out for the composite composed of aluminum matrix and nickel fibers. Physical properties of components have been given in the above, whereas the volume fraction of the fibers is c(2) = 0.4.

92

Linear and Nonlinear Waves in Microstructured Solids

Figure 5.6 Effective shear modulus of order η 2 [reprinted with permission from Elsevier].

Dispersive diagram is composed of two parts separated by dotted vertical line. The right hand side correspond to the orthogonal (ϕ = 0), whereas the left hand side corresponds to diagonal (ϕ = π/4) direction of the wave propagation. In the long wave interval (ω → 0) the solution becomes isotropic and does not depend on the angle ϕ. However, decrease of the wave length (and increase of the frequency ω) yields exhibition of the anisotropic properties of the composite material. Based on the obtained results one may conclude that the homogenized wave equation (5.21) preserves high accuracy for η < 0.4 (for ϕ = 0) and for η < 0.5 (for ϕ = π/4).

5.3

ANALYTICAL SOLUTION FOR STATIONARY WAVES

Let a stationary wave is propagated in direction defined by the wave vector k. In this case the solution satisfies the following condition u (x,t) = u(ξ ),

(5.26)

where: ξ = ek · x − vt, ek is the unit wave vector, ek = e1 cos ϕ + e2 sin ϕ. Let us introduce nondimensional deformation of wave profile: f=

du . dξ

(5.27)

Substituting relations (5.27), (5.26) into equation (5.21) and carrying out the integration with respect to ξ , the following equation of the anharmonic oscillator with a cubic nonlinearity is obtained d2 f + a f + b f 3 + = 0, dξ 2

(5.28)

Antiplane Shear Waves in Fiber Composites with Structural Nonlinearity

93

Figure 5.7 Acoustic branches of the dispersion curves of the composite material “aluminumnickel” (linear case) [reprinted with permission from Elsevier].

where: a = µ 1 1 − v2 /v20 / µ 3 l 2 , b = β µ 2 / 3µ 3 l 2 and c is the constant of integration. The condition of equality to zero of the averaged deformation along period of the wave in the considered case yields c = 0. We multiply equation (5.28) by d f /dξ , and the carried out integration yields 1 df 2 a 2 b 4 + f + f = W0 , 2 dξ 2 4

(5.29)

where W0 is the total energy of the oscillator with W0 > 0; Wk = (1/2)(d f /dξ )2 is the kinetic energy; Wp = (a/2) f 2 + (b/4) f 4 is the potential energy, and W0 = Wk +Wp . Separation of variables in equation (5.29) gives: √ df 2dξ = q . W0 − 2a f 2 − b4 f 4

(5.30)

The solution is bounded and periodic if the kinetic energy Wk = W0 −Wp = W0 − (a/2) f 2 − (b/4) f 4

(5.31)

takes the positive values on interval between its two real roots. The form of the solution depends on the signs of the coefficients a and b. We consider separately the case of soft (β < 0, b < 0) and hard (β > 0, b > 0) nonlinearity. Soft nonlinearity. If a < 0, b < 0, the polynomial Wk does not have real roots (Fig. 5.8a). Bounded periodic solution of equation (5.28) does not exist.

94

Linear and Nonlinear Waves in Microstructured Solids

Figure 5.8 Kinetic energy of oscillator with cubic nonlinearity; a) a < 0, b < 0 ; b) a > 0, b < 0; c) a > 0, b > 0; d) a < 0, b > 0 [reprinted with permission from Elsevier].

If a > 0, b < 0, the polynomial Wk has four real roots ± f1 , ± f2 (Fig. 5.8b), where p p a − a2 + 4bW0 a + a2 + 4bW0 2 2 f1 = , f2 = , f12 < f22 . (5.32) −b −b The periodic solutions exist for f1≥ f ≥ − f1 . Let us express the polynomial Wk by its roots Wk = − (b/4) f12 − f 2 f22 − f 2 , and let us carry out the following change of variables 0 ≤ g2 ≤ 1, (5.33) g2 = f 2 / f12 , s2 = f12 / f22 ,

0 ≤ s2 ≤ 1.

Then equation (5.30) takes the following form r b dg . − f22 dξ = p 2 2 (1 − g ) (1 − s2 g2 )

(5.34)

(5.35)

Integration of equation (5.35) and inverse of the elliptic integral yields the follow-

Antiplane Shear Waves in Fiber Composites with Structural Nonlinearity

95

ing function ! b 2 − f2 ξ , s , 2

r f = f1 sn where

(5.36)

r

b − f22 , 2 and F stands for the amplitude (F > 0, κ - constant). Then, formula (5.36) takes the following form F = 2 f1 ,

κ=

(5.37)

F sn (κξ , s) . (5.38) 2 The wave length is equal L = 4K (s) /κ. Based on the relations (5.32), (5.34), (5.37) and after the trivial transformations, the following transcendental equation is obtained, which allows to find the module s: β F 2 µ2 s2 K(s)2 = − , (5.39) 2 384η µ3 (sin4 ϕ + cos4 ϕ) The wave velocity is described by the following formula f=

µ3 v2 = 1 − 16(1 + s2 )K(s)2 η 2 (sin4 ϕ + cos4 ϕ). µ1 v20

(5.40)

Hard nonlinearity. Let b > 0. Graphs of the kinetic energies are shown in Fig. 5.8c (for a > 0) and in Fig. 5.8d (for a < 0). In both cases the polynomial Wk has two real ± f1 and two imaginary roots ±i f2 of the following forms p p −a + a2 + 4bW0 a + a2 + 4bW0 2 2 f1 = , f2 = . (5.41) b b The periodic solutions exist if f1 ≥ f ≥ − f1 . We substitute Wk in the form Wk = (b/4)( f12 − f 2 )( f22 + f 2 ) and introduce the −1 2 following variables: g2 = 1 − ff 2 , 0 ≤ g2 ≤ 1; s2 = 1 + f22 / f12 . Here 0 ≤ s2 ≤ 1/2 1 q for a > 0 for 1/2 ≤ s2 ≤ 1 for a < 0 and F = 2 f1 > 0, κ = (b/2) f12 + f22 . We carry out the transformations described earlier, and in result we find f= s2 K(s)2 =

F cn (κξ , s) , 2

β F 2 µ2 , 384η 2 µ3 (sin4 ϕ + cos4 ϕ)

v2 µ3 = 1 − 16(1 − 2s2 )K(s)2 η 2 (sin4 ϕ + cos4 ϕ). µ1 v20

(5.42) (5.43) (5.44)

The wave length is equal to L = 4K(s)/κ. Equations (5.43) and (5.39) turn to each other while changing the sign of the parameter β .

96

Linear and Nonlinear Waves in Microstructured Solids

5.4

ANALYSIS OF SOLUTION AND NUMERICAL RESULT

In the considered case the nonlinearity type (soft for β < 0 and hard for β > 0) has a principal influence on the solution character. The form of periodic waves of deformation is shown in Fig. 5.9. The computations are carried out based on the formulas (5.38) and (5.42).

Figure 5.9 Forms of periodic nonlinear waves of deformations: (a) soft nonlinearity (β < 0) and (b) hard nonlinearity (β > 0) [reprinted with permission from Elsevier].

In the case of s = 0, we have two limiting transitions to the linear solution: 2π F ξ for β < 0, f = sin 2 L F 2π f = cos ξ for β > 0, (5.45) 2 L v2 µ3 = 1 − 4π 2 η 2 (sin4 ϕ + cos4 ϕ). 2 µ1 v0

Antiplane Shear Waves in Fiber Composites with Structural Nonlinearity

97

Figure 5.10 Localized nonlinear waves of deformations: (a) soft nonlinearity (β < 0) and (b) hard nonlinearity (β > 0) [reprinted with permission from Elsevier].

In the case s = 1 in the composite material the localized waves deformation appears. If the nonlinearity is soft, the shock wave is created (kink in Fig. 5.10a): F 24µ3 (sin4 ϕ + cos4 ϕ) ξ ∆2 f = tanh =− , , 2 2 ∆ l F 2 β µ2 (5.46) 2µ3 l 2 v2 4 4 = 1− (sin ϕ + cos ϕ), β < 0. µ1 ∆2 v20 Kink is propagated in the under sonic regime (v < v0 ). The increase of the wave amplitude F yields decrease of its width ∆ and velocity v. If the nonlinearity is hard, the localized solutions takes the form of soliton (Fig. 5.10b): F ∆2 24µ3 (sin4 ϕ + cos4 ϕ) f= , = , 2 2cosh(ξ /∆) l F 2 β µ2 (5.47) v2 µ3 l 2 4 4 = 1+ (sin ϕ + cos ϕ), β > 0. µ1 ∆2 v20 In the latter case, the propagation regime is supersonic (v > v0 ). Increase of the soliton amplitude implies decrease of its width with increase of its velocity. Therefore, in the considered problem the type of nonlinearity defines the form of the localized wave of deformation, but not the mechanical properties of material. We analyze the numerical results for the composite composed on the aluminum matrix (µ (1) = 27.9 GPa, ρ (1) = 2700 kg/m3 ) and fibers made from nickel (µ (2) = 75.4 GPa, ρ (2) = 8940 kg/m3 ). The volume fraction of fiber is c(2) = 0.4. The following values of the adhesion parameters are fixed: α = 0.1, |β | = 105 . The effective elastic coefficients are: µ1 = 33.1 GPa, µ2 = 21.6 GPa, µ3 = 0.119 GPa. The wave propagates in direction orthogonal with respect to the sizes of the periodicity cell: ϕ = 0.

98

Linear and Nonlinear Waves in Microstructured Solids

Figure 5.11 Phase velocity of nonlinear wave of deformations: (a) soft nonlinearity (β < 0) and (b) hard nonlinearity (β > 0) [reprinted with permission from Elsevier].

Antiplane Shear Waves in Fiber Composites with Structural Nonlinearity

99

Figure 5.12 Modulus s characterizing intensity of nonlinear effects [reprinted with permission from Elsevier].

The dependence of the phase velocity v versus modulus s is reported in Fig. 5.11. In the case of soft nonlinearity one deals with the subsonic regime for which v < v0 . In the case of the hard nonlinearity one has supersonic regime and v < v0 if s2 < 1/2 and v > v0 if s2 > 1/2. The threshold value s2 = 1/2, for which the change of the velocity regime takes place, is defined by the qualitative character of the analytical solution (5.44) and does not depend neither on the properties of the composite material nor on direction of the wave propagation. Fig. 5.12 presents the parametric dependence of the modulus s versus F obtained based on the numerically found solution to equation (5.39) (or (5.43)). The area of elastic deformation is bounded by the value F ≤ 10−3 being characteristic for the majority of the materials used in real constructions. As it follows from Fig. 5.9, 5.11, influence of the nonlinearity on the form and velocity of the wave becomes important for s > 0.6. For η < 0.2, the solution can be obtained with a help of the employed method of homogenization. Accuracy of the homogenized model (5.21) is decreased for η > 0.4 (see Fig. 5.7) (in this case s < 0.34), and the nonlinear effects can be neglected. Therefore propagation of nonlinear waves can be investigated in scope of the developed long-wave models, whereas the short waves with strong dispersion effects can be approximated by linear models.

of Localized 6 Formation Nonlinear Waves in Layered Composites This chapter deals with nonstationary wave propagation and formation of localized nonlinear waves in layered composite materials. First, the mathematical model is given and the pseudo-spectral method is described. Then, the Fourier-Pad´e approximation is used to decrease the Gibbs-Wilbraham effects. The process of formation of the localized nonlinear waves originated from the initial impulses of deformation is modeled numerically. The following special cases are considered: (i) generation of a single localized wave; (ii) generation of a train of the localized waves; (iii) scattering of the initial tension impulse.

6.1

INITIAL MODEL AND PSEUDO-SPECTRAL METHOD

Solutions obtained in the previous describe stationary waves which propagate without change of their forms and velocities. However, important role plays analysis of non-stationary dynamic processes. In this section we study evolution of the initial impulses of deformations and formation of the localized nonlinear waves. Here we employ numerical methods. Consider longitudinal waves propagating in a layered composite material in a direction perpendicular to the layers arrangement. Let us define deformation of the wave profile as f = du/dx and introduce the non-dimensional variable f = f /F, x = x/l, t¯ = t/T , where f is the deformation amplitude, T is the time needed by wave propagating in linear homogenous medium to move along the size of periodicity cell p l, and T = l/ν0 , ν0 = E/ρ. Then wave equation (4.22) can be presented in the following form 2 2 ∂ 2 f FE2 ∂ f ∂2 f E3 ∂ 4 f f , P f = = P + + . (6.1) E1 ∂ x4 ∂t 2 ∂ x2 2 E1 ∂ x2 We take the following initial conditions f¯ = f0 (x), ¯

df =0 dt

at t¯ = 0,

(6.2)

where the function f0 = (x) defines the form of initial impulse of deformation. In order to solve the Cauchy problem (6.1), (6.2), the following numerical procedure is employed. Integration in time is carried out by the 4th order Runge-Kutta 101

102

Linear and Nonlinear Waves in Microstructured Solids

method. We present the searched solutions f (x,t) in the form of the discrete sequence of the approximating functions f¯ (x, ¯ t¯) = fk (x) ¯

for t¯ = k∆t,

k = 0, 1, 2 ...,

(6.3)

where ∆t stands for the step of integration. The function fk (x) ¯ is estimated based on the following recurrent relations [245] · 1 fk+1 = fk + fk ∆t + (m1 + m2 + m3 ) ∆t, 6 · · · 1 f0 = 0, fk+1 = fk + (m1 + 2m2 + 2m3 + m4 ) , 6 ·

m1 = P ( fk ) ∆t, m2 = P fk + fk ∆t/2 ∆t, · m3 = P fk + fk ∆t/2 + m1 ∆t/4 ∆t, · m4 = P fk + fk ∆t + m2 ∆t/2 ∆t.

(6.4)

In order to approximate the searched solution in the spatial variable we use the Fourier series. The wave equation (6.1) is symmetric with regard to the co-ordinate’s origin x¯ = 0. If we consider the case when the impulse f0 (x) ¯ is described by an even ·

¯ = function then the solution should be also represented by an even function, fk (x) fk (−x). ¯ Each of the functions fk (x) ¯ can be presented by the following series forms N

fk (x) ¯ =

2π x¯ c cos n , ∑ n,k L0 n=0

k = 0, 1, 2, ...,

(6.5)

where L0 stands for the non-dimensional size of the spatial domain. The coefficients cn,0 , cn,1 are defined through the initial conditions (6.2), and they take the following form 2 cn,0 = L0

LZ0 /2 −L0 /2

2π x¯ , f0 (x) ¯ cos n L0

cn,1 = cn,0 .

(6.6)

The remaining coefficients cn,k , k = 2, 3, 4, ..., are computed with the use of formulas (6.4). The series (6.5) takes into account the boundary conditions of the periodic extension for x¯ = L0 /2. Since we consider the waves in infinite medium, we consider the solution evolution in the interval 0 < x¯ < L0 /2. We have known that the wave equation (6.1) can be used if η = l/L < 0.4. The minimal period of harmonic in series (6.5) is equal to L = L0 l/N. Then we get the enequality N/L < 0.4. (6.7)

Formation of Localized Nonlinear Waves in Layered Composites

103

Condition (6.7) implies the restriction on the number of the terms of the series (6.5). Series (6.5) present a continuous approximation where the Runge-Kutta method is based on the discrete difference scheme. Combination of both approaches is named the pseudo-spectral method [175, 393]. The pseudo-spectral method has found the wide application while solving numerically nonlinear wave equations [69, 243, 395].

6.2

THE FOURIER-PADE APPROXIMATION

In order to improve convergence of the series (6.5) and to decrease the GibbsWilbraham effects [96, 143, 220], we employ the method of Fourier-Pad´e approximation. It allows to decrease the number of terms in the series (6.5) and to increase the minimum harmonic period. The latter circumstance is of particular importance. It allows to extend the area of applicability of the wave equation (6.1) the rational Pad´e approximation of the function g(z) and it can be defined in the following way. Let us present g(z) in the form of the series g (z) = c0 + c1 z + c2 z2 + ... + cN zN + O zN+1 . (6.8) Then the Pad´e approximation takes the following form: g (z) =

a0 + a1 z + a2 z2 + · · · + aK zK + O zN+1 , 2 M 1 + b1 z + b2 z + · · · + bM z

(6.9)

where K + M = N. The coefficients are defined by the following rule: development of (6.9) into the Maclaurin series should coincide with the series (6.8) up to the term O(zN ) inclusively. Transformation (6.9) allows essentially increase convergence of the series (6.8). In practice mostly the diagonal Pad´e approximation are used, where K = M = N/2. In what follow we consider the diagonal approximations. There are a few algorithms devoted to computation of the coefficients while using the Pad´e approximation [47]. In this section we employ the following procedure. The coefficients of that denominator b are defined through the solution of the system of linear algebraic equation of the following form: c1 c2 c3 ... cN/2 bN/2 cN/2+1 c2 c3 c4 ... cN/2+1 bN/2−1 cN/2+2 c3 c c ... c = (6.10) b c 4 5 N/2+2 N/2−2 N/2+3 ... ... ... ... ... ... ... cN/2 cN/2+1 cN/2+2 ... cN−1 b1 cN and then the numerator coefficients ai are defined using the following recurrent formula i

a0 = c0 ,

ai = ci + ∑ bk ci−k , k=1

i = 1, 2, 3, ..., N/2.

(6.11)

104

Linear and Nonlinear Waves in Microstructured Solids

In order to solve system (6.10), the Gauss-Jordan method is employed (it belongs to the one of the most effective methods from the computational point of view). The given algorithm requires O[(N/2)3 ] arithmetic operations, where N/2 stands for the number of the system equations. We use the Fourier series based on the following exponential form ! N N i 2πx L0 n 2π x¯ = Re ∑ ck,n e fk (x) ¯ = ∑ ck,n cos n , (6.12) L0 n=0 n=0 i 2πx L n

and we carry out the replacement e 0 → z. Then, the diagonal Fourier-Pad´e approximation can be presented in the following form ! a0 + a1 z + a2 z2 + ... + aN/2 zN/2 fk (x) ¯ = Re , (6.13) 1 + b1 z + b2 z2 + ... + bN/2 zN/2 where z = exp(2π xi/L ¯ 0 ), and the coefficients ai , bi are yielded by relations (6.10), (6.11). As the case study, we consider the piece-wise continuous function 0 for − 50 < x¯ < −10, f (x) ¯ = 1 for − 10 < x¯ < 10, (6.14) 0 for 10 < x¯ < 50. Fig. 6.1 presents a part of the Fourier series sum (solid curve) being compared with the Fourier-Pad´e approximation (dashed curve) for N = 32. The absolute error is shown in Fig. 6.2 in the logarithmic scale for N = 32 and N = 64. Employment of the Fourier-Pad´e approximation allows for essential improvement of the convergence of the considered series. In the points of discontinuity there are local oscillation of the Fourier series observed, yielded by the Gibbs-Wilbraham phenomena.

Figure 6.1 Approximation of the piece-wise discontinuous function N = 32 [reprinted with permission from Elsevier].

Formation of Localized Nonlinear Waves in Layered Composites

105

Figure 6.2 Absolute error of approximations of the piece-wise discontinuous function: (a) N = 32; (b) N = 64. 1-Fourier series; 2- Fourier-Pad´e approximation [reprinted with permission from Elsevier].

Figure 6.3 Approximations of the piece-wise discontinuous function near the point of discontimaty by Fourier series (solid curve) and Fourier-Pad´e (dashed curve) approximations (N = 256) [reprinted with permission from Elsevier].

Figure 6.4 Approximation of the localized wave by Fourier series (solid curve) and FourierPad´e (dashed curve) approximation (N = 16) [reprinted with permission from Elsevier].

106

Linear and Nonlinear Waves in Microstructured Solids

Figure 6.5 Absolute error of approximations of the localized wave by Fourier series (curve 1) and Fourier-Pad´e (curve 2) approximations (N = 16) [reprinted with permission from Elsevier].

In the case of the Fourier-Pad´e approximation the latter effect is more weak represented (Fig. 6.3). In the case of smooth functions application of the Fourier-Pad´e method is even more effective. Fig. 6.4 presents the results for the case of localized solution which is defined by formula f = sec h(x)2 . Here L0 = 100, and the number of the series terms is N = 16. For the given (relatively small) number of series terms, the Fourier series gives rather bad approximation, whereas the Fourier-Pad´e approximations almost perfectly describe the analyzed function. The absolute error is shown in Fig. 6.5.

6.3

NUMERICAL MODELING OF NON-STATIONARY NONLINEAR WAVES

We consider the processes of formation of the localized nonlinear waves from the initial impulses of deformations. In order to carry out the numerical tests, the program code in C language has been developed. With the use of GNU Compiler Collection we have employed, while carrying out the computations, the values of physical properties of the composite material. We have considered the case of soft nonlinearity, when the ratio of nonlinear to linear stiffness modulus is E2 /E1 ≈ 10. The mentioned value is typical for majority of the construction based on composites fabricated from metals and polymers (see, for instance, [290, 328]). The effective phase velocity in the linear √ quasi-homogenous case is closed to the geometric mean value of velocities ν0 ≈ ν (1) ν (2) . Volume fractions of the components are the same: c(1) = c(2) = 0.5, whereas the ratio of the acoustic components impedances is z(2) /z(1) = 2. The numerical integration of the input wave equation (6.1) has been carried out in the following space-time area: −L0 /2 ≤ x ≤ L0 /2, L0 = 10000, 0 ≤ t ≤ 5000. The number of the included Fourier series terms (Fig. 6.5) is N = 4000, and the time integration step ∆t = 0.5.

Formation of Localized Nonlinear Waves in Layered Composites

We consider the evolution of the initial impulse of the rectangular form L 0 for − 20 < x¯ < − ∆2 , f0 (x) ¯ = 1 for − ∆2 ≤ x¯ ≤ ∆2 , L0 ∆ 0 for 2 < x¯ < 2 ,

107

(6.15)

where ∆ stands for the nondimensional impulse width. The numerical computation is carried out for the three various scenarios: generation of the separate localized wave, generation of a sequence of the localized waves and scattering of the initial impulse. 1. Generation of a single localized wave. Let the initial excitation forms are relatively narrow impulse of width ∆ = 5. The deformation amplitude is F = 10−2 . Observe that such a relatively high value of the elastic deformations is characteristic for the elastomers and rubber-type materials, as well as for polymers and organic molecular chains.

Figure 6.6 Evolution of the “narrow” impulse [reprinted with permission from Elsevier].

108

Linear and Nonlinear Waves in Microstructured Solids

The evolution of the nonlinear wave is shown in Fig. 6.6. Here and further the dashed curves correspond to the solution for time instant t = 0. The rectangular impulse is collapsed into two symmetric parts, which move into opposite directions. We consider the interval 0 < x < L0 /2, since in the interval −L0 /2 < x < 0 the solution is the same. The initial impulse is transformed into the bell-shape localized wave (soliton) with the fast oscillating tail. It should be emphasized that the formation of the localized wave, is carried out in the interval of order x ∼ 103 l. The characteristic size of the internal structure of the composite materials is typically in intervals l ∼ 10−6 − 10−3 m. Consequently, the solitons can be observed in the real constructions of the size l ∼ 10 m and more. 2. Generation of a train of the localized waves. The initial excitation in the form of the wide impulse implies formation of the sequence of solitons. The evolution of the rectangular impulse for ∆ = 20, F = −10−2 is reported in Fig. 6.7. “High” solitons have smaller width and are propagated faster than “low” solitons. Both numerical and analytical solutions of the stationary localized waves of various amplitude and width are in a good agreement (see Fig. 6.8).

Figure 6.7 Evolution of the “wide” impulse of compression [reprinted with permission from Elsevier].

Formation of Localized Nonlinear Waves in Layered Composites

109

Figure 6.8 Stationary localized waves for t = 4800; numerical/analytical solution are denoted by solid/dashed curve, respectively [reprinted with permission from Elsevier].

3. Scattering of an initial impulse of tension. Impulse of tension ∆ = 5, F = 10−2 does not imply formation of the localized waves. Instead, we observe the scattering of energy, which yields the delocalization of the initial excitation (Fig. 6.9). The reported results are in the agreement with conclusion carried out in section 4 while analyzing the analytical solution for the material with nonlinearity where only localized waves of compression are propagated. The results obtained in this section are also in a qualitative agreement with the results reported by Porubov [370] and Samsonov [398] regarding properties of the localized nonlinear waves propagating in solid bodies. It should be also pointed out that we illustrated here the phenomena associated with occurrence of the structural dispersion caused by non-homogeneity of the internal microstructure of the composite materials. The obtained solutions allow to establish a dependence between parameters of the microstructure and characteristics of nonlinear waves of deformation which are propagated in materials on the macrolevel.

110

Linear and Nonlinear Waves in Microstructured Solids

Figure 6.9 Delocalization of the initial impulse of tension [reprinted with permission from Elsevier].

Localization in 7 Vibration 1D Linear and Nonlinear Lattices: Discrete and Continuous Models This chapter deals with the localization of vibrations in one-dimensional linear and nonlinear lattices. The vibration localization can occur in the case of inhomogeneity under the following conditions: (i) the frequency spectrum of the periodic structure includes stopbands (ii) a perturbation of periodicity is present, and (iii) the eigenfrequency of the perturbed element falls into a stopband. Under these conditions, the energy can be spatially localized in the vicinity of the defect with an exponential decay in the infinity. The influence of nonlinearity can shift frequency into the stopband zone. The localization frequencies are determined and the attenuation factors are calculated. Discrete and continuous models are developed and compared. The limits of the applicability of the continuous models are established. Analysis of the linear problem has allowed a better understanding of particular features of the nonlinear problem and has led to developing a new approach for the analysis of nonlinear lattices alternative to the method of continualization.

7.1

INTRODUCTION

The effect of spatial localization of oscillations plays an important role in dynamics of materials and structures. Local perturbation of properties of the dynamical system (presence of defects, cracks, holes, inclusions, etc.) leads to concentration of energy. Under certain conditions it may cause localized modes in form of standing waves with zero group velocity. In this case all the energy is concentrated in the vicinity of the perturbed element and decays exponentially with distance from it. A nonlinearity of the system can cause a similar effect on its behavior leading to localized vibrations [441]. Localization of vibrations can lead to local loss of stability of structures and result in their failure. At the same time, this effect allows the designer to control the distribution of dynamic loads that can be used to create the vibration dampers and to reduce the vibration amplitude in the most critical parts of the system. Localized modes play an important role in the acoustic diagnostics methods, which are used to detect various defects. Localization effects in homogeneous and near-homogeneous structures are investigated in [218, 280]. The problems of localization of oscillations in linear and 111

112

Linear and Nonlinear Waves in Microstructured Solids

nonlinear mass lattices are reviewed in [295], where attention is paid to the construction of asymptotic solutions in the continuous approximations. Homogenization and high-frequency asymptotics are used to describe localization in one-dimensional lattices in [131, 339]. Problems of localization of oscillations in two-dimensional lattices are considered in [127]. Mode localization phenomenon in infinite periodic or bi-periodic mass-spring systems with disorders was investigated in [104, 106] using so-called U-transformation method. This method is based on the expansion normal mode. Many authors used Green’s functions to describe the effect of localization. The vibrational spectra of the defected polymers are analyzed in [254]. Localizations in the linear continuous systems with defects (beam and plate on an elastic foundation; non-uniform strings, rods and beams), as well as in discrete systems (a discrete lattice on a discrete elastic foundation; bi-periodic discrete lattice) are studied in [324]. The perturbation method was used in [363] to analyze the localization of vibrations in irregular structures.

7.2

MONATOMIC LATTICE WITH A PERTURBED MASS

The spectrum of infinite lattice in linear approximation does not contain localized modes because of symmetry restrictions. Such a solution can be valid for the lattice with broken symmetry. The detailed analysis of the influence of symmetry breaking on the vibration localization of lattice is given in [299–301]. Periodic systems are sensitive to certain types of periodically-breaking disorder, resulting in a phenomenon known as mode localization. Localization of periodic oscillations in a discrete system implies that some amplitude substantially exceed the rest. As a result the energy of the system is found to be predominantly confined on such a part [441]. The majority of existing studies of this phenomenon relate to linear systems; in particular, it was shown that in a linear regular system localization can occur when weak perturbations of the periodicity are introduced [104].

Figure 7.1 Monatomic lattice with a perturbed mass [reprinted with permission from Springer Nature].

Consider a monatomic lattice in which the mass of an element n = 0 differs from all the other elements and is equal to m0 , while masses of all other elements are equal to m1 , see Fig. 7.1. The equations of motion are m0 u¨0 + k (2u0 − u1 − u−1 ) = 0,

(7.1)

m0 u¨0 + k (2u0 − u1 − u−1 ) = 0.

(7.2)

113

Vibration Localization in 1D Linear and Nonlinear Lattices

We seek a spatially localized solution in the following form: u0 = A0 eiωt ,

un = A1 e−α|n| eiβ n eiωt ,

n = ±1, ±2, ...,

(7.3)

where α is the coefficient of localization, α > 0. Conditions for existence of solution (7.3) and the numerical values of its parameters are determined from the compatibility conditions for equations of motion. Substituting Eq. (7.3) into Eqs. (7.1) and (7.2), we obtain −m0 ω 2 A0 + 2k[A0 − e−α cosh(iβ )A1 ] = 0, −m1 ω 2 A1 + k(2A1 − A0 eα e−iβ − A1 e−α eiβ ) = 0, −m1 ω 2 A1 + k(2A1 − A0 eα eiβ − A1 e−α e−iβ ) = 0,

(7.4) n = 1,

(7.5)

n = −1,

(7.6)

−m1 ω 2 + k(2 − e−α eiβ − eα e−iβ ) = 0,

n ≥ 2,

(7.7)

−α −iβ

n ≤ −2.

(7.8)

2

−m1 ω + k(2 − e

e

α iβ

− e e ) = 0,

From Eqs. (7.5), (7.7) or (7.6), (7.8) we find A0 = A1 , and from Eqs. (7.7), (7.8) we obtain sinh(iβ ) = 0. Hence, β = 0 or β = π. The first root corresponds to a trivial solution ω = 0 and can be discarded. For β = π we obtain a perturbed π waveform un = (−1)n A1 e−α|n| eiωt .

(7.9)

Equations (7.4) and (7.7) for β = π allow to determine the coefficient of localization: 1−δ , (7.10) α = ln 1+δ where δ = m0 /m1 − 1 is a dimensionless parameter that determines the degree of disturbance. Vibration localization is possible only if α > 0, and therefore Eq. (7.9) yields: −1 < δ < 0. Otherwords, localization is possible only for the perturbed mass which is smaller than other masses. For small values of δ we obtain α ≈ −2δ .

(7.11)

From Eq. (7.7) we find the frequency at which the localization takes place ω2 2 = . 1−δ2 ω12

(7.12)

The numerical results are shown in Figs. 7.2 and 7.3. Decreasing√ mass m0 leads to a shift in the frequency of localization to the stop band zone: ω > 2ω1 .

114

Linear and Nonlinear Waves in Microstructured Solids

Figure 7.2 Frequency of localization in the monatomic lattice [reprinted with permission from Springer Nature].

Figure 7.3 Coefficient of localization in the monatomic lattice [reprinted with permission from Springer Nature].

7.3

MONATOMIC LATTICE WITH A PERTURBED MASS – THE CONTINUOUS APPROXIMATION

The basic equations in the framework of envelope continualization approximation (semi discrete approach) [247, 250] and section 10.5 can be written as follows m1 utt± + 4ku± + kh2 u± xx = 0,

(7.13)

u+ = u− = u,

(7.14)

at x = 0, u+ (x,t),

− kh(u+ x − ux ) = −δ m1 utt . u− (x,t) describe the envelope

(7.15)

Here, functions of the saw-tooth vibrations to the right and from the left of zero, respectively, and h is the distance between the masses. The solution is sought in the form u± = C± e−α|x| eωt ,

(7.16)

Vibration Localization in 1D Linear and Nonlinear Lattices

where

115

r

m1 ω 2 − 4k . kh2 Equation (7.14) yields C+ = C− . Assume that α=

m1 ω 2 = 4k + ω12 ,

ω12 2.

(8.14)

Figure 8.3 Layered composite with a defect unit cell (shaded) [reprinted with permission from John Wiley and Sons].

Now let us suppose that the layered composite has a defect unit cell (Fig. 8.3). For the determination of the localization wave number k one has the following condition: 2 cos(k(1) l (1) ) cos(k(2) l (2) ) − sin(k(1) l (1) ) sin(k(2) l (2) )[

(λ (2) + 2µ (2) )k(2) + (λ (1) + 2µ (1) )k(1)

(λ (1) + 2µ (1) )k(1) ] = ±2. (λ (2) + 2µ (2) )k(2)

(8.15)

From Eq. (8.15) one obtains: k = 0, π/l . Dispersion equation for the defect unit cell is used for the determination of the localization frequency ω ∗ : tr(T∗ ) = ±2

at k = 0,

where T∗ is the transfer matrix for the defect cell.

π/l ,

(8.16)

134

Linear and Nonlinear Waves in Microstructured Solids

In the case of the wave localization, the solution for the whole structure can be written as follows: u = U0 exp [i (k + iα) x] exp(iω ∗t), (8.17) where α is the attenuation factor. Dispersion equation for the regular unit cell is used for the determination of α: exp [i (k + iα) l] = Λ1,2

at ω = ω ∗ .

(8.18)

Figure 8.4 Wave localization at the beginning of the 1st stop band induced by the decrease of density of the defect cell: a) localization frequency, b) attenuation factor [reprinted with permission from John Wiley and Sons].

Figure 8.5 Wave localization at the end of the 1st stop band induced by the increase of density of the defect cell: a) localization frequency, b) attenuation factor [reprinted with permission from John Wiley and Sons].

Let us consider the results of calculation of Eqs. (8.16), (8.18) for the steelaluminium composite characterized by the following values of the parameters: the volume fractions c(a) = l (a) /l of the components are the same c(1) = c(2) = 0.5, the elastic coefficients λ (1) + 2µ (1) = 112 GPa and λ (2) + 2µ (2) = 275 GPa, the mass densities ρ (1) = 2700 kg/m3 and ρ (2) = 7800 kg/m3 . We will study an influence of different parameters of the defect cell on the wave localization. Firstly, we consider perturbation of the density of the defect cell:

Spatial Localization of Linear Elastic Waves in Composite Materials with Defects

135

Figure 8.6 Wave localization at the beginning of the 1st stop band induced by the perturbation of the volume fraction of an inclusion: a) localization frequency, b) attenuation factor [reprinted with permission from John Wiley and Sons].

Figure 8.7 Wave localization at the end of the 1st stop band induced by the perturbation of the volume fraction of an inclusion: a) localization frequency, b) attenuation factor [reprinted with permission from John Wiley and Sons].

ρ (2)∗ = ρ (2) (1 − δ ), ρ (2)∗ < ρ (2) . The parameter δ ≤ 1 characterizes the measure of perturbation. Numerical results depicted in Fig. 8.4 show that decrease in mass density ρ (2) induces localization at the beginning of the 1st stop band with ω > ωSB . Here and in the sequel ω0 denotes the frequency of the original perfectly periodic structure; ωSB denotes the frequency of the first stop band. Increase in mass density ρ (2) (ρ (2)∗ = ρ (2) (1 + δ ), ρ (2)∗ > ρ (2) ) induces localization at the end of the 1st stop band (Fig. 8.5) with ω < ωSB . Perturbation of the volume fraction of inclusions leads to the localization at the beginning of the 1st stop band with ω > ωSB (Fig. 8.6) or at the end of the 1st stop band with ω < ωSB (Fig. 8.7). The volume fractions of the components of defect cell are defined as c(1)∗ , c(2)∗ (c(1)∗ + c(2)∗ = 1).

136

Linear and Nonlinear Waves in Microstructured Solids

8.3

WAVE LOCALIZATION IN A LAYERED COMPOSITE MATERIAL: LATTICE APPROACH

The transfer-matrix method allows the exact solution, but it is focused on the use of a computer. In this section we construct an approximate analytical solution. For this aim we replace the layered composite (Fig. 8.1) to the diatomic chain (Fig. 8.8) according to the scheme described in [326]. Dispersion relation for 1D composite (8.12) can be written as follows ξ2 +1 sin Ω sin(Ωτ), 2ξ r √ (i) (i) (λ (1) +2µ (1) )ρ (1) l (2)C1 ωl (1) where Ω = C1 , τ = l (1)C , ξ = √ (2) , Ci = λ ρ+2µ . (i) (2) (2) cos(kl) = cos Ω cos(Ωτ) −

2

(λ

+2µ

(8.19)

)ρ

Figure 8.8 Diatomic lattice [reprinted with permission from John Wiley and Sons].

From the physical point of view, it is clear that the dynamics of layered composite with narrow rigid layers (ξ >> 1, τ ωSB (Fig. 8.10) as well as at the end of the 1st stop band with ω < ωSB (Fig. 8.11).

Vibrations of 9 Nonlinear Viscoelastic Heterogeneous Solids of Finite Size: Internal Resonances and Modes Interactions In this chapter, nonlinear vibrations of a layered viscoelastic solid are studied. A macroscopic wave equation taking into account the properties of the microstructure is proposed. Through use of the developed model, the interplay between the effects of nonlinearity and dissipation is analyzed. It gives possibility to predict how viscous damping influences modes coupling and to justify truncation of the original infinite system to a finite number of the leading order modes. The interaction between the effects of nonlinearity and dissipation is also investigated. We have found that in the case of a purely elastic material, an infinite number of the vibration modes may be coupled by nonlinear internal resonances. This results in periodic energy transfer between different modes and in a self-generation of higher-order modes. Hence, truncation to the modes having non-zero initial energy is prohibited.

9.1

INTRODUCTION

Real materials and structures are never perfectly elastic. In dynamical problems, part of the mechanical energy is always transformed to heat because of the internal friction. Dissipative behavior of heterogeneous solids can be determined by various factors, such as properties of the components, features of the microstructure, bonding conditions at the ”matrix-inclusion” interface, and so on [62, 158, 304, 369]. In this chapter we address the issue when energy dissipation is caused by the viscoelasticity of the components, which is typical, for example, for polymer-based materials. Viscoelastic properties of the medium can be governed by the well-known KelvinVoigt model (see, for example, [177]). In hydrodynamics, it corresponds to the classical behavior of a viscous gas, where shear stresses are proportional to the deformation rates and the proportionality coefficients are determined by the gas density. For solids, the Kelvin-Voigt model can be naturally deduced from a lattice-type model through passing to the continuous limit and assuming that the interaction forces between neighboring particles depend on the rate of the distance change rather than on the distance itself [304].

141

142

Linear and Nonlinear Waves in Microstructured Solids

Palmov [343,344] studied nonlinear vibrations of semi-infinite and finite rods subjected to a dissipation. He employed the method of harmonic linearization, which gave first-order approximation coinciding with the Rayleigh-Ritz approach. Equations in slow variables were obtained and analyzed. High-frequency deformations of nonlinear rate dependent materials induced by the propagation of transient waves were considered by Varley and Rogers [445] and Seymour and Varley [404]. Mortell and Varley [323] discussed nonlinear elastic waves in finite-size bodies and studied the dynamic response of a viscoelastic rod subjected to a pulse load [322]. In the first-order approximation, the solution was developed as a superposition of two modulated waves travelling in opposite directions and not interacting with each other. Vibrations of continuous structures can be described by dynamical systems having infinite number of degrees of freedom. Nonlinearity leads to localization of energy and its transfer from the low- to the high-frequency part of the spectrum, and vice versa. The vibration modes can then be involved in complicated interactions, resulting in internal resonances and self-generation of higher-order modes. In such a case, truncation to the modes having non-zero initial energy (which is usually applicable in linear problems) is not possible and all the resonant modes should be taken into account. The effects of mode coupling and internal resonance have attracted the considerable attention of many authors. A number of results were obtained for vibrations of homogeneous structures and numerical [383] as well as asymptotic [24, 84, 85, 293, 331] approaches have been widely applied. However, the non-linear dynamic behavior of heterogeneous solids was studied to a significantly less extend. Only recently, one-dimensional vibrations of microstructured rods were considered by Andrianov et al. [21] in regard to a nonlinear elastic external medium and geometrical and physical non-linearity. Heterogeneity results in dispersion of energy and, thus compensates the influence of nonlinearity. As the spatial period of the modes decreases and approaches the size of the microstructure, internal resonances are suppressed and truncation to only a few leading order modes can be justified. It should be noted that dissipation restrains energy transfers between the vibration modes and on a large time scale modes coupling vanishes. In that sense, dispersion and dissipation acting in a nonlinear system may lead to qualitatively similar physical consequences (Zabusky and Kruskal [468] encountered this analogy analysing the FPU problem, see also [456]).

9.2

INPUT PROBLEM AND HOMOGENIZED DYNAMICAL EQUATION

Let us consider a heterogeneous solid consisting of periodically repeated viscoelastic layers Ω(1) and Ω(2) (Fig. 9.1). We shall study natural longitudinal vibrations in the direction x. This model can describe the properties of laminated composite materials, phononic crystals and acoustic diodes (see, for example, references [217, 282, 317]). Notice that layered structures are employed in band gap engineering for the design of vibration and sound control devices [216]. The mechanical behavior of each of the layers Ω(i) is described by the KelvinVoigt model [177], which includes a purely elastic spring connected in parallel with

Nonlinear Vibrations of Viscoelastic Heterogeneous Solids of Finite Size

143

Figure 9.1 Periodically heterogeneous solid under consideration [reprinted with permission from Elsevier].

a viscous dashpot. The properties of the dashpot are assumed to be linear, while the spring exhibits nonlinear response. Geometric nonlinearity is taken into account using the Cauchy-Green strain tensor and physical nonlinearity is modeled with the help of the Murnaghan elastic potential (see Chapter 4.1). The time dependent longitudinal stress σ (i) is given by

σ

(i)

=α

(i) (i) ∂ u

β (i) + ∂x 2

∂ u(i) ∂x

!2 + ν (i)

∂ 2 u(i) , ∂ x∂t

(9.1)

where u(i) is the displacement; α (i) and β (i) are the elastic coefficients; α (i) = λ (i) + 2µ (i) , λ (i) , µ (i) stand for the Lam´e elastic constants; β (i) = 3 λ (i) + 2µ (i) + 2 A(i) + 3B(i) +C(i) , A(i) , B(i) , C(i) are the Landau elastic constants; ν (i) is the viscosity. Here and in the sequel the upper indexes (i), i = 1, 2, refer to the different components Ω(1) , Ω(2) of the medium. The governing dynamical equation is as follows ∂ ∂ 2 u(i) ∂ u(i) ∂ 2 u(i) ∂ 2 u(i) + β (i) = ρ (i) , α (i) + ν (i) 2 2 ∂t ∂x ∂x ∂x ∂t 2

(9.2)

where ρ (i) is the mass density. At the interface ∂ Ω, we assume the conditions of perfect bonding that imply continuity of the displacement and stress fields: u(1) = u(2) ,

σ (1) = σ (2)

at ∂ Ω.

(9.3)

Let us suppose the characteristic size l of the microstructure to be essentially smaller than the spatial period Ln of a considered vibration mode. Then the input problem (9.2), (9.3) can be replaced by a homogenized dynamical equation of the

144

Linear and Nonlinear Waves in Microstructured Solids

following form ∂ ∂ 2u ∂ u ∂ 2u ∂ 2u hαi + hνi + hβ i = hρi , ∂t ∂ x2 ∂ x ∂ x2 ∂t 2

(9.4)

where u is the macroscopic displacement field and h·i denotes the homogenized (so called effective) properties of the medium. Equation (9.4) presents the leading order O η 0 approximation, where η = l/L 1 is the natural small parameter. We notice that taking into account higherorder terms in powers of η will lead to additional high-gradient terms in equation (9.4), which describe dispersion of the vibration energy by the microstructure. Higher-order homogenized models have been considered in Chapter 4.3. In this chapter we focus on dissipation and, for the sake of clarity, restrict the carried out analysis to the O η 0 approximation only. The effective mass density ρ is given by a simple rule of mixture: hρi = c(1) ρ (1) + (2) c ρ (2) , where c(i) are the volume fractions of the components, c(i) = l (i) /l. In the first approximation, the elastic and the viscous properties can be homogenized independently of each other. This simplified procedure may provide a reasonable approach if nonlinearity and viscosity are small. The effective elastic coefficients hαi and hβ i are evaluated as follows Chapter 4.3: α (1) α (2) , c(1) α (2) + c(2) α (1) 3 3 c(1) β (1) α (2) + c(2) β (2) α (1) hβ i = . 3 c(1) α (2) + c(2) α (1) hαi =

(9.5)

(9.6)

In order to determine the effective viscosity hνi, let us apply to equations (9.2), (i)

R∞

(9.3) the Laplace transform us (x, s) = u(i) (x,t) exp (−st) dt. Assuming zero initial 0

conditions, in the linear approximation we obtain ∂ 2 u(i) s (i) α (i) + sν (i) = s2 ρ (i) us , ∂ x2 ∂ u(1) ∂ u(2) s s α (1) + sν (1) = α (2) + sν (2) ∂x ∂x Homogenization of the problem (9.7), (9.8) gives [306] (1)

(2)

us = us ,

(9.7)

at ∂ Ω.

(9.8)

∂ 2 us (i) = s2 hρius , (9.9) ∂ x2 h i−1 where α + sν = c(1) / α (1) + sν (1) + c(2) / α (2) + sν (2) . Application of the inverse Laplace transform leads to an integro-differential equation, which complicates significantly further analysis. To avoid this, in the case of hα + sνi

Nonlinear Vibrations of Viscoelastic Heterogeneous Solids of Finite Size

145

small viscosity we represent the homogenized parameter hα + sνi as the power series expansion 2 2 (1) ν (1) α (2) (2) ν (2) α (1) (1) (2) c + c α α hα + sνi = (1) (2) +s + O s2 . 2 (2) (1) (1) (2) (2) (1) c α +c α c α +c α (9.10) Substituting (9.10) into (9.9) and inverting the transform, one obtains the linear part of the homogenized equation (9.4), where the effective elastic coefficient hαi is given by formula (9.5) and the effective viscosity hνi is obtained as follows 2 2 c(1) ν (1) α (2) + c(2) ν (2) α (1) . (9.11) hνi = 2 c(1) α (2) + c(2) α (1) Equation (9.4) describes the dynamic behavior of a heterogeneous solid on the macro scale associated with the spatial period of the vibration modes. We note that all the effective coefficients are determined explicitly in terms of the microscopic properties of the medium. This contrasts with many well-known phenomenological approaches like Cosserat’s [129] and Biot’s theories, where the material parameters are usually left undetermined.

9.3

DISCRETIZATION PROCEDURE

p Let us introduce the nondimensional variables x¯ = x (π/L), t¯ = t (π/L) α/ρ, u¯ = u/A, where L is the length of the entire heterogeneous solid and A is the vibration amplitude. For the simplicity, the overbars are omitted in the sequel. Equation (9.4) takes the following form: ∂ 3u ∂ u ∂ 2u ∂ 2u ∂ 2u + γ + ε = 2, (9.12) ∂ x2 ∂ x2 ∂t ∂ x ∂ x2 ∂t p where γ = πhνi/ L hαihρi , ε = πAhβ i/ (Lhαi) are the non-dimensional small parameters characterizing viscosity and nonlinearity. The coefficient γ is always positive, whereas the sign of ε depends on the physical properties of the medium. For the most of materials (e.g., metals, polymers, stones) we have hβ i < 0 and ε < 0, which results in a soft nonlinearity. A hard nonlinearity, hβ i > 0, ε > 0, can be observed for elastomers and rubber-like materials. Equation (9.12) represents an asymptotic model, which accounts the case of small viscosity and small nonlinearity. That is why the damping term is considered in a linear form and the nonlinear term is purely elastic. A refined model may include a coupled damping and nonlinear term of the order O (γε). However, supposing γε → 0, we can asymptotically neglect it in the present approximation. Equation (9.12) may allow various modifications. Adding a dispersion term with the forth-order spatial derivative and neglecting the dissipative term setting γ = 0, we will obtain a version of the well-known Boussinesq equation that is widely used to

146

Linear and Nonlinear Waves in Microstructured Solids

study wave propagation in nonlinear heterogeneous media (see, for example, [306] and references therein). Similar models have been recently applied to describe nonlinear vibrations of finite size heterogeneous bodies [21, 456]. Employing two or three dispersion terms makes it possible to develop refined gradient models [74], which are applicable in a wider frequency range. Double- and triple-dispersion equations were used to predict the propagation of linear transient waves induced by pulse and harmonic loads [43, 126]. The governing dynamic model introduced in the particular form (9.12) is intended to study the interplay between nonlinear and dissipative effects, while the period of the vibration modes is considered to be essentially larger then the size of the microstructure. Let us consider a case of clamped-clamped edges. The boundary conditions are u(0,t) = u(π,t) = 0. (9.13) In order to solve the boundary value problem (9.12), (9.13), a discretization procedure is employed. Satisfying conditions (9.13), the displacement field is represented as a Fourier sine series expansion u(x,t) = q1 (t) sin(x) + q2 (t) sin(2x) + q3 (t) sin(3x) + ...

(9.14)

Substituting ansatz (9.14) into equation (9.12), we come to an infinite system of nonlinear ordinary differential equations dq1 d 2 q1 +γ + q1 + ε(q1 q2 + 3q2 q3 + 6q3 q4 + ...) = 0, dt 2 dt 2 q1 dq2 d 2 q2 + 4γ + 4q2 + ε + 3q1 q3 + 8q2 q4 + ... = 0, dt 2 dt 2 dq3 d 2 q3 + 9γ + 9q3 + ε(3q1 q2 + 6q1 q4 + ...) = 0, 2 dt dt dq4 d 2 q4 + 16γ + 16q4 + ε(6q1 q3 + 4q22 + ...) = 0, dt 2 dt ...,

(9.15)

which can be written in more general form reads d 2 qn dqn ε ∞ + n2 γ + n2 qn + ∑ m2 qm |m − n|q|m−n| − (m + n)qm+n = 0, (9.16) 2 dt dt 2 m=1 where n = 1, 2, 3, ... The obtained nonlinear system is non-symmetric with respect to the odd and even vibration modes. A simple analysis reveals two fundamentally different types of the mode interactions those described by Chechin and Sakhnenko [118]. An initial excitation of the odd modes leads necessarily to the appearance of even modes, i.e., equations (9.15) do not permit the solution q2n−1 6= 0, q2n = 0. The even modes undergo a so called ”force” excitation. On the other hand, the solution q2n−1 = 0, q2n 6= 0 is allowed and, in general, the presence of the even modes does not give

Nonlinear Vibrations of Viscoelastic Heterogeneous Solids of Finite Size

147

rise to the odd modes. However, vibrations by even modes appear to be unstable and a small perturbation of the initial conditions induces energy transfers to the odd modes [21]. In this case the odd modes are subjected to a ”parametric” excitation.

9.4

METHOD OF MULTIPLE TIME SCALES

We seek an asymptotic solution supposing nonlinearity to be small, |ε| 1. Let us introduce different time scales described by new independent variables t0 = t, t1 = εt, ..., and represent qn as an expansion in powers of ε: qn (t) = qn0 (t0 ,t1 ) + εqn1 (t0 ,t1 ) + O(ε 2 ).

(9.17)

The number of required time scales depends on the order of approximation. We will carry out expansion (9.17) to O(ε 2 ), therefore, two time scales (”fast” t0 and ”slow” t1 ) are needed. The derivatives with respect to t are represented as follows ∂ ∂ d = +ε + O(ε 2 ), dt ∂t0 ∂t1

∂2 d2 ∂2 + 2ε = + O(ε 2 ). 2 dt 2 ∂t0 ∂t1 ∂t0

(9.18)

Splitting each equation of the system (9.15) in powers of ε, in the O(ε 0 ) approximation we obtain ∂ 2 qn0 ∂ qn0 + n2 qn0 = 0. (9.19) + n2 γ 2 ∂t0 ∂t0 The solution of equation (9.19) is qn0 = exp(−n2 γt0 /2)[an (t1 ) cos(ωnt0 ) + bn (t1 ) sin(ωnt0 )],

(9.20)

where ωn is the natural frequency of the nth mode in the linear case, ωn2 = n2 (1 − n2 γ 2 /4); an and bn are slow varying amplitudes. The O(ε 1 ) approximation of the system (9.15) gives: ∂ qn1 ∂ 2 qn1 + n2 γ + n2 qn1 = ∂t0 ∂t02 ∂ 2 qn0 ε ∞ 2 −2 − ∑ m qm0 |m − n|q|m−n|0 − (m + n)q|m+n|0 . ∂t0 ∂t1 2 m=1

(9.21)

A straightforward integration of the system (9.21) will induce secular terms in the expressions for qn1 . Secular terms infinitely grow in time, which is inconsistent with the physical properties of the conservative system under consideration. In order to eliminate secular terms, the coefficients of cos(ωnt0 ) and sin(ωnt0 ) in the r.h.s. of equations (9.21) must be equal to zero. Substituting (9.20) into (9.21) and expanding the products q j0 qk0 using the standard trigonometric identities, we obtain a system of equations for an and bn , which gives a possibility to investigate the interactions between different modes.

148

Linear and Nonlinear Waves in Microstructured Solids

In the non-dissipative case, γ = 0, the frequencies ωn become proportional to each other ω j /ωk = j/k. (9.22) Thus, an infinite number of modes are coupled by internal resonances. The presence of viscosity leads to a ”detuning” of relation (9.22) and, on a large time scale, prevents energy transfers between the vibration modes. Let us suppose viscosity to be small, γ 1, and represent cos(ωnt0 ) and sin(ωnt0 ) in expression (9.20) as follows n3 γ 2t0 sin(nt0 ) + O(n6 γ 4t02 ), 8 n3 γ 2t0 cos(nt0 ) + O(n6 γ 4t02 ). sin(ωnt0 ) = sin(nt0 ) − 8 cos(ωnt0 ) = cos(nt0 ) +

(9.23)

Truncating expansions (9.23) at leading order, we hold strictly the resonance condition (9.22). The physical sense of this approximation is that viscosity is considered to be responsible for energy dissipation (i.e., for exponential attenuation of qn0 ), but its influence on the natural frequencies is neglected and, thus, the internal resonances are not violated. The developed approach is applicable on a short time scale as n3 γ 2t0 /8 1. As follows from (9.20), the attenuation coefficient of the nth mode is proportional to n2 . We observe that the internal dissipation exhibits a quadratic growth with the increase of the mode number and, therefore, the lowest modes can be the most important in vibrations of real structures. Let us examine resonant interactions between modes 1 and 2. It is convenient to introduce the amplitude rn (t1 ) and the phase ϕn (t1 ) as follows: an = rn cos(ϕn ), bn = rn sin(ϕn ). Keeping the first two equations of system (9.21), the condition of elimination of secular terms gives: dr1 1 = r1 r2 exp(−2γt0 ) sin(ϕ2 − 2ϕ1 ), dt1 4 dϕ1 1 r1 = − r1 r2 exp(−2γt0 ) cos(ϕ2 − 2ϕ1 ), dt1 4 1 2 dr2 = − r1 exp(γt0 ) sin(ϕ2 − 2ϕ1 ), dt1 16 dϕ2 1 r2 = − r12 exp(γt0 ) cos(ϕ2 − 2ϕ1 ). dt1 16

(9.24)

The solution of system (9.24) in the purely elastic case (γ = 0) was analyzed by Andrianov et al. [21]. We note that vibration by the single mode 1 is not possible. If all the initial energy is accumulated in mode 1, i.e. r1 (0) 6= 0, r2 (0) = 0, then the mode 2 is necessarily excited and a periodic energy exchange between the modes takes place. On the other hand, if we start with zero initial energy the mode 1, r1 (0) = 0, r2 (0) 6= 0, then dr2 /dt1 = dϕ2 /dt1 = 0. The amplitude r2 and the phase ϕ2 are constant in time, so the system can vibrate through mode 2 only. However,

Nonlinear Vibrations of Viscoelastic Heterogeneous Solids of Finite Size

149

this regime is not stable in the sense that even a small perturbation of the initial conditions will induce excitation of mode 1. The described behavior is illustrated in the phase plane (r2 , ϕ2 − 2ϕ1 ) (see Fig. 2 reported in [21]).

9.5

NUMERICAL SIMULATION OF THE MODES COUPLING

The distribution of energy among the vibration modes can be determined using a Lagrangian formalism. Let us introduce a generalized equation of motion for the n-th mode as follows ∂T ∂T ∂V dqn d , (9.25) − =− − n2 γ dt ∂ (dqn /dt ∂ qn ∂ qn dt where T is the kinetic and V is the potential energy of the whole system. Integrating equations (9.15), we obtain T= ( Z 1 ∞ V = ∑ n2 q2n + ε 2 n=1

∞

∑

1 ∞ ∂ qn 2 ∑ ∂t , 2 n=1

) m qm |m − n|q|m−n| − (m + n)qm+n dqn . 2

(9.26)

(9.27)

m=1

The term (∂ qn /∂t)2 in expression (9.26) and the term n2 q2n in expression (9.27) contribute to the nth equation of system (9.15). Then, in the leading order approximation and omitting the coefficient 1/2, the total energy En of the nth mode can be evaluated as follows dqn 2 + n2 q2n + O(ε). (9.28) En = dt The second term in expression (9.27) represents a correction of order O(ε) to the potential energy V . It can include products qm q|m−n| and qm qm+ and, thus, its contribution is shared between modes m, |m − n| and m + n. Below we are restricted by the O(ε 0 ) approximation and calculate the energy by formula (9.28). The numerical examples are presented for the case of soft nonlinearity, which is typical for the most industrial materials, and ε = −0.1. The increase in the magnitude of ε makes the energy transfers faster, however, the qualitative behavior of the solution remains the same. Numerical integration is performed by the Runge-Kutta fourth-order method in the open-source CAS Maxima. Practical convergence is verified by decreasing twice the step of integration and checking that this does not affect the obtained numerical data. Firstly, let us consider a two mode approximation and compare the developed asymptotic approach (9.24) with the direct numerical integration of the two leading equations of the nonlinear system (9.15). The initial energy is assumed to be localized in mode 1. System (9.24) has a singularity at r2 = 0; to avoid this the initial

150

Linear and Nonlinear Waves in Microstructured Solids

conditions are taken as follows r2 = q2 = 0.01,

r1 = q1 =

dr1 dq1 dr2 dq1 = = = =0 dt dt dt dt

q 1 − 4r12 = 0.99979998,

(9.29)

at t = 0.

Fig. 9.2 displays a periodic energy exchange between modes 1 and 2. The asymptotic approximation of the method of multiple time scales is formally applicable at a relatively short time scale t ∼ O(ε −1 ). However, it is numerically useful far beyond their nominal range of validity. Next, let us examine interactions between the

a)

b)

c)

d)

Figure 9.2 Energy exchange between the two leading modes (solid curves - numerical solution, dotted curves - asymptotic solution): (a) γ = 0 (non-dissipative case), (b) γ = 0.0005, (c) γ = 0.001, (d) γ = 0.002 [reprinted with permission from Elsevier].

six leading modes. The initial conditions correspond to the case when all the input energy is localized in the mode 1: q1 = 1,

qk = 0,

k = 2, ..., 6,

dqn = 0, dt

n = 1, ..., 6

at t = 0.

(9.30)

Fig. 9.3 presents the results of the numerical integration of system (9.15) truncated with n = 1, ..., 6. We observe that the increase in dissipation suppresses energy

Nonlinear Vibrations of Viscoelastic Heterogeneous Solids of Finite Size

a)

b)

c)

d)

151

Figure 9.3 Energy transfers between the six leading modes: (a) γ = 0 (non-dissipative case), (b) γ = 0.0005, (c) γ = 0.001, (d) γ = 0.002 [reprinted with permission from Elsevier].

transfers and makes it possible to truncate the original infinite system to only a few leading order modes.

9.6

CONCLUDING REMARKS

We studied natural vibrations of a heterogeneous solid consisting of periodically repeated layers of two different materials. The viscoelastic properties of the components were represented by the Kelvin-Voigt model. Geometric nonlinearity was introduced by the Cauchy-Green strain tensor and physical nonlinearity was modeled employing the Murnaghan elastic potential. The characteristic size of the microstructure (e.g., length of the unit cell) was supposed to be essentially smaller than the scale of the macroscopic problem (e.g., spatial periods of the vibration modes). A homogenized dynamical equation was proposed to describe the dynamic properties of the medium on the macro level. An important contribution of the chapter is that the coefficients of the homogenized equation were determined explicitly basing on rigorous theoretical origins. The developed macroscopic model encapsulate information about the properties of the microstructure.

152

Linear and Nonlinear Waves in Microstructured Solids

Using a Fourier series expansion, the input continuous problem was discretized and reduced to an infinite system of nonlinear ordinary differential equations. An asymptotic solution was developed by the method of multiple time scales and numerical simulations performed by the fourth-order Runge-Kutta method. The obtained numerical and analytical results exhibit good agreement. If the viscosity increases, the dissipation suppresses the influence of nonlinearity. The energy transfers between the vibration modes are restricted and, on a large time scale, mode coupling vanishes. The attenuation coefficient of the nth mode is proportional to n2 , so internal dissipation exhibits a quadratic growth with increase of the mode number. In such a case, truncation of the original infinite system at only a few leading order modes can provide a reasonable approximation. Despite, from the mathematical point of view, an infinite number of modes are involved in nonlinear interactions, we have shown that for real structures even a considerably small viscosity makes it possible to employ approximate models with only a few degrees of freedom.

Gradient and 10 Nonlocal, Local Models of Elastic Media: 1D Case This chapter deals with local/nonlocal and gradient one-dimensional models of elastic media. First, modeling of a lattice of elastically couple particles is considered. Second, the classical continuous approximations of a discrete problem is illustrated and discussed. Next, splashes, envelope continualization and intermediate continuous models are described and investigated. Benefits of the use of the Pad´e approximations for the construction of continuous models are outlined. Normal modes expansion and theories of elasticity with couple-stresses are revisited. Then, the correspondence between functions of discrete arguments and continuous systems as well as relations between the kernels of integro-differential equations of the discrete and continuous systems are outlined. Moreover, the following topics are discussed: dispersive wave propagation, Green function, double-dispersive equations, Toda lattices, discrete kinks, continualization of the Fermi-Pasta-Ulam lattice, anticontinuum limit and 2D lattices. Finally, the problems regarding molecular dynamics vs. continualization, continualization vs. discretization, as well as opened problems are addressed.

10.1

INTRODUCTION

Over the last few years, a number of new materials and designs have appeared that require more sophisticated research than the capabilities of a classical continuous media. There are, in particular, ultra dispersive and nanocrystalline materials [137, 195, 355]. The nanocrystalline material is represented by a regular or quasi-regular lattice of granules, fullerenes, nanotubes, carbon nanostructures, etc. and possesses internal degrees of freedom [374]. This situation is also usual for various problems of nanomechanics [217], because correct description of the mechanical properties of nanomaterials required taking into account size effects. Models based on a classical continuous media cannot govern high frequency vibrations, material behavior in the vicinities of cracks and on the fronts of destruction waves, and during phase transitions [340]. It is not possible to reach bifurcation points, i.e., thresholds of lattice stability under catastrophic deformations [6]. Wave dispersion in granular materials [354, 375] represents an important example of microstructure effects too. Microstructural effects are essential for correct description of softening phenomena [356] in damage mechanics [41, 115, 136] and in the theory of plasticity [174, 384]. Do not forget also problems of biomechanics and molecular biology. As it is mentioned in [237], “From the behavior of calcium waves in living cells 153

154

Linear and Nonlinear Waves in Microstructured Solids

to the discontinuous propagation of action potentials in the heart or chains of neurons and from chains of chemical reactors or arrays of Josephson junctions to optical waveguides, dislocations and the DNA double strand, the relevant models of physical reality are inherently discrete”. Acoustic (or mechanical) metamaterials, i.e. cellular periodic structures, only in the long wavelength range behave like continuous materials. The study of manifestations of discreteness, dispersion, dissipation and nonlinearity of acoustic waves in metamaterials is not only of theoretical interest. It is also about the prospects of practical applications of metamaterials [137, 183, 476], for example, the creation of super-absorbers of sound. Discrete lattice-type models are widely used to describe vibrations in crystals, in foams, in cellular structures and bone tissues. Some novel applications include modeling of polymer molecules, atomic lattices (e.g., graphene). Discrete models can also appear in engineering, e.g., for simulating lightweight truss structures with attached masses. In contrast to continuous media, discrete lattices sometimes allow evaluation of exact dispersion relations in a closed analytical form, which is convenient for further analysis. That is why they can be considered as benchmark models to highlight the main effects of the wave propagation in heterogeneous structures. The effects mentioned may be analyzed within the frame of discrete models, using molecular dynamics [255], quasicontinuum analysis [426, 455] or other numerical approaches. However, a sought result is difficult to obtain using high tech computers in an economical way. For example, modern practical problems are still intractable for molecular dynamics, even if the most powerful computing facilities are used. Situation can be described by Dirac’s words [138]: “The physical laws necessary for the mathematical theory of a large part of physics and whole of chemistry are thus completely known, and the difficulty is only that the exact application of these laws leads to equations much too complicated to be solvable. Therefore, it becomes desirable that approximate practical methods of applying quantum mechanics should be developed, which can lead to an explanation of the main features of complex atomic systems without too much computations”. Hence, refinement of the existing theories of continuous media for the purpose of more realistic predictions of mechanical properties seems to be the actual goal. The most challenging problems in multiscale analysis is that of finding continuous models for atomistic lattice starts from the first principles. In statistical physics, these question as already addressed 100 years ago. Most important is the question how to obtain irreversible thermodynamics as a macroscopic limit from microscopic models that are reversible. Recently, a certain progress has been outlined in solving these problems [288, 471], but it is still far from the final conclusions. The purpose of this chapter is much more modest than the global tasks described above. On simple models, we consider various ways of obtaining models of intermediate complexity between classical continuous and discrete ones. Here the following strategies exist.

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case

155

(i) Phenomenological approach. Additional terms are added to the energy functional or to the constitutive relation. The structure and character of these terms are postulated in references [8, 204, 307]. Phenomenological approach is useful in the applied sciences when it is necessary to solve problems of practical significance. However, the range of applicability of these approaches is usually unknown, and the basic pecularities of behavior of discrete systems remain unclear. (ii) Statistical approach. Starting from an continuous inhomogeneous theories it is aimed to obtain refined (e.g. couple-stress) theories of homogeneous continuum [73]. We know only two work in which this idea is brought to concrete results [291, 292]. In these papers polycrystal are considered as a micro-inhomogeneous elastic medium, which consists of homogeneous anisotropic crystallites with random orientation. It is shown that the elastic energy density of the polycrystalline medium depends non-locally on the non-uniform field of average deformations. In the case of smooth fields of average deformations it could be considered that the energy density locally depends not only on the values of deformations, but also on the values of their derivatives. This dependence in the isotropic case is characterized by five gradient modules, in addition to the two elastic moduli of the classical theory of elasticity. For the first time, explicit expressions are obtained for the gradient modules of polycrystalline materials. (iii) Homogenization and continualization approaches [20, 28, 39, 40, 43, 80, 81, 94,236–238,257–259,353,382]. They are based on various approximations of nonlocal (discrete, pseudodifferential, integral) operators by the local (differential) ones. This part of book is devoted to the continualization approaches and their features.

10.2

A CHAIN OF ELASTICALLY COUPLED MASSES

In this Section we follow paper [329]. We study a chain of n + 2 material points with the same masses m, located in equilibrium states in the points of the axis x with coordinates jh ( j = 0, 1, ..., n, n + 1) and suspended by elastic couplings of stiffness c (Fig. 10.1).

Figure 10.1 A chain of elastically coupled masses.

Owing to the Hooke’s law the elastic force acting on the j-th mass is as follows σ j (t) = c[y j+1 (t) − y j (t)] − c[y j (t) − y j−1 (t)] = c[y j−1 (t) − 2y j (t) + y j+1 (t)], j = 1, 2, ...., n,

(10.1)

156

Linear and Nonlinear Waves in Microstructured Solids

where y j (t) is the displacement of the j-th material point from its static equilibrium position. Applying the second Newton’s law one gets the following system of ODEs governing chain dynamics my jtt (t) = c[y j−1 (t) − 2y j (t) + y j+1 (t)],

j = 1, 2, ...., n.

(10.2)

This system of ODEs is called Lagrange lattice, because Lagrange studied it in his “Analytical Mechanics” [267]. Sometimes one can read term “Newton lattice” [98], referring to Principia (livre II, proposition XLIX), however, this section of Principia contains only some general discussions about the speed of sound. In fact, the ODEs (10.2) were appeared only in Lagrange book. System (10.2) can be recast into the following form: mσ jtt (t) = c(σ j+1 − 2σ j + σ j−1 ),

j = 1, ..., n.

(10.3)

Let the chain ends be fixed y0 (t) = yn+1 (t) = 0.

(10.4)

In general, the initial conditions have the following form: (0)

y j (t) = ϕ j ,

(1)

y jt (t) = ϕ j

at t = 0.

(10.5)

As it has been shown in [329], for any solution of the BVP (10.2), (10.4), (10.5) the total energy is constant. Besides, the solutions mentioned so far are not asymptotically stable due to the Lyapunov stability definition. A solution to the BVP (10.2), (10.4), (10.5) can be expressed by elementary functions applying the discrete variant of the method of variables separation. For this purpose normal vibrations are constructed in the form y j (t) = C j T (t),

j = 1, . . . , n,

(10.6)

where constants C j are defined via solution of the following eigenvalue problem −λC j = C j+1 − 2C j +C j−1 ,

j = 1, . . . , n,

C0 = Cn+1 = 0.

(10.7)

Function T (t) satisfies the following equation: mTtt + cλ T = 0.

(10.8)

Eigenvalues of the problem (10.7) follow [329] λk = 4sin2

kπ , 2(n + 1)

k = 1, 2, . . . , n.

(10.9)

A solution to Eq. (10.8) has the form T = A exp(iωt). Hence, Eqs. (10.8), (10.9) yield the following Lagrange formula for frequencies ωk of discrete system (10.3): r c kπ ωk = 2 sin , k = 1, 2, . . . , n. (10.10) m 2(n + 1)

157

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case

Since all values λk are distinct, then all eigenvalues are different. Therefore, each (k) (k) (k) of the eigenvalues is associated with one eigenvector Ck (C1 ,C2 , ...,Cn ) of the form: 2kπ nkπ kπ kπ , sin , ..., sin sin , k = 1, 2, . . . , n. (10.11) Ck = cosec n+1 n+1 n+1 n+1 Eigenvectors are mutually orthogonal, whereas |Ck |2 =

kπ n+1 cosec2 , 2 n+1

k = 1, 2, . . . , n.

(10.12)

Each of the eigenfrequencies (10.10) is associated with a normal vibration (k)

(k)

y j (t) = C j [Ak cos(ωk t) + Bk sin(ωk t)],

k = 1, 2, . . . , n.

(10.13)

A general solution of the BVP (10.3)–(10.5) is obtained as a result of superposition of normal vibrations n

y j (t) =

(k)

∑ Cj

[Ak cos(ωk t) + Bk sin(ωk t)],

j = 1, . . . , n.

(10.14)

k=1

Let us study now the problem of chain movement under action of a unit constant force on the point number zero. Motion of such system is governed by Eq. (10.3) with the following boundary and initial conditions σ0 (t) = 1,

σn+1 (t) = 0,

σ j (t) = 0, σ jt (t) = 0

at t = 0.

(10.15) (10.16)

In what follows the initial BVP with non-homogeneous BCs (10.3), (10.15), (10.16) will be reduced to that of homogeneous BCs for Eq. (10.3) with nonhomogeneous initial conditions, and then the method of superposition of normal vibrations can be applied. The formulas of normal forms obtained so far can be applied in a similar way with exchange of y j (t) for σ j (t). As result, the following exact solution to the BVP (10.3), (10.15), (10.16) is obtained [289, 329]: σj =

10.3

1 n πk j πk ∑ sin n + 1 ctg 2 (n + 1) [1 − cos(ωkt)], j = 1, 2, . . . , n. n + 1 k=1

(10.17)

CLASSICAL CONTINUOUS APPROXIMATIONS

For large values of n usually continuous approximation of discrete problem is applied. Let us introduce the continuous coordinate x scaled in such a way that x = nh at the nodes of the lattice, where h is the distance between the particles. Then classical continuous approximation for discrete model described by the Eqs. (10.3), (10.15), (10.16) takes the form mσtt (x,t) = ch2 σxx (x,t), (10.18)

158

Linear and Nonlinear Waves in Microstructured Solids

σ (0,t) = 1,

(10.19)

σ (l,t) = 0,

(10.20)

σ (x, 0) = σt (x, 0) = 0,

(10.21)

where l = (n + 1)h, σ (x,t) = chyx (x,t). Let us analyse BC (10.19). Using expression for force h2 ∂ 3 ∂ h ∂2 + + · · · y(x,t) σ0 (t) = c[y1 (t) − y0 (t)] = ch + ∂ x 2 ∂ x2 6 ∂ x3

(10.22)

and leaving the first term on the right-hand side of equation (10.22), we obtain the BC (10.19). BVP (10.18)–(10.22) can be used, for example, for modeling of stresses in couplings of the rolling stocks [261]. Having in hand a solution to continuous BVP (10.18)–(10.22), one obtains an approximate solution of a discrete problem due to the following formulas σ j (t) = σ ( jh,t),

j = 0, 1, ..., n, n + 1.

(10.23)

Formally, the approximation described so far can be obtained in the following way. Let us denote the difference operator occurring in Eq. (10.3) as D, i.e. mσ jtt (t) = cDσ (t). Applying the translation operator exp(h∂ /∂ x), one gets [319] ∂ ∂ ih ∂ 2 D = exp h + exp −h − 2 = −4sin − . ∂x ∂x 2 ∂x

(10.24)

(10.25)

Let us explain Eq. (10.25) in more details. The Maclaurin formula for infinitely differentiable function F(x) has the following form: ∂ ∂ 1 ∂2 F(x + 1) = 1 + + + · · · F(x) = exp F(x). (10.26) ∂ x 2! ∂ x2 ∂x Observe that exp(h∂ /∂ x) belongs to the so called pseudo-differential operators. Using relations (10.24)–(10.26), we cast Eq. (10.3) into pseudo-differential equation of the following form: ∂ 2σ ih ∂ m 2 + 4csin2 − σ = 0. (10.27) ∂t 2 ∂x On the other hand, splitting the pseudo-differential operator into the Maclaurin series yields ih ∂ 1 h2k ∂ 2k sin2 − =− ∑ = 2 ∂x 2 k=1 (2k)! ∂ x2k (10.28) h2 ∂ 2 h2 ∂ 2 h4 ∂ 4 h6 ∂ 6 − 1+ + + +... . 4 ∂ x2 12 ∂ x2 360 ∂ x4 10080 ∂ x6

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case

159

Keeping in right-hand of the Eq. (10.28) only the first term, one obtains a continuous approximation (10.18). Note that an application of the Maclaurin series implies that displacements of the neighborhood masses differ slightly from each other. From a physical point of view, it means that we study vibrations of the chain with a few masses located on the spatial period (Fig. 10.2), i.e. the long-wave approximation takes place. This is so called in-phase or acoustical mode.

Figure 10.2 Spatial form of oscillation at a fixed time t = const (points - discrete system, curve - continuous system) for acoustic mode.

Note that the vertical axis in Fig. 10.2 represents the displacement in the x direction, since the problem is 1D. Continuous system (10.18) possesses the following discrete infinite spectrum r c k αk = π , k = 1, 2, ... (10.29) m n+1 Relations (10.29) relatively good approximate low frequencies of discrete system (10.10), whereas the n-th frequency αk of a continuous system strongly differs from the corresponding n-th frequency ωk of a discrete system. Accuracy of continuous approximations can be improved, what will be discussed further. Replacing the finite spectrum of the discrete system (10.10) with the first n terms of the infinite spectrum (10.29) can be called the Debye approximation, since he used such an approximation in his theory the specific heat (heat capacity) in a solid.

10.4

“SPLASHES”

One can obtain an exact solution to the BVP (10.18)–(10.22), using the d’Alembert method matched with operational calculus [261, 289, 329]: r π c σ (x,t) = H nh arcsin sin t −x , (10.30) 2n m where H(...) is the Heaviside function. From Eq. (10.30) one obtains the following estimation: |σ (x,t)| ≤ 1.

(10.31)

It was believed that estimation (10.31) can be applied also to a discrete system [222]. However, analytical as well as numerical investigations [165–168, 260, 261]

160

Linear and Nonlinear Waves in Microstructured Solids

indicated a need to distinguish between global and local characteristics of a discrete system. In other words, classical continuous approximation can be used only for the low frequency part of the discrete system spectrum [303]. Numerical investigations show that for given masses in a discrete chain quantity the Pj = σ j (t) may exceed the values of unity in certain time instants (Table 10.1 reported in [165]).

Table 10.1 Splashes n Pn

8 1.7561

16 2.0645

32 2.3468

64 2.6271

128 2.9078

256 3.1887

n→∞ Pn → ∞

Observe that splash amplitude does not depend on the parameter m/c. In addition, the amplitude of the chain vibrations increases with increase of n, whereas its total energy does not depend on n. However, this is not a paradox. Namely, amplitude of vibrations has an order of sum of quantities σ j (t), whereas its potential energy order is represented by a sum of squares of the quantities mentioned [329]. On the other hand, a vibration amplitude of a mass with a fixed number is bounded for n → ∞, but amplitude of vibrations of a mass with a certain number increasing with increase of n tends to infinity for n → ∞ following ln n [329]. “In the language formulas! of mechanics what we just said means that when analyzing the so-called “local properties” of a one-dimensional continuous medium, one cannot treat the medium as the limiting case of a linear chain of point masses, obtained when the number of points increases without limit” [261]. Earlier the same effect of continualization was predicted by Ulam, who wrote [439]: “The simplest problems involving an actual infinity of particles in distributions of matter appear already in classical mechanics. Strictly speaking, one has to consider a true infinity in the distribution of matter in all problems of the physics of continua. In the classical treatment, as usually given in textbooks of hydrodynamics and field theory, this is, however, not really essential, and in most theories serves merely as a convenient limiting model of finite systems enabling one to use the algorithms of the calculus. The usual introduction of the continuum leaves much to be discussed and examined critically. The derivation of the equations of motion for fluids, for example, runs somewhat as follows. One images a very large number N of particles, say with equal masses constituting a net approximating the continuum, which is to be studied. The forces between these particles are assumed to be given, and one writes Lagrange equations for the motion of N particles. The finite system of ordinary differential equations becomes in the limit N = ∞ one or several partial differential equations. The Newtonian laws of conservation of energy and momentum are seemingly correctly formulated for the limiting case of the continuum. There appears at once, however, at least possible

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case

161

objection to the unrestricted validity of this formulation. For the very fact that the limiting equations imply tacitly the continuity and differentiability of the functions describing the motion of the continuum seems to impose various constraints on the possible motions of the approximating finite systems. Indeed, at any stage of the limiting process, it is quite conceivable for two neighboring particles to be moving in opposite directions with a relative velocity which does not need to tend to zero as N becomes infinite, whereas the continuity imposed on the solution of the limiting continuum excludes such a situation. There are, therefore, constraints on the class of possible motions which are not explicitly recognized. This means that a viscosity or other type of constraints must be introduced initially, singling out “smooth” motions from the totality of all possible ones. In some cases, therefore, the usual differential equations of hydrodynamics may constitute a misleading description of the physical process”. The explanation of the illusory contradiction between discrete and continuous models is quite simple. The exact solution to the discrete problem (10.17) contains both slow and fast spatialy changing harmonics. The solution of continuous system (10.30) accurately describes only the slow components of a solution. Thus, the correct continuous model of the discrete system must take into account also high harmonics.

10.5

ENVELOPE CONTINUALIZATION

A classical continuous approximation gave good description of a low part of the vibration spectrum of a finite chain of masses. In what follows we study now another limiting case, antiphase vibration, when σk = −σk+1 (Fig. 10.3). In this case one obtain the following ODE: mΩtt + 4cΩ = 0. (10.32)

Figure 10.3 Antiphase vibrations of a mass chain (optical or π-mode).

This is so-called optical or π-vibrational mode. In the case of vibrations close to the π-mode, the “envelope continualization” or “semidiscrete approximation” is usually used [247, 250, 251, 382] (Fig. 10.4). Namely, first we use “staggering transformation” [164] σk = (−1)k Ωk , (10.33)

162

Linear and Nonlinear Waves in Microstructured Solids

Figure 10.4 Envelope continualization (semidiscrete approach).

and then the Eq. (10.3) is reduced to the following form: mΩktt + c(4Ωk + Ωk−1 − 2Ωk + Ωk+1 ) = 0. Then, the following relations are applied: ih ∂ Ωk−1 (t) − 2Ωk (t) + Ωk+1 (t) = −4sin2 − Ω(x,t) = 2 ∂x 2 h4 ∂ 4 h6 ∂ 6 2 ∂ h + + + · · · Ω(x,t), k = 0, 1, 2, ..., n, n + 1. ∂ x2 12 ∂ x4 360 ∂ x6

(10.34)

(10.35)

Using Eqs. (10.36), (10.33) and considering h2 as a small parameter, one gets (we take zeroth and first-order approximations only) mΩtt + 4cΩ + ch2 Ωxx = 0.

(10.36)

Appropriate BCs for Eq. (10.36) for the case of natural oscillations are: Ω=0

at x = 0, l.

(10.37)

It is interesting to mention, that the Einstein theory of the heat capacity of solids used the so far presented conception of π-mode. The Einstein solid is a model of a solid based on two assumptions: each atom in the lattice is an independent 3D quantum harmonic oscillator and all atoms oscillate with the same frequency (in contrast to the Debye model).

10.6

INTERMEDIATE CONTINUOUS MODELS

In what follows we are going to construct improved continuous approximations. Local modeling of such systems (nonlocal theories of elasticity) requires gradient formulation. The integral formulation may be reduced to a gradient form by truncating the series expansion of the nonlocal kernel in the dual space [362]. In what follows we apply the gradient formulation approach. If, in the series (10.28), we keep three first terms, the following model is obtained 2 ∂ 2σ ∂ h2 ∂ 4 h4 ∂ 6 m 2 = ch2 + + σ. (10.38) ∂t ∂ x2 12 ∂ x4 360 ∂ x6

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case

163

Equation (10.38) includes the fourth- and sixth-order spatial derivatives and, consequently, the auxiliary BCs are required. This is a typical difficulty that arises when higher-order models, derived originally for infinite media, are applied to bounded domains [258, 259]. To overcome this difficulty, several approaches are possible. The first, originating from [231], can be called phenomenological. In [231] authors used exact expression for frequencies spectrum and proposed to introduce auxiliary BCs in a way that guarantee the most accurate frequencies approximations. As result they obtained the following BCs: σ = σxx = σxxxx = 0

at x = 0, l.

(10.39)

The same approach was used in [28] for the pulse load problem. The analytical solution was compared with a numerical simulation of the discrete lattice. Three types of higher-order auxiliary BCs were examined and BC gave the best agreement of continuous and discrete solutions was choosen. Second approach based on the variational principle [166]. In this case the auxiliary boundary conditions treats as the natural boundary conditions for the suitable variational formulation of problem. Proposed in [166] BCs coincide with (10.39). It can also be noted that the setting of boundary conditions during continualization is quite similar to the introduction of additional points in the finite difference method. There is some arbitrariness here, and the success of a choise is evaluated a posteriori. Specifically, we can arbitrarily choose values in auxiliary points k < 0 (k > n + 1) [17]. In particular, if we want to keep the translation symmetry and choose y−1 = −y1 (t), etc., the BCs (10.39) are obtained. Comparison of n-th frequency of a continuous system (10.38), (10.39) with that of a discrete system exhibits essential accuracy improvement (coefficient 2.1 instead of 2 in an exact solution yields an error of ∼ 5%). In a general case, keeping in series (10.28) N terms, one gets equations of the so-called intermediate continuous models [166] m

N h2k ∂ 2k σ ∂ 2σ = 2c . ∑ 2k ∂t 2 k=1 (2k)! ∂ x

(10.40)

BCs for Eq. (10.40) have the following form: ∂ 2k σ =0 ∂ x2k

for x = 0, l,

k = 0, 1, ..., N − 1.

(10.41)

From Eq. (10.40) one obtains αk2

c N h2k =2 ∑ m k=1 (2k)!

kπ l

2k .

(10.42)

By reflectional symmetry and periodicity it suffices to consider the wave numbers in the interval Brillouin first zone. Solution is then stable if and only if r.h.p. of (10.42) is positive for all k. This condition is the far reaching generalization of

164

Linear and Nonlinear Waves in Microstructured Solids

the Legendre-Hadamard condition of strong ellipticity in continuum elasticity [435]. One can see that BVP (10.40),(10.41) is stable for odd N. In this case Eq. (10.40) is of hyperbolic type [166]. Application of intermediate continuous models allows take into account the above mentioned splashes effect.

10.7

USING OF PADE APPROXIMATIONS

The construction of intermediate continuous models is mainly based on the splitting of a nonlocal difference operator into Maclaurin series. However, very often application of Pad´e approximations (PA) is more effective for approximation [47]. Collins [125] proposed to construct continuous models using PA. Then this approximation was widely used by Rosenau [385–389]. Further developments of this approach were done in [438, 453, 454]. Sometimes these continuous models are called quasicontinuum approximations. If only two terms are left in the series (10.28), then the PA can be cast into the following form: ∂2

h2 ∂ 4 ∂2 ∂ x2 + ≈ . 2 4 h2 ∂ 2 ∂x 12 ∂ x 1 − 12 ∂ x2

(10.43)

For justification of this procedure Fourier or Laplace transforms can be used. The corresponding quasicontinuum model reads h2 ∂ 2 m 1− σtt − ch2 σxx = 0. (10.44) 12 ∂ x2 The BCs for Eq. (10.44) have the form σ =0

for x = 0, l.

(10.45)

Therefore, using Eq. (10.44) we need not to formulate additional unphysical BCs. The error regarding estimation of n-th frequency in comparison to that of a discrete chain is of ∼ 16.5%. However, Eq. (10.45) is of lower order in comparison to Eq. (10.38). In the theory of elasticity equation of the type (10.45) is usually called Love Eq. [190] (but as Love mentioned [285], this equation was obtained earlier by Rayleigh [379]). Term σxxtt can be treated as the lateral inertia. Eq. (10.45) has hyperbolic type. Kaplunov et al. [230] refer to these type theories as theories with modified inertia. Passage to Eq. (10.45) can be treated as regularization procedure for Eq. (6.3) with N = 2 which is conditionally stable. The model governed by Eq. (10.45) is unconditionally stable and propagating waves cannot transfer energy quicker than the velocity c. However, the model governed by Eq. (10.45) predicts that short waves transfer elastic energy with almost zero speed [314], that is not correct from the physical standpoint.

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case

165

Equation (10.38) can be using PA for two last terms in r.h.p. transformed to the following form 2 ∂ h2 ∂ 4 h2 ∂ 2 ∂ 2 σ 2 = ch + m 1− σ. (10.46) 30 ∂ x2 ∂t 2 ∂ x2 20 ∂ x4 In the theory of elasticity equation of the type (10.46) is usually called Bishop Eq. [79]. Eq. (10.46) with BCs σ = σx = 0

or σ = σxx = 0

at x = 0, l

(10.47)

is conditionally stable. It is worth noting that Eq. (10.37) describing semidiscrete approach also can be regularized using PA as follows [162, 164]: h2 ∂ 2 Ωtt + cΩ = 0. (10.48) m 1− 4 ∂ x2 Finally, having in hand both long and short waves asymptotics, one may also apply two-point PA [11, 12]. In what follows we construct two-point PA using the first term of the series (10.28) as a one of limiting cases. We suppose h2k ∂ 2k ih ∂ 1 2 = sin − =− ∑ 2 ∂x 2 k=1 (2k)! ∂ x2k (10.49) 2 2 − h4 ∂∂x2 h2 ∂ 2 h2 ∂ 2 h4 ∂ 4 − 1+ + +··· ≈ 2 . 4 ∂ x2 12 ∂ x2 360 ∂ x4 1 − a2 ∂∂x2 The improved continuous approximation is governed by the following equation ∂2 m 1 − α 2 h2 2 σtt − ch2 σxx = 0. (10.50) ∂x Now we require the n-th frequency of a continuous and discrete system to coincide (compare (10.10) and (10.29)) p (10.51) αn ≈ 2 c/m. Using condition (10.51) one gets α 2 = 0.25 − π −2 .

(10.52)

Highest error in estimation of the eigenfrequencies appears for k = [0.5(n + 1)] and consists of 3%. Observe that approximate models described by Eq. (10.46) with values of a2 slightly differs from (10.52) are already known. Eringen [155–157] using a correspondence between the dispersion curves of the continuous and discrete models

166

Linear and Nonlinear Waves in Microstructured Solids

[87, 98] obtained α 2 = 0.1521. This value is very close to that proposed in [42, 315] on the basis of a some physical hypothesis “dynamically consistent model”. Interesting, that Mindlin and Herrmann used very similar to two-point PA idea for construction their well-known equation for longitudinal waves in rod [319]. Dispersion relation (10.50) does not satisfy condition dαk /dk = 0 at the end of first Brillouin zone [98]. That is why in [156,273] so-called bi-Helmholtz type equation was proposed. In [273], this equation takes the following form ∂4 ∂2 (10.53) m 1 − α 2 h2 2 + α12 h4 4 σtt − ch2 σxx = 0, ∂x ∂x where α1 = 1/π. BCs associated with this equation are σ = σxx = 0

at x = 0, l

or σ = σx = 0

at x = 0, l.

(10.54)

Unfortunately, this equation is unstable. This is the price one has to pay is that the group velocity is off at the end of the Brillouin zone [273]. Let us also analyse lattice with inertially linked masses (Fig. 10.5).

Figure 10.5 A chain of inertially coupled masses.

Governing equations can be written as follows [271] 4cy j (t) = m

d2 y j−1 (t) − 2y j (t) + y j+1 (t) , 2 dt

j = 1, 2, ...., n.

Frequencies ωk of discrete system (10.55) are r c −1 kπ ωk = sin , k = 1, 2, . . . , n. m 2(n + 1)

(10.55)

(10.56)

Continuous approximation for this model is as follows 4cy(x,t) = mh2 and describes highest frequencies.

d2 ytt (x,t), dx2

(10.57)

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case

167

Antiphase mode of the following forms cy(x,t) = −mytt (x,t), presents the lowest frequency. Quasicontinuous models are governed by the following PDEs 2 h2 d 2 2 d c 1− y(x,t) = mh ytt (x,t), 12 dx2 dx2 2 2 2 2 d 2 d ytt (x,t). c 1−α h y(x,t) = mh dx2 dx2

(10.58)

(10.59)

(10.60)

BCs for Eqs. (10.57),(10.59) and (10.60) take the form y(0,t) = y(l,t) = 0.

10.8

(10.61)

NORMAL MODES EXPANSION

In the previous sections, we studied the effectiveness of various continualization approaches for calculating the natural oscillations of discrete system. The possibility of a satisfactory approximation of natural frequencies over the entire range of their variation is shown. However, the study of free or forced oscillations requires normal modes expansion. We consider as an example the discrete problem (10.3), (10.15), (10.16), which possesses the exact solution (10.17). Let us use for continuous approximation Eqs. (10.50),(10.52) with BCs (10.19) and ICs (10.22) and the following ansatz x σ (x,t) = 1 − + u(x, l). l Function u(x,t) is defined by the following BVP: ∂ m 1 − α 2 h2 2 utt − ch2 uxx = 0, ∂x

(10.62)

(10.63)

u(0,t) = u(l,t) = 0, (10.64) x u(x, 0) = −1 + , ut (x, 0) = 0. (10.65) l Solution to the BVP (10.63)–(10.65) can be obtained via Fourier method kπx x 2 ∞ 1 cos(βk t), (10.66) σ = 1 − − ∑ sin l π k=1 k l l αk . l +α 2 π 2 h2 k2

where βk are defined by βk = √ 2

168

Linear and Nonlinear Waves in Microstructured Solids

For the approximation of the chain motion we keep in an infinite sum only n first harmonics x 2 n 1 kπx cos(βk t). (10.67) σ = 1 − − ∑ sin l π k=1 k l Let us compare solutions (10.17) and (10.67). Function 1 − x/l serves as a good approximation of truncated series 1 n πk j πk sin cot . ∑ n + 1 k=1 n + 1 2(n + 1)

(10.68)

Frequencies βk stand for the good approximation for frequencies ωk . But the coefficients in the truncated series (10.67) and (10.68) differ from each other. Projections onto normal modes of discrete and continuous systems, πk 1 cot n+1 2(n + 1)

(10.69)

2 and πk respectively, strongly differ from each other for k 1. This is because during projection into normal modes for the discrete system one must use summation over k from 0 to n, whereas for the continuous system - integration with regard to x from 0 to l. The problem occurring so far can be overcome using the Euler-Maclaurin formulas [2] n+1 Z

n+1

1 f (x)dx + [ f (0) + f (n + 1)] + 2 0 j ∞ (−1) j+1 d f (n + 1) d j f (0) B − , j ∑ dx j dx j j=1 j + 1

∑ f (k) = k=0

(10.70)

where Bi are the Bernoulli numbers [2], having the following values: B0 = 1, B1 = −1/2, B2 = 1/6, B3 = 0, ... In addition, the following formulas hold [377]: Bn = −

1 n k+1 ∑ Cn+1 Bn−k , n + 1 k=1

n+1

kπ j

∑ sin2 n + 1 =

k=0

n+1 , 2

(10.71)

(10.72)

n+1

∑ k=0

j kπ j 1 πj 1− sin = ctg . n+1 n+1 n+1 2(n + 1)

(10.73)

The corresponding integrals read n+1 Z

sin2

0

π jx n+1 dx = , n+1 2

(10.74)

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case n+1 Z

1−

0

x π jx 2 sin dx = . l n+1 πj

169

(10.75)

Observe that the values of sum (10.72) and integral (10.74) coincide. Using the Euler-Maclaurin formula one obtains n+1 Z π jx kπ j x j sin 1− dx+ ∑ 1 − n + 1 sin n + 1 = l n +1 k=0 0 " # 1 jπ 2 π 2 j2 [sin 0 + sin( jπ)] − cos 0 + ... = 1− . 2 6(n + 1) πj 12(n + 1)2

n+1

(10.76)

Owing to formula (10.76), one can construct a simple expression relatively good approximating sum (10.73) for arbitrary j values from j = 1 to j = n. For this purpose, we change second term of the right hand side of Eq. (10.76) in the following way: " # n+1 kπ j 2 j2 j (10.77) ∑ 1 − n + 1 sin n + 1 ≈ π j 1 − (n + 1)2 . k=0

10.9

THEORIES OF ELASTICITY WITH COUPLE-STRESSES

Since the release of the classic monograph by Cosserat’ brothers [129] and Le Roux paper [274], activity has continued in the direction of generalizations of the theory of elasticity, which expand the possibilities for describing the effects accompanying elastic deformations of materials with an internal structure [257–259]. A good description of these theories can be found in comprehensive reviews including [308, 446]. It was expected that the results of such work will lead to a significant change in the values of the concentration coefficients and the types of stress singularities [318, 434]. As a problem that impedes the use of generalized theories for solving real problems, there is a lack of quantitative data on the physical constants of these theories [308, 446]. As it is mentioned in [446], “Generalized elasticity theories even for isotropic materials contain many additional constants that are difficult or impossible to determine experimentally”. Theoretically, gradient moduli were previously determined [291] for a microinhomogeneous medium composed of homogeneous and isotropic grains, whose Lam´e’s constants are random variables. Recently, gradient modules have been defined for two-phase composites in the case of a low concentration of inclusions in a homogeneous matrix [46, 78]. It is shown that it is possible to estimate the values of the gradient modules and the corresponding characteristic lengths for the crystal lattice of metals by the methods of the density functional theory [406]. However, at present, the problem of determining the constants of the theory of elasticity with couple-stress by directly continualization of a real atomic lattice is far from solving. In this regard, the work [292] is of great interest. In this paper closed-form expressions for five physical constants of the Toupin-Mindlin theory of isotropic gradient

170

Linear and Nonlinear Waves in Microstructured Solids

elasticity for polycrystalline materials were obtained. A polycrystal is considered as a micro-inhomogeneous elastic medium, which consists of homogeneous anisotropic crystallites with random orientation. It is shown that the elastic energy density of the polycrystalline medium depends nonlocally on the nonuniform field of average deformations. In the case of smooth fields of average deformations it could be considered that the energy density locally depends not only on the values of deformations, but also on the values of their derivatives. This dependence in the isotropic case is characterized by five gradient modules, in addition to the two elastic moduli of the classical theory of elasticity. For the first time, explicit expressions are obtained for the gradient modules of polycrystalline materials. Although a single sample of a polycrystalline body is described by the local classical theory of elasticity of micro-inhomogeneous bodies, the averaged macroscopic properties of a representative ensemble of polycrystalline samples turn out to be homogeneous in a macroscopic sense. Therefore, the transition from the consideration of a particular sample to the description of the averaged macroscopic properties of an ensemble of samples can be called homogenization. In this case, it turns out that macroscopic properties are described by a nonlocal theory of elasticity. It is necessary to distinguish the homogenization of a continuous microinhomogeneous medium from the continualization of a discrete elastic medium, such as a crystal lattice [257–259]. Formally, both approaches lead to theories with a nonlocal dependence of the density of elastic energy on the displacement field, but physically these are completely different theories. But from the physical point of view, the result of the lattice continualization differs significantly from the homogenization of a continuous microinhomogeneous medium. First, nonlocal effects for the lattice are include into the theory from the very beginning due the long-range interatomic forces. Secondly, the characteristic lengths of nonlocal lattice effects correspond in order of magnitude to interatomic distances, i.e. their influence is many orders of magnitude less than in the case of polycrystals. And thirdly, a correct description of the lattice behavior requires consideration of its anisotropy, which further complicates the already cumbersome description of nonlocal effects. For example, the local Toupin-Mindlin gradient theory obtained as a result of homogenization requires the introduction of five additional physical constants. But after the continualization of even a simple cubic lattice, eleven additional physical constants appear [45, 199].

10.10

CORRESPONDENCE BETWEEN FUNCTIONS OF DISCRETE ARGUMENTS AND APPROXIMATING ANALYTICAL FUNCTIONS

For continualization we must construct a function u(x,t) representing a continuous approximation of the function of discrete argument u j (t) u( jh,t) = u j (t),

(10.78)

where h is the distance between points of discrete function. Observe that it is defined with an accuracy to any arbitrary function, which equals zero in nodal points x = jh . For this reason, from a set of interpolating functions one

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case

171

may choose the smoothest function owing to filtration of fast oscillating terms. As it is shown in [258], the interpolating function is determined uniquely, if one requires its Fourier image Z∞

u(q,t) ¯ =

−iqx

u(x,t)e −∞

1 dx; u(x,t) = 2π

Z∞

iqx u(q,t)e ¯ dx

(10.79)

−∞

to differ from zero only on the segment −π/h ≤ q ≤ π/h. From this condition one obtains n sin π(x−kh) h . (10.80) u(x,t) = ∑ uk (t) π(x − kh) k=1 Function

sin(πx) (10.81) πx is familia normalized sinc function, often called Whittaker-Kotelnikov-Shannon (WKS) interpolating function. The value of this function at the removable singularity at zero is understood to be the limit value 1. The sinc function is then analytic everywhere and hence an entire function. Also this function has interesting properties: Z∞ sin πx dx = 1, (10.82) πx sinc(x) =

−∞

sin πx h = δ (x). (10.83) h→0 πx We note that the concept of concentrated force in the theory of elasticity with couple-stresses must be changed in comparison with classical theory of elasticity. Namely, delta-function must be replaced to the sinc function due size effect caused by internal structure of material. This statement is illustrated by identity (10.83). lim

10.11

THE KERNELS OF INTEGRO-DIFFERENTIAL EQUATIONS OF THE DISCRETE AND CONTINUOUS SYSTEMS

Let us consider the chain of material points with the equal masses m, located in equilibrium states in the points of the axis x with coordinate’s jh, j = 0, ±1, ±2, ... and suspended by elastic couplings with stiffness c. The governing ODEs are as follows d 2 y j (t) m = c(y j+1 − 2y j + y j−1 ), j = 1, 2, 3, ... (10.84) dt 2 where y j (t) is the displacement of the j-th material point from its static equilibrium position. Instead of the dimensional coordinates x, y,t, we introduce dimensionless coordip nates ξ = x/h, τ = t c/m, z j = y j /h and rewrite (10.84) as d2z j = z j+1 − 2z j + z j−1 . dτ 2

(10.85)

172

Linear and Nonlinear Waves in Microstructured Solids

Differential-difference Eq. (10.85) can be reduced to the following integrodifferential equation [182, 400]: ∂ 2 z(x, τ) =− ∂ τ2

Z∞

Φd (ξ − ξ1 )y(ξ1 , τ)dξ1 ,

(10.86)

−∞

Φd (ξ ) =

2 π

Zπ −π

sin2

q 2

cos(qξ )dq =

2 (2ξ 2 − 1) sin(πξ ). πξ (ξ 2 − 1)

(10.87)

Equations (10.86), (10.87) describe the media with nonlocal interactions. The classical continuous approximation is: ∂ 2z ∂ 2z = . ∂ τ2 ∂ξ2

(10.88)

Thus, replacement of the discrete media with the continuous one leads to two reasons for error. The first one is connected with replacement of the integral with finite limits of integration on the integral with infinite limits of integration Φ(ξ ) =

4 π

Z∞

sin2

q 2

cos(qξ )dq.

(10.89)

0

Such a replacement from a physical standpoint is caused due the transition from the discrete to the continuous media. The second reason for error type is connected with approximation of the operator 4sin2 (q/2). The general approach to improvement of approximation (10.88) consists in approximation of the integral operator from the r.h.p. of Eq. (10.87) with higherorder derivatives in the assumption that nonlocal property is weak. For example, replacing integration limits in integral (10.87) on infinite ones and using truncated Maclaurin series q 1 1 6 4sin2 ≈ q2 − q4 + q (10.90) 2 12 360 we obtain intermediate continuous model (Chapter 10.6): 2 ∂ 1 ∂4 1 ∂6 ∂ 2z = + + z. (10.91) ∂ τ2 ∂ ξ 2 12 ∂ ξ 4 360 ∂ ξ 6 One of the ways for improvement of the local approximation can consist in more precise approximation of the operator sin2 2q . Using for this aim PA one obtains (Chapter 10.7) 1 2 2 q 2 4sin ≈ q / 1+ q . (10.92) 2 12 Using Eq. (10.92) one obtains the following model: 2 1 ∂2 ∂ z ∂ 2z 1− = . 12 ∂ ξ 2 ∂ τ 2 ∂ξ2

(10.93)

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case

173

Two-point PA gives more precise approximation (Chapter 10.7) 4sin2

q 2

≈

q2 , 1 + α 2 q2

α 2 = 0.25 − π −2 .

Using Eq. (10.94) one obtains the following approximation: 2 2 ∂ z ∂ 2z 2 ∂ 1−α = . ∂ ξ 2 ∂ τ2 ∂ξ2

(10.94)

(10.95)

We investigate the accuracy of the approximation of the kernel of an integrodifferential equation (10.86), which describes the deformation of a discrete media. Integral (10.87) has the following asymptotics Φd (ξ ) →

sin(πξ ) 4 sin(πξ ) ≈ 1.2732 π ξ ξ Φd (ξ ) → 2 Φd (ξ ) → −1

at ξ → ∞,

at ξ → 0, at ξ → 1.

(10.96) (10.97) (10.98)

The kernels of integro-differential equations of classical continuous approximation (10.90) Φc (ξ ) and intermediate continuous approximation (10.91) Φci (ξ ) have the following expressions and asymptotics: 1 Φc (ξ ) = π

Zπ 0

π 2 ξ 2 − 2 sin (πξ ) + 2πξ cos (πξ ) , q cos (qξ ) dq = πξ 3 2

Φc (ξ ) → π

sin (πξ ) ξ

at ξ → ∞,

π2 ≈ 3.2899 at ξ → 0, 3 Φc (ξ ) → −2 at ξ → 1, π Z 1 q4 q6 2 Φci (ξ ) = + q − cos (qξ ) dq = π 12 360 0 2 4 2 π4 π sin (πξ ) 2 − π3 + π60 cos (πξ ) 1 − π12 + 360 + − ξ ξ2 4 2 2 − π 2 + π12 sin (πξ ) 2 − π3 cos (πξ ) + − πξ 3 ξ4 2 − π 2 sin (πξ ) 2 cos (πξ ) 2 sin (πξ ) + − , πξ 5 ξ6 πξ 7 Φc (ξ ) →

(10.99)

(10.100) (10.101) (10.102)

(10.103)

174

Linear and Nonlinear Waves in Microstructured Solids

2 π4 1 − π12 + 360 π sin (πξ )

sin (πξ ) ≈ 1.4077 at ξ → ∞, (10.104) ξ ξ π2 π2 π4 Φci (ξ ) → 1− + ≈ 2.0479 at ξ → 0, (10.105) 3 20 840

Φci (ξ ) →

2π 2 π 4 − ≈ −1.0437 at ξ → 1. (10.106) 3 60 The kernels of integro-differential equations continuous approximation (10.93) Φqc (ξ ) and improved continuous approximation (10.95) Φqci (ξ ) can be written as follows Φqc (ξ ) = Φ0 b2 , ξ for b2 = 1/3, (10.107) Φqci (ξ ) = Φ0 b2 , ξ for b2 = 1 − 4/π −2 , (10.108) Φci (ξ ) → −6 +

where 8 Φ0 b , ξ = π 2

π/2 Z

q2 cos (2qξ ) dq. 1 + b2 q2

(10.109)

0

Evaluating the integral (10.109) one obtains 4 sin ξ π 8 2ξ 2ξ + Re Si πξ + i sinh + Φ0 b2 , ξ = πb2 ξ πb3 b b 2ξ 2ξ 2ξ ImCi πξ + i − ImCi i cosh , b b b

(10.110)

where RSi(·) and Ci(·) are the familiar sine and cosine integrals, Ci(y) = γ + R ln y + 0y t −1 (cost − 1) dt, Si(y) = 0y t −1 sint dt, γ is the Euler constant, γ = 0.5772156649... ( [2], Chapter 5). Asymptotics of kernels of continuous approximation (10.93) Φqc (ξ ) and improved continuous approximation (10.95) Φqci (ξ ) are 12π sin(πξ ) sin(πξ ) ≈ 1.7238 at ξ → ∞, 12 + π 2 ξ ξ √ π 3π − 6 3arctg( 2√ ) 3 Φqc (ξ ) → 4 ≈ 2.2532 at ξ → 0, π Φqc (ξ ) → −1.2123 at ξ → 1,

Φqc (ξ ) →

(10.111)

(10.112) (10.113)

4 sin(πξ ) at ξ → ∞, (10.114) π ξ √ √ π 2 −4 4π 2 π 2 − 4 − 2arctg 2 q Φqci (ξ ) → ≈ 1.8360 at ξ → 0, (10.115) 3 2 (π − 4) Φqci (ξ ) →

175

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case

Φqci (ξ ) → −0.92036

at ξ → 1.

(10.116)

For a good continuous approximation is the most important as a more accurate approximation at ξ → ∞ the kernel of a integro-differential equation [258]. The best approximation gives the continuous approximation (10.95), which provides an accurate approximation up to the order O(ξ −2 ).

10.12

DISPERSIVE WAVE PROPAGATION

Let us analyse dispersive wave propagation in the following mass-spring lattice mY jττ (τ) = c[Y j−1 (τ) − 2Y j (τ) +Y j+1 (τ)]; j = 0, ±1, ±2, ±3, ...,

(10.117)

where Y j (τ) is the displacement of the j-th material point from its static equilibrium position, τ is the time. p Let us introduce new variables y j (t) = Y j (τ)/h, t = τ c/m, then Eq. (10.117) can be transformed to the following one: y jtt (t) = y j−1 (t) − 2y j (t) + y j+1 (t); j = 0, ±1, ±2, ±3, ...

(10.118)

Suppose that at t = 0 all masses in the lattice are at rest with the sole exception of the mass numbered zero, which has been displaced by 1 y j (0) = δ j0 , y jt (0) = 0,

(10.119)

where δ ji is the Kronecker delta. Solution of initial value problem (IVP) (10.4) was firstly obtained by Schr¨odinger [400] and can be written as follows [182] ym (t) = J2m (2t) =

π/h Z

h 2π

qh cos 2t sin cos (mhq) dq, 2

(10.120)

−π/h

where J2m (2t) is the Bessel function of the first kind with integer order 2m, m denotes the m-th node. Let us analyse continuous approximations. Let us introduce the continuous coordinate x scaled in such a way that x = jh at the nodes of the lattice. We assume that ym (t) is discrete approximation to a continuous function u(mh,t). We have ym (t) = u(mh,t).

(10.121)

Then initial-boundary value problem for continuous function u(x,t) can be written as follows utt − h2 uxx = 0, (10.122) Conditions (10.119) are transformed using Whittaker-Kotelnikov-Shannon interpolating function sin c(x) = sin(x)/x (see Chapter 10.10) u(x, 0) =

h sin(πx/h) , πx

ut (x, 0) = 0.

(10.123)

176

Linear and Nonlinear Waves in Microstructured Solids

The solution of initial-boundary value problem (10.122), (10.123) may be expressed as follows π/h Z

h u(x,t) = 2π

cos(qht) cos (qx) dq = (10.124)

−π/h

1 sin(π(t − x/h)) sin(π(t + x/h)) . + 2π t − x/h t + x/h The continuous approximation qualitatively correctly describes the behavior of the discrete lattice far from the wave front. The construction of a continuous model that is completely adequate to the discrete case requires additional research.

10.13

GREEN’S FUNCTION

Dynamic Green’s functions for nonlocal (10.3), local (10.18) and improved local (10.50) models are r 1 ω m |x| = G(x) = − √ sin 2 arcsin 2 mchω 2h c (10.125) r ω m 1 |x| , − cos arcsin ch 2h c r 1 m |x| sin ω , (10.126) G(x) = − √ 2 mchω c h ! r 1 ω m p |x| . G(x) = − √ sin (10.127) 2 mchω h 1 − α 2 mω 2 h2 /c c Kunin [258, 259] proposes to construct continuous approximation of the Green’s functions of a discrete chain using by the first roots of the characteristic equation. Note that approximation (10.127) gives also satisfactory results. Very detail analysis of Green’s function for continuous approximations can be found in [116, 117].

10.14

DOUBLE- AND TRIPLE-DISPERSIVE EQUATIONS

Let us consider an infinite lattice consisting of identical particles of the mass m connected by massless springs of rigidity c. The equation of motion reads m

d 2 un + c (2un − un+1 − un−1 ) = 0, dT 2

(10.128)

where u is the displacement; n is the index number of the particle, n = 0, ±1, ±2, . . .; T is the time variable.

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case

177

The time-harmonic wave is represented by the expression u = Aexp (−ikn) exp (iΩT ) ,

(10.129)

where A is the amplitude; k is the non-dimensional wave number and Ω is the frequency. Substituting (10.129) into (10.128), we obtain the dispersion relation as follows ω 2 = 4sin2 (k/2) ,

(10.130)

where ω is the non-dimensional frequency, ω 2 = Ω2 m/c. A simple analysis of formula (10.130) shows that wave propagation is allowed in the frequency range 0 < ω < 2. At the long-wave limit, as k → 0, the frequency vanishes, ω → 0, so no vibrations occur and the motion is simply a rigid body translation. The opposite limit, k → π , describes a standing wave with zero group velocity and non-zero frequency, ω → 2. This regime can be considered as a “hidden” or “trapped” mode, in the sense that no energy is transmitted on macro scale, but on micro scale the lattice exhibits antyphase oscillations. As ω > 2, the wave number k becomes complex. Then the spectrum of the lattice exhibits a band gap and the signal decays exponentially with an attenuation coefficient equal to the imaginary part of the wave number. In the limiting cases discussed above, the dispersion relation (10.130) can be expressed by asymptotic relations ω 2 ∼ k2

at k → 0,

ω 2 ∼ 4 − (π − k)2

(10.131)

at k → π .

(10.132)

Matching expressions (10.131) and (10.132) with the help of two-point PA (Chapter 10.7), we obtain a1 k2 + a2 k4 . (10.133) ω2 ≈ 1 + a3 k2 + a4 k4 Here the coefficients a1 , ... ,a4 are determined in such a way that the leading terms of the power series expansions of PA (10.133) at kh→ 0 and ki → π must coincide with formulas (10.131) and (10.132) up to O k2 , O (π − k)2 accordingly. Using this condition, we derive a1 = 1,

a2 =

64 − π 4 , π6

a3 =

π2 −8 , 4π 2

a4 =

64 + 4π 2 − π 4 . 4π 6

(10.134)

In Fig. 10.6, formula (10.133) is compared with the exact dispersion relation (10.130). We note that the numerical results are essentially indistinguishable. For any real k, the denominator of the derived PA does not equal zero. Therefore, expression (10.133) can be rewritten as follows ω 2 − a1 k2 − a2 k4 + a3 ω 2 k2 + a4 ω 2 k4 = 0.

(10.135)

178

Linear and Nonlinear Waves in Microstructured Solids

Figure 10.6 Dispersion relation of the lattice. Solid curves - exact solution (10.130), circles - PA (10.133).

Let us introduce the continuous coordinate X scaled in such a way that X = nl at the nodes of the lattice, where l is the distance between the particles. Using non-dimensional variables, the time-harmonic solution (10.129) reads u = Aexp (−ikx) exp (iωt) ,

(10.136)

where x = X/l, t = T (c/m)1/2 , k = 2π l/L, L is the wave length. Then one can easily show ∂ 4u ∂ 2u ∂ 2u 2 4 = −k u, = k u, = −ω 2 u, ∂ x2 ∂ x4 ∂t 2 ∂ 6u ∂ 4u 2 2 = ω k u, = −ω 2 k4 u. ∂ x2 ∂t 2 ∂ x4 ∂t 2

(10.137)

The dispersion equation (10.135) allows us to obtain a PDE that describes wave propagation for all wave numbers 0 ≤ k ≤ π : a1

∂ 2u ∂ 2u ∂ 4u ∂ 4u ∂ 6u − 2 − a2 4 + a3 2 2 − a4 4 2 = 0. 2 ∂x ∂t ∂x ∂ x ∂t ∂ x ∂t

(10.138)

Equation (10.138) includes three dispersive terms and may be considered as a generalization of double-dispersive equations, which were employed by many authors to simulate elastic waves in waveguides with a free lateral surface (see, for example, [369] and references therein). In the theory of waves in structured solids, double- and triple-dispersion equations can be obtained by imposing some additional internal degrees of freedom on the system (see, for example, a review [74]). It should be noted that such gradient models include a number of phenomenological parameters, which for real materials remain usually unknown. In contrary, the approach proposed in this section allows us to evaluate all the coefficients of Eq. (10.138) theoretically basing on the information about the internal structure of the medium and

179

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case

its properties. The developed macroscopic model is able to describe the long-wave case and, at the same time, it is valid in a high-frequency domain in the vicinity of the stop band threshold.

10.15

TODA LATTICE

Let nonlinear springs in 1D problem have potential energy U(rn ), where rn = yn+1 − yn . The chain dynamics is governed by the following infinite system of PDEs [401]: ∂U(rn+1 ) ∂U(rn ) ∂U(rn−1 ) ∂ 2 rn = −2 , + 2 ∂t ∂ rn+1 ∂ rn ∂ rn−1

(10.139)

where rn = yn+1 − yn . Assume that solution to the (10.139) is a travelling wave, rn = R(z), z = n − vt. Then Eq. (10.139) is cast into the following form: v2 R00 (z) = U 0 (R(z − 1)) − 2U 0 (R(z)) +U 0 (R(z + 1)),

(10.140)

where (...)0 = d(...) dz . Introducing notation Φ(z) = U 0 (R(z)) and applying the Fourier transformation to Eq. (10.140) one gets ¯ R(q) =

Z∞

¯ R(z) exp(−iqz)dz; Φ(q) =

−∞

Z∞

Φ(z) exp(−iqz)dz.

(10.141)

−∞

From (10.140) one obtains ¯ ¯ v2 R(q) = f (q)Φ(q),

(10.142)

2

where f (q) = 4 sin q(q/2) . 2 Term f (q) can be approximated by PA or two-point PA in the following way f (q) =

1 1 + q2 /12

or

f (q) =

1 , 1 + α 2 q2

(10.143)

where α 2 = 0.25 − π −2 . In result one obtains equation of continuous approximation v2 (1 −

1 d2 )R(z) = U 0 (R(z)) 12 dz2

(10.144)

or

d2 v2 1 − a2 2 R(z) = U 0 (R(z)). (10.145) dz We show also a simultaneous application of PA with a perturbation procedure using an example of the Toda lattice [401]: m

d 2 yn = a[exp(b(yn−1 − yn )) − exp(b(yn − yn+1 ))]. dt 2

(10.146)

180

Linear and Nonlinear Waves in Microstructured Solids

System of ODEs (10.146) can be rewritten as pseudo-differential equation: m

2 1 ∂ ∂ 2y − 4a sinh exp(−by) = 0. ∂t 2 2 ∂x

(10.147)

Equation (10.147) can be approximately factorized [258] r r b ∂ b ∂ m ∂ 1 ∂ m ∂ 1 ∂ + y − y y = 0. − 2 sinh + 2 sinh ab ∂t 2 ∂x 2 ∂x ab ∂t 2 ∂x 2 ∂x (10.148) For wave spreading in right direction one obtains r m ∂ 1 ∂ h ∂ + 2 sinh − y y = 0. (10.149) ah ∂t 2 ∂x 2 ∂x Formally expanding function sinh 12 ∂∂x in a Maclaurin series up to the terms of the third order one obtains from (10.149) r m ∂y ∂y 1 ∂ 3y b ∂ y + + − y = 0. (10.150) ab ∂t ∂ x 24 ∂ x3 2 ∂ x p Using variables transform t1 = abt/m, y1 = 0.5yb, the Kortewegde Vries Eq. [258, 401] of the following form is obtained: ∂ y1 ∂ y1 1 ∂ 3 y1 ∂ y1 + + − y1 = 0. ∂t1 ∂x 24 ∂ x3 ∂x

(10.151)

Let us construct regularized long-wave equation, described in references [1, 72, 357]. Using PA one gets −1 1 ∂2 1 ∂2 ∼ 1− . 1+ 24 ∂ x2 24 ∂ x2

(10.152)

Then, using (10.152) one obtains from Eq. (10.151) (up to the highest terms) the following regularized long-wave equation: 1 ∂ 2 ∂ y1 ∂ y1 ∂ y1 1− + − y1 = 0. (10.153) 24 ∂ x2 ∂t1 ∂x ∂x On the other hand, there are nonlinear lattices with a special type nonlinearities allowing to achieve exact solutions (Toda, Ablowitz-Ladik, Langmuir, Calogero, etc. [72, 135, 139, 184, 305, 357]) in the case of infinite lattices or in the case of boundary conditions. In many cases non-integrable systems like a discrete variant of sine-Gordon equation possesses soliton-like solution. Occurrence of exact solutions of a discrete system allows applying the following approach: fast changeable solution part is constructed using a discrete model,

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case

181

whereas a continuous approximation is applied for slow components. The latter approach is used by Maslov and Omel’yanov [305], who analyzed Toda lattice with variable coefficients d 2 yk = −ak [exp bk (yk − yk−1 ) − 1]+ dt 2 ak+1 [exp(bk+1 (yk+1 − yk ) − 1], k = 0, ±1, ±2, ...

mk

(10.154)

They construct soliton solutions in the following way: rapidly changing part of soliton is constructed using Toda lattice with constant coefficients, and for slowly part of solution continuous approximation is used. Then these solutions are matched.

10.16

DISCRETE KINKS

We consider the nonlinear Klein-Gordon equation C1

∂ 2 z ∂ 2 z ∂V (z) − − = 0. ∂ y2 ∂t 2 ∂z

(10.155)

Here V (z) is the potential having at least two degenerate minimums. The travelling wave solution of Eq. (10.155) describes the following equation: C

∂ 2 z ∂V (z) − = 0, ∂ x2 ∂z

(10.156)

where x = y − ct; z(x) ≡ z(y − ct); C = C1 − c2 . The reason for the transition from the PDE (10.155) to the ODE (10.156) is the invariance of the equations to Lorentz transformations. Discrete analog of Eq. (10.156) is given by ∂V (z) −C(zn−1 − 2zn + zn+1 ) + = 0, (10.157) ∂ z z=zn where zn = z(n); without loss of generality the mesh width is taken as 1. The estimation of Peierls-Nabarro barrier value for the kinks in the Eq. (10.157) represents a problem of great importance. The following approach is proposed in [173,208]. The energy is estimated based on a discrete model and the discrete values of variables are replaced with the values calculated within the framework of the continuous model. By virtue of the fact that the approximation accuracy is small, in [172] it was proposed perturbation approach basing on the averaging. As a result 2 for the Φ4 model with V (z) = 41 (z2 − 1) potential, the following equation is derived d2z 1 2 1 C 2 − z(z2 − 1) 1 + − z = 0, (10.158) dx 12C 4C and for sine-Gordon equation with V (z) = 1−cos(z) potential the improved equation takes the form of double sine-Gordon equation C

d2z 1 − sin(z) + sin(2z) = 0. dx2 24C

(10.159)

182

Linear and Nonlinear Waves in Microstructured Solids

Solution of Eq. (10.158) is given by [172] q 1 √x tanh 1 − 6C 2C , q z(x) = 1 1 √x sech2 1 − 6C 1 − 6C 2C

(10.160)

for Eq. (10.159) it is: "r

1 cosech 1− 12C

z(x) = 2π − 2 arctan "r z(x) = −2 arctan

1 1− co sech 12C

r

1 x √ 1− 12C C

r

1 x √ 1− 12C C

!# x ≥ 0, (10.161)

,

!# ,

x ≤ 0.

The continuous approximation for the discrete model (10.157) yields d2z 1 d 2 ∂V (z) C 2 − 1− = 0. dx 12 dx2 ∂z For the Φ4 model one obtains d2z 1 1 2 1 dz 2 2 C 2 1− + z − z(z − 1) + z = 0. dx 12C 4C 2 dx

(10.162)

(10.163)

(10.164)

1 1 2 If C >> 1, the coefficient 1 − 12C + 4C z can be transformed using PA:

1 2 1 1 2 −1 1 1− + z ∼ 1+ − z . 12C 4C 12C 4C

(10.165)

Using the Eq. (10.165) and omitting the higher-order terms, the Eq. (10.164) is replaced by the following one ( 2 ) 1 1 2 1 ∂z ∂ 2z 2 − z + z = 0. (10.166) C 2 − z(z − 1) 1 + ∂x 12C 4C 2 ∂x Let us estimate an influence of the braced terms. In the neighborhood of zero the linear terms have a dominant role. Using the solution (10.160), we find

∂z ∂x

2 ∼

1 4

2Csech

√x 2C

.

(10.167)

Therefore the braced term can be neglected and Eq. (10.166) is the same as Eq. (10.163) obtained in [355] by distinctly other means. In the similar way for the sineGordon equation the continuous approximation can be reduced to Eq. (10.164).

183

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case

The equations obtained on the basis of the continuous approximation are: α 2 3α 2 2 d2z 2 C 2 − z(z − 1) 1 + − z = 0, (10.168) dx C C d2z α2 − sin(z) + sin(2z) = 0. dx2 2C Solution of Eq. (10.168) is q 2α 2 √x tanh 1 − C 2C q , z(x) = 2 2α 2 2α 2 √x 1 − C sech 1 − C 2C

(10.169)

C

whereas for Eq. (10.169) we have "r !# r α2 α2 x √ z(x) = 2π − 2 arctan 1− 1− cosech , C C C "r z(x) = −2 arctan

α2 cosech 1− C

r

α2 x √ 1− C C

(10.170)

x ≥ 0, (10.171)

!# ,

x ≤ 0.

(10.172)

Solutions (10.170), (10.172) make possible to obtain the values for the PeierlsNabarro barrier with the accuracy better than the accuracy received when using the solutions (10.160)- (10.162).

10.17

CONTINUALIZATION OF β -FPU LATTICE

We study vibrations of a monatomic lattice consisting of identical particles connected by cubically nonlinear elastic springs (Fig. 10.7). Neighbouring particles are depicted by different colors illustrating that they can move with different amplitudes, although the masses of the particles are the same. The length of the lattice is L and the distance between the particles is l. Every particle is denoted by a number n, n = 0, 1, 2, . . . , N, where N = L/l. The total number of the particles is N + 1.

Figure 10.7 The lattice under consideration.

184

Linear and Nonlinear Waves in Microstructured Solids

We seek a continuous model capable to describe both acoustic and optical forms of motion. Let us employ different notations Y and Z for the displacements of black and white particles accordingly. Vasiliev et al. [447] called this approach as a twofield model (see also [371]). It is also consistent with the continualization procedures proposed by Zabusky and Deem [467]. Below we follow paper [27]. The governing equations of motion read d 2Yn + c1 (2Yn − Zn−1 − Zn+1 ) + dT 2 c3 (Yn − Zn−1 )3 + c3 (Yn − Zn+1 )3 = 0,

m

d 2 Zn+1 m + c1 (2Zn+1 −Yn −Yn+2 ) + dT 2 c3 (Zn+1 −Yn )3 + c3 (Zn+1 −Yn+2 )3 = 0.

(10.173)

Here T is time, m is the mass of the particle, c1 and c3 are the elastic coefficients of the spring. Systems of this type are called β -Fermi-Pasta-Ulam (β -FPU) lattice [456]. In a dimensionless form, equations (10.173) can be written as follows d 2 yn + (2yn − zn−1 − zn+1 ) + ε(yn − zn−1 )3 + ε(yn − zn+1 )3 = 0, dt 2 (10.174) d 2 zn+1 3 3 + (2zn+1 − yn − yn+2 ) + ε(zn+1 − yn ) + ε(zn+1 − yn+2 ) = 0, dt 2 p where t = T c1 /m; yn = Yn /A; zn = Zn /A; A is the vibration amplitude; ε = A2 c3 /c1 . We suppose that neighboring particles do not collide each other, so |A| < l/2. In order to separate low- and high-frequency motions of the lattice, let us introduce the acoustic un and optical vn fields as follows yn + zn−1 , 2 yn − zn−1 vn−1 = , 2

un−1 =

yn + zn+1 yn+2 + zn+1 , un+1 = , 2 2 yn − zn+1 yn+2 − zn+1 vn = , vn+1 = . 2 2 un =

(10.175)

Here un represents the continuous vibration mode (when the neighboring particles move in-phase) and vn is the envelope of the π mode (when the particles move outof-phase, (see Chapter 10.5)). Let us introduce the continuous coordinate X scaled in such a way that X = nl at the nodes of the lattice, where l is the distance between the particles. Let us also introduce the non-dimensional co-ordinate x = Xπ/L, 0 ≤ x ≤ π, and assume that un (t), vn (t) are discrete approximations to a pair of continuous functions u (x,t), v (x,t), i.e. un (t) = u (x,t)|x=nη , vn (t) = v (x,t)|x=nη , (10.176) where η = πl/L = π/N.

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case

185

We seek a long-wave solution, whose spatial period (or the period of the envelope) is much larger then the distance between the particles and η 1. Using a Taylor series expansion, one can write (±η)i ∂ i u (x,t) , i! ∂ xi i=0 ∞

un±1 (t) = u (x ± η,t) = ∑

(±η)i ∂ i v (x,t) vn±1 (t) = v (x ± η,t) = ∑ . i! ∂ xi i=0 ∞

(10.177)

Adding together and subtracting from each other equations (10.174), and taking into account expressions (10.175)–(10.177), we obtain the macroscopic dynamic equations for u and v. Within an error O η 6 they read 2 2 ∂ u ∂u ∂v 1 4 ∂ 4u ∂ 2u 2∂ u 2 − η − 12εη v v + 2 − − η ∂t 2 ∂ x2 ∂ x2 ∂x ∂x 12 ∂ x4 " # 2 2 ∂ 4u ∂u ∂ u ∂ 3v ∂ 3u ∂ v ∂ 2u ∂v εη 4 v2 4 + 3 2 + 4v + + + (10.178) ∂x ∂x ∂x ∂x ∂ x ∂ x3 ∂ x3 ∂ x ∂ u ∂ v ∂ 2v ∂ 2u ∂ 2v = 0, 6v 2 2 + 6 ∂x ∂x ∂ x ∂ x ∂ x2 " # 2 ∂ 2v ∂u 2 ∂v 2 ∂ 2v 3 2∂ v 2 + 4v + 16εv + η + 12εη v + +v 2 + ∂t 2 ∂ x2 ∂x ∂x ∂x " # 2 2 ∂u 1 4 ∂ 4v ∂ 4v ∂ 2v ∂v η + εη 4 v2 4 + 3 2 + + 4 12 ∂ x ∂x ∂x ∂x ∂x " 2 2 2 # ∂ 2u ∂ v ∂ u ∂ 3u ∂ v ∂ 3v ∂ u ∂ 2u ∂ v + +4v +6 = 0. 3v + ∂ x2 ∂ x2 ∂ x ∂ x3 ∂ x ∂ x3 ∂ x ∂ x2 ∂ x (10.179) It should be noted that acoustic and optical motions are coupled through the nonlinear terms in (10.178), (10.179). The variables η and ε are natural small parameters characterizing, accordingly, the rate of heterogeneity and the rate of non-linearity; η 1, |ε| 1. In a general case, the asymptotic behavior of the model (10.178), (10.173) can depend on a scaling relation between the small parameters η, ε. Imposing ε ∼ η α , one can obtain different asymptotic solutions for different α. Equations (10.178), (10.173) widely used for infinite lattices [371,467]. Their use to describe the dynamics of a finite chain requires further investigation, because, one way or another, the system has to be discretized. It may be more appropriate to use the normal modes of linear oscillations of a discrete system from the very beginning, without going over to a continuous representation.

186

10.18

Linear and Nonlinear Waves in Microstructured Solids

ACOUSTIC BRANCH OF α-FPU LATTICE

Classical continualization of α-FPU lattice [456] or homogenization of a periodically heterogeneous rod [26] leads to the same PDE E1

∂ u ∂ 2u ∂ 4u ∂ 2u ∂ 2u + E + E = ρ . 2 3 ∂ x2 ∂ x ∂ x2 ∂ x4 ∂t 2

(10.180)

Coefficients of Eq. (10.180) have different values for rod and lattice, but in both cases they take into account nonlinearity, dispersion and dissipation effects. It should be noted that dissipation restrains energy transfers between the vibration modes and on a large time scale modes coupling vanishes. In that sense, dispersion and dissipation acting in a nonlinear system may lead to qualitatively similar physical consequences (Zabusky and Kruskal encountered this analogy analysing the FPU problem, see [456]). Therefore, the main conclusions made in [21] for the problem of nonlinear vibrations of a composite rod of finite length can be carried over to the case of acoustic branch of α - FPU lattice. If the distance between particles relatively small in comparison to the amplitude of the vibrations, the effect of internal resonance takes place. It results in periodic energy transfers between different modes and in a modulation of their amplitudes. The resonant modes are coupled in the main approximation, so the truncation to the modes having non-zero initial energy is not possible. If the distance between particles increases, the dispersion supresses the influence of nonlinearity. The energy transfers to higher-order modes are restricted, so truncation to only a few leading modes can provide a reasonable approach. The further increase of dispersion eliminates the energy exchange between the modes and the internal resonances become negligible.

10.19

ANTI-CONTINUUM LIMIT

Consider the discrete nonlinear Schr¨odinger equation in the form 2p iσ jt (t) = ε(σ j+1 − 2σ j + σ j−1 ) + σ j σ j ,

(10.181)

p ∈ N and ε define the coupling constant. The anti-continuum limit [44] corresponds to ε = 0, in which case the Eq. (10.181) becomes an infinite system of uncoupled ODEs.

10.20

2D LATTICE

In order to analyze the 2D case, we use 9-cell square lattice (Fig. 10.8) [316, 361]. The central particle is supposed to interact with eight neighbors in the lattice. The mass centers of four of them are on horizontal and vertical lines, while the mass centers of the other four neighboring particles lie along diagonals. Interactions between the neighboring particles are modeled by elastic springs of three types.

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case

187

Horizontal and vertical springs with rigidity c1 define interaction forces of extension/compression of the material. Governing equations of motion are [361]: mu¨m,n = c1 (um,n−1 − 2um,n + um,n+1 ) + c2 (um−1,n − 2um,n + um+1,n )+ 0.5c0 (um−1,n−1 + um+1,n−1 + um−1,n+1 + um+1,n+1 + vm−1,n−1 − vm+1,n−1 − vm−1,n+1 + vm+1,n+1 − 4um,n ), mv¨m,n = c1 (vm,n−1 − 2vm,n + vm,n+1 ) + c2 (vm−1,n − 2vm,n + vm+1,n )+ 0.5c0 (vm−1,n−1 + vm+1,n−1 + vm−1,n+1 + vm+1,n+1 + um−1,n−1 − um+1,n−1 − um−1,n+1 + um+1,n+1 − 4vm,n ).

(10.182)

Here ui. j , vi. j is the displacement vector for a particle situated at point (xi , y j ), xi = ih, y j = jh, c0 , c1 , c2 are the stiffnesses of diagonal longitudinal, axial longitudinal and axial shear springs, respectively.

Figure 10.8 2D lattice.

The standard continualization procedure for Eq. (10.182) involves introducing a continuous displacement field u(x, y), v(x, y) such that u(xm , yn ) = um,n ; v(xm , yn ) = vm,n , and expanding um±1,n±1 , vm±1,n±1 into Maclaurin series around um,n , vm,n . Second-order continuous theory in respect to the small parameter h is [361]: 2 2 2 ∂ 2u 2∂ u 2∂ u 2 ∂ v = c h + c h + 2c h , 1 2 0 ∂t 2 ∂ x2 ∂ y2 ∂ x∂ y ∂ 2v ∂ 2v ∂ 2v ∂ 2u . m 2 = c1 h2 2 + c2 h2 2 + 2c0 h2 ∂t ∂x ∂y ∂ x∂ y

m

(10.183)

Naturally, one can construct equations of higher order, but, as it is shown in [361], it leads to the principal difficulties. Let us construct semidiscrete approximation.

188

Linear and Nonlinear Waves in Microstructured Solids

Using staggered transformations

one obtains:

uk = (−1)k u, vk = (−1)k v,

(10.184)

∂ 2u ∂ 2u ∂ 2u m 2 = 4 c1 2 + c2 2 , ∂t ∂x ∂y ∂ 2v ∂ 2v ∂ 2v m 2 = 4 c1 2 + c2 2 . ∂t ∂x ∂y

(10.185)

As in 1D case (see Eq. (10.32)), Eq. (10.185) do not contain parameter h2 . The existence of the continuous approximations (10.183) and (10.185) give a possibility to construct the composite equations, which is uniformly suitable in the whole interval of the frequencies and the oscillation forms of the 2D lattice of masses. Let us emphasize, that the composite equations, due to Van Dyke [443], can be obtained as a result of synthesis of the limiting cases. The principal idea of the method of the composite equations can be formulated in the following way [443]: (i) Identify the terms in the differential equations, the neglection of which in the straightforward approximation is responsible for the nonuniformity. (ii) Approximate those terms insofar as possible while retaining their essential character in the region of nonuniformity. In our case the composite equations will be constructed in order to overlap (approximately) with the Eq. (10.183) for long wave solution and with the Eq. (10.185) for short wave solution. As a result of the described procedure one gets 2 2 2 2 2 ∂ u 2 2 ∂ 2∂ u 2∂ u 2 2 ∂ − a h = c h + c h − m 1−a h 1 2 ∂ x2 ∂ y2 ∂t 2 ∂ x2 ∂ y2 ∂ 4u 1 ∂ 2 ∂ 2v (c1 + c2 )h4 γ 2 2 2 + 2c0 h2 1 + , ∂x ∂y 4(c1 + c2 ) ∂t 2 ∂ x∂ y (10.186) 2 2 2 2 2 ∂ v 2 2 ∂ 2 2 ∂ 2∂ v 2∂ v m 1−a h −a h = c1 h + c2 h − ∂ x2 ∂ y2 ∂t 2 ∂ x2 ∂ y2 ∂ 4v 1 ∂ 2 ∂ 2u (c1 + c2 )h4 γ 2 2 2 + 2c0 h2 1 + . ∂x ∂y 4(c1 + c2 ) ∂t 2 ∂ x∂ y Here a2 = 0.25 − π −2 , γ 2 = (4 − π 2 + 8π 2 α 2 )/(4π 2 ). For 1D case from Eq. (10.186) one obtains Eq. (10.50) for u and the same equation for v. For small variability in spatial and time variables Eq. (10.186) can be approximated by Eq. (10.183), for large variability in spatial and time variables Eqs. (10.186) can be approximated by Eq. (10.185). For further results see [18, 25, 32].

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case

10.21

189

MOLECULAR DYNAMICS SIMULATIONS AND CONTINUALIZATION: HANDSHAKE

Molecular dynamics (MD) simulations have become prominent as a tool for elucidating complex physical phenomena, such as solid fracture and plasticity. However, the length and time scales probed using MD are still fairly limited. To overcome this problem, it is possible to use MD only in localized regions in which the atomic-scale dynamics is important, and a continuous simulation method (for example, FEM) everywhere else [452]. Then the problem of coupling MD and continuum mechanics simulations appears. There have been a large number of contributions on the subject, see, e.g., [65, 66] and references therein for a small representative example. From a physical point of view, the problem is related to coupling between either, nonlocal and local continuum mechanics [287], or discrete and continuum models (atomisticto-continuum coupling) [58,346,360,463], or, possibly, local and global models [64]. As a rule, the proposed approach relies on the so-called bridging (overlap) domains (“gluing zones”, “handshake region”), see, e.g., [212]. As noted in [66], these methods are closely related to the overlapping Schwarz methods [422] stemming from the classical alternating Schwarz algorithm. The main idea of these methods can be described as follows: part of the system in the vicinity of the defect or boundary is considered within the framework of discrete media, whereas the rest is assumed to be homogenized. Within the overlap domain, the discrete and homogenized solutions should match in some sense. For example, the discrete solutions may be interpolated (or continuous solutions could be discretized). “In this transition region, approximations are made such as treating finite element nodes as atoms, or vice versa, to accommodate the incompatibility between a nonlocal atomistic description and a local finite element description” [346]. Linear interpolation was used in [58] for addressing this issue, however, other types of interpolation could also be applied. Gluing of local and global solutions may also rely on energy method [66]; another option is the Lagrange multiplier method or augmented Lagrangian method [463]. An alternative approach involves formulation of certain artificial boundary conditions on the interface between discrete and continuous domains. As mentioned in [151], numerical simulations of crystal defects are necessarily restricted to finite computational domains, supplying artificial boundary conditions that emulate the effect of embedding the defect in an effectively infinite crystalline environment. Let us finally discuss problems closely connected with brittle fracture of elastic solids [416–421]. Observe that a continuous model, which does not include material structure, is not suitable since any material crack occurs on the material structure level. This is a reason why some of the essential properties of damages of the classical continuous model theory are not exhibited. For instance, in a discrete medium the propagated waves transport part of the energy from the elastic body into the crack edges. This is why application of nonlocal theories during explosion process modeling (for instance for the composite materials) looks very promising. As it is mentioned in [256], “The continuous development of advanced materials ensures that a “one size fits all” approach will no longer serve the engineering community

190

Linear and Nonlinear Waves in Microstructured Solids

in terms of predicting and preventing fatigue failures and reducing their associated costs”.

10.22

CONTINUALIZATION AND DISCRETIZATION

The connection between these operations is deeply nontrivial, which is shown in detail in the Section 11. Here we dwell on several issues directly related to the approaches described above. In the theory of finite differences the method of differential approximation is widely used [407]. It may be described as follows. Let us compare local operator ∂2 (10.187) −h2 2 ∂x and nonlocal operator ih ∂ 2 sin − . (10.188) 2 ∂x In previous sections we approximated nonlocal operator by infinite number of local ones: ih ∂ ∂2 h4 ∂ 4 h6 ∂ 6 2 4sin − = −h2 2 + − +... (10.189) 2 ∂x ∂x 12 ∂ x4 360 ∂ x6 Using (10.189) one obtains ∂2 ih ∂ h4 ∂ 4 h6 ∂ 6 −h2 2 = 4sin2 − − + −... ∂x 2 ∂x 12 ∂ x4 360 ∂ x6 4

(10.190)

6

Using the same procedure for local operators ∂∂x4 , ∂∂x6 ,..., one obtains nonlocal difference scheme [302]. As result local operator (10.187) can be exactly approximated by infinite numbers of nonlocal ones [429] −h2

10.23

∞ (−1)k π2 ∂ 2 y(x,t) = y (t) + yn (t). n−k ∑ 2 ∂ x2 3 k=−∞,k6=0 k

(10.191)

POSSIBLE GENERALIZATION AND APPLICATIONS AND OPEN PROBLEMS

Demands of engineering and biology [134] require further study of lattices of complex structure: hexagonal, zigzag, kiral, etc. [110, 126, 250, 294, 296, 297, 373], as well as lattices with interaction not only nearest neighbors [249]. The creation of new metamaterials necessitates the study of mass-in-mass systems and lattices with internal resonators [213, 478]. May be, three-point or multy-point Pad´e approximations will be useful for this aim. An interesting objects for study are lattices with large deformations [95, 335, 341, 342]. An example of complex non-smooth nonlinearity is Hertzian contacts describing elastic interactions among grains of a monatomic lattice in the absence of any

Nonlocal, Gradient and Local Models of Elastic Media: 1D Case

191

precompression (i.e., in the so-called sonic-vacuum regime) [335]. We can also mention investigation of discrete breathers and nonlinear normal modes [119]. Surface stress [154] and microstructural instabilities [244] may also be the subject of further study. Note that discrete systems can be described equations with microinhomogeneous coefficients. Homogenization of this system [253] can be used befor continualization. Finally, the most challenging problem is a study of the real interaction of atoms in a chain based on the Mie, Lennard - Johnes or more realistic potentials. The most promising here is combination of MD with quantum mechanics approaches.

and Chaotic 11 Regular Dynamics Based on Continualization and Discretization In this chapter, continualization and discretization algorithms preserving various properties of original difference-differential equations (DDE) and ordinary differential equations (ODE) are proposed and analyzed. Logistic ODE serves as an example of a deterministic system and logistic DDE is a classic example of a simple system with very complicated (chaotic) behavior. Here we present examples of deterministic discretization and chaotic continualization. Continualization procedure is based on the Pad´e approximations. In order to correctly characterize the dynamics of the obtained ODE, we have measured such characteristic parameters of chaotic dynamical systems as the Lyapunov exponents and the Lyapunov dimensions.

11.1

INTRODUCTION

Differential and difference equations are the main tools for mathematical modeling of physical, economic, environmental, and social processes [309, 397, 405]. In order to study differential equations, the entire arsenal of Calculus and Functional Analysis is used. Difference equations are the standard objects for numerical analysis. The relationship between differential and difference equations is nontrivial, and in addition discretization or continualization algorithms often may change fundamentally the nature of their solution. Therefore, the study of approaches that allow these operations to preserve the basic properties of the original systems stands for the hot topic of research. In order to give more light to the considered problem, we choose and analyze the simplest possible examples, i.e., logistic differential and difference equations. Verhulst belongs to the first who studied the following ODE dN N = rN 1 − (11.1) dt K and named it logistic equation [449, 450]. Later investigators proposed variations of the Verhulst equation and they considered the difference logistic equation yielded by logistic models. The first application of ODE (11.1) was connected with population problems, and more generally with the problems arised in ecology. If the Verhulst model is used for describing change 193

194

Linear and Nonlinear Waves in Microstructured Solids

in population size N over time t, then in equation (11.1) r is the so called Malthusian parameter (rate of maximum population growth) and K is the parameter responsible for carrying capacity (i.e., the maximum sustainable population). Equation (11.1) is widely used in problems of ecology, economics, chemistry, medicine, pharmacology, and epidemiology [211, 309, 321, 397, 405, 424]. As a rule, this model is oversimplified for quantitative estimations, but reflects the key qualitative features of processes under consideration. Equation (11.1) can be reduced to the form dx = rx(1 − x), dt

(11.2)

where x = N/K. We introduce the following initial condition x(0) = a.

(11.3)

The Cauchy problem (11.2), (11.3) has the exact solution x=

a . a + (1 − a)e− rt

(11.4)

The discrete logistic equation can be written as follows xn+1 = Rxn (1 − xn ),

(11.5)

where parameter R characterizes the rate of reproduction (growth) of the population. We have R = rh, and parameter h defines the time between consecutive measurements. It should be mentioned that the nonlinear difference equation (11.5) exhibits period doubling bifurcation leading to chaos [211, 321]. In what follows we will analyze a slightly different discrete logistic equation xn+1 − xn = Rxn (1 − xn ).

(11.6)

This equation has two equilibrium positions xn = 0,

(11.7)

xn = 1.

(11.8)

Difference equation (11.6) is obtained from ODE (11.2) using a forward difference scheme for the derivative with the step of discretization h. Ordinary difference equation (O∆E) (11.6) is close enough in behavior to solutions of the following equation [309, 321] xn+1 = xn exp[R(1 − xn )].

(11.9)

Regular and Chaotic Dynamics Based on Continualization and Discretization

195

On the other hand, O∆E (11.9) is close enough in behavior to solutions of equation (11.6) for xn ≈ 1. Initial condition for O∆Es (11.5), (11.6) or (11.9) is taken as follows x0 = a. (11.10) The discrete Cauchy problems regarding (11.5) and (11.10); (11.6) and (11.10), or (11.9) and (11.10) for sufficiently large values of the parameter R exhibits the complicated chaotic behavior of the system [211, 309, 321, 397, 405, 424]. For O∆E (11.6), as it is shown in [405] for R = 2.3, the solution starts to oscillate √ periodically around the value x = 1. This solution is stable as long as R < 6 ≈ 2.449. For R = 2.500 the process comes to steady periodic oscillations with a period of four. It can be mentioned that the chaotic threshold for O∆E (11.9) takes the value of 2.6824 [309, 321]. After description of the objects of our research, we proceed to the formulation of its goals. Both continuous and discrete logistic equations have been extensively investigated. The results of these studies are described in a large number of research including books and review papers [113, 211, 309, 321, 397, 424]. Our study focuses on comparison of the results obtained through the discretization and continualization of nonlinear ODE and O∆E, and we employed logistic equations as convenient and simple examples to study the mentioned problem. The following questions arise while investigating the mentioned problems. First problem: is it possible to discretize ODE (11.2) in such a way that the resulting O∆E has only regular solutions? This practically important issue has been studied resonably well [68, 205, 234, 359], hence we address this issue briefly. On the other hand, many researchers pointed out that discrete logistic models are more adequate to describe the essence of the physical, economic or biological processes because they include chaotic regimes [405]. In this regard, our second problem is: does a continualization of the original O∆E exist that the resulting ODE possesses a chaotic solution? It is difficult to expect that standard continualization, based on the Taylor series, will provide the desired result. However, it can be achieved based on the use of Pad´e approximants (Chapter 10).

11.2

INTEGRABLE O∆E

As it is mentioned in [113], non-invertible maps, such as the logistic map, may display chaos. Therefore, it is of interest to find the transformation of the original discrete logistic equation into a form leading to deterministic solutions. Following the ideas of reference [205], we rewrite O∆E (11.6) into the following form xn+1 − xn = Rxn − Rxn+1 xn . (11.11) This presentation makes it possible to express xn+1 not as polynomial, but as a rational function of xn . Equation (11.11) with initial condition (11.10) has the exact solution of the form a . (11.12) xn = a + (1 − a)(1 + R)−n

196

Linear and Nonlinear Waves in Microstructured Solids

Thus, representation (11.11) allows one to obtain a difference scheme without chaotic behavior.

11.3

CONTINUALIZATION WITH PADE APPROXIMANTS

Let us try to construct a continuous model, describing the chaotic behavior like that exhibited by the original O∆E. As it is mentioned in [113], for generating chaotic behavior a nonlinear ODE must have an order x ≥ 3. To construct a logistic-like ODE with chaotic behavior, additional modifications were included introduction of a piecewise constant argument, delay, and fractional derivative [9, 221, 327, 403, 430]. Here, we use only continualization based on Maclaurin expansion and Pad´e approximations. In order to carry out the continualization of O∆E (11.6), let us introduce the continuous coordinate x scaled in such a way that xn = x(nh). Assuming that x(t) is a slightly changing function, we employ the Maclaurin expansion at the vivinity of equilibrium position (11.7) xn+1 − xn = hxt +

h3 h2 xtt + xttt + ... 2 6

(11.13)

The third-order equation yielded by using the above described procedure takes the following form h3 xttt + 3h2 xtt + 6hxt − 6Rx + 6Rx2 = 0,

(11.14)

and it describes completely regular deterministic trajectories. Let us consider fluctuations around the second equilibrium position of equation (11.6), xn = 1. Changing the variables |yn | 3.0, the largest Lyapunov exponent becomes positive, which indicates the appearance of chaos in the system (Figs 11.14 and 11.15). The obtained values of Lyapunov exponents confirm the earlier conclusions about the absence or presence of chaos in the system. The Lyapunov dimension DL can be calculated using the formula: j

DL = j + ∑ i=1

λi , λ j+1

(11.27)

Regular and Chaotic Dynamics Based on Continualization and Discretization

201

Figure 11.7 Chaotic oscillations for R = 3.05.

Figure 11.8 Chaotic oscillations for R = 3.1.

where j is defined from the following conditions j

∑ λi > 0

i=1

j+1

and

∑ λi < 0.

(11.28)

i=1

For R = 3.05 and R = 3.10 one obtains DL (3.05) = 2.0102 and DL (3.10) = 2.0316, which are consistent with that of a third-order chaotic system [179]. In this section, we looked at some toy problems, the solutions of which lead to interesting conclusions. Logistic ODE serves as example of deterministic system and discrete logistic equation is a classic example of simple system with chaotic behavior. Standart discretization of logistic ODE leads to the difference equation with chaotic behavior. Classic continualization transform discrete logistic equation to the deterministic ODE. However, using fairly simple techniques of nonstandart discretization and enhanced generalized continualization (see Chapter 10), it is possible to construct deterministic O∆E and ODE with chaotic behavior. This expands the possibilities of mathematical modeling of real processes.

202

Linear and Nonlinear Waves in Microstructured Solids

a)

b)

c) Figure 11.9 Numerical solution of the Cauchy problem (equations (11.25) and (11.26)) for R = 3.1. Phase trajectory and Poincar´e section (a) and trajectories in 3D space (b). A very small change in initial conditions created a significantly different outcome (see (c)).

Figure 11.10 Plane phase portrait for R = 3.1.

Regular and Chaotic Dynamics Based on Continualization and Discretization

Figure 11.11 3D phase portrait for R = 3.1.

Figure 11.12 Dynamics of Lyapunov exponents for R = 2.5.

203

204

Linear and Nonlinear Waves in Microstructured Solids

Figure 11.13 Dynamics of Lyapunov exponents for R = 3.0.

Figure 11.14 Dynamics of Lyapunov exponents for R = 3.05.

Regular and Chaotic Dynamics Based on Continualization and Discretization

Figure 11.15 Dynamics of Lyapunov exponents for R = 3.1.

205

References 1. Ablowitz, M.J. and Segur, H. 1981. Solitons and the Inverse Scattering Transform. Philadelphia: SIAM. 2. Abramowitz, M. and Stegun, I.A. (eds.) 1965. Handbook of Mathematical Functions, with Formulas, Graphs, and Mathematical Tables. New York: Dover Publications. 3. Abramyan, A.K., Bessonov, N.M., Indeitsev, D.A., Mochalova, Yu.A. and Semenov, B.N. 2011. Influence of oscillation localization on film detachment from a substrate. Vestnik St. Petersburg Univ.: Math. 44(1):5–12 . 4. Achenbach, J.D. and Herrmann, G. 1968. Dispersion of free harmonic waves in fibrereinforced composites. AIAA J. 6:1832–1836. 5. Achenbach, J.D. and Zhu, H. 1989. Effect of interfacial zone on mechanical behavior and failure of fibre-reinforced composites. J. Mech. Phys. Sol. 7:381–393. 6. Aero, E., Fradkov, A., Andrievsky, B. and Vakulenko, S. 2006. Dynamics and control of oscillations in a complex crystalline lattice. Phys. Lett. A 353(1):24–29. 7. Ahsani, S., Boukadia, R., Droz, C., Claeys, C., Deckers, E. and Desmet W. 2020. Diffusion based homogenization method for 1D wave propagation. Mech. Sys. Sig. Proc., 136:106515. 8. Aifantis, E.C. 1999. Gradient deformation models at nano, micro, and macro scales. ASME J. Eng. Mater. Techn. 121:189–202. 9. Akhmet, M., Altintan, D. and Ergenc, T. 2010. Chaos of the logistic equation with piecewise constant argument. arXiv:1006.4753. 10. Allaire, G., Lamacz, A. and Rauch, J. 2018. Crime pays; homogenized wave equations for long times. Mathematics arXiv:1803.09455 [math.AP]. 11. Andrianov, I.V. 1991. Continuous approximation of higher-frequency oscillation of a chain. Doklady AN Ukr. SSR Ser. A 2:13–15 (in Russian). 12. Andrianov, I.V. 2002. The special feature of limiting transition from a discrete elastic media to a continuous one. J. Appl. Math. Mech. 66(2):261–265. 13. Andrianov, I.V. 2021. Mathematical models in pure and applied mathematics. In: Nonlinear Dynamics of Discrete and Continuous Systems, 15–29. Advanced Structured Materials 139. Abramian A.K., Andrianov I.V., Gaiko V.A. (eds.).Cham: Springer Nature. 14. Andrianov, I.V. and Awrejcewicz, J. 2000. Numbers or understanding: analytical and numerical methods in the theory of plates and shells. Facta Univ., series Mech., Aut. Contr. Robot., University of Nis 2(10):1319–1327. 15. Andrianov, I.V. and Awrejcewicz, J. 2003. Homo analyticus or homo computicus? Facta Univ., series Mech., Aut. Contr. Robot., University of Nis 3(13):765–770. 16. Andrianov, I.V. and Awrejcewicz, J. 2001. New trends in asymptotic approaches: summation and interpolation methods. Appl. Mech. Rev. 54(1):69–92. 17. Andrianov, I.V. and Awrejcewicz, J. 2005. Continuous models for chain of inertially linked masses. Eur. J. Mech. A/Sol. 24(3):532–536. 18. Andrianov, I.V. and Awrejcewicz, J. 2008. Continuous models for 2D discrete media valid for higher-frequency domain. Comp. & Struct. 86:140–144. 19. Andrianov, I.V., Awrejcewicz, J. and Danishevskyy, V.V. 2018. Asymptotical Mechanics of Composites. Modelling Composites without FEM. Berlin: Springer Nature.

207

208

References

20. Andrianov, I.V., Awrejcewicz, J. and Weichert, D. 2010. Improved continuous models for discrete media. Math. Probl. Eng. ID 986242. 21. Andrianov, I.V., Awrejcewicz, J., Danishevskyy, V.V. and Markert, B. 2017. Influence of geometric and physical nonlinearities on the internal resonances of a finite continuous rod with a microstructure. J. Sound Vib. 386:359–371. 22. Andrianov, I.V., Bolshakov, V.I., Danishevskyy, V.V. and Weichert, D. 2008. Higherorder asymptotic homogenization and wave propagation in periodic composite materials. Proc. R. Soc. A 464:1181–1201. 23. Andrianov, I.V., Danishevskyy, V.V. and Kalamkarov, A.L. 2013. Vibration localization in one-dimensional linear and nonlinear lattice: discrete and continuum models. Nonl. Dyn. 72:37–48. 24. Andrianov, I.V., Danishevskyy, V.V., and Markert, B. 2015. Nonlinear vibrations and mode interactions for a continuous rod with microstructure. J. Sound Vib. 351:268–281. 25. Andrianov, I.V., Danishevskyy, V.V. and Rogerson, G. 2018. Elastic waves in periodically heterogeneous two-dimensional media: locally periodic and anti-periodic modes. Proc. Roy. Soc. A 474:2215. 26. Andrianov, I.V., Danishevskyy, V.V. and Rogerson, G. 2018. Internal resonances and modes interactions in non-linear vibrations of viscoelastic heterogeneous solids. J. Sound Vib. 433:55–64. 27. Andrianov, I.V., Danishevskyy, V.V. and Rogerson, G. 2020. Vibrations of nonlinear elastic lattices: low- and high-frequency dynamic models, internal resonances and modes coupling. Proc. R. Soc. A 476:20190532. 28. Andrianov, I.V., Danishevskyy, V.V., Kaplunov, J. and Markert, B. 2019. Wide frequency higher-order dynamic model for transient waves in a lattice. In: Problems of Nonlinear Mechanics and Physics of Materials, Advanced Structured Materials 94, Andrianov, I.V., Manevich, A.I., Mikhlin, Yu.V.,Gendelman, O.V. (eds.) Springer Nature, pp. 3–12. 29. Andrianov, I.V., Danishevskyy, V.V., Ryzhkov, O.I. and Weichert, D. 2013. Dynamic homogenization and wave propagation in a nonlinear 1D composite material. Wave Motion 50:271–281. 30. Andrianov, I.V., Danishevskyy, V.V., Topol, H. and Luyt, A.S 2018. Shear wave propagation in layered composites with degraded matrices at locations of imperfect bonding. Wave Motion 78:9–31. 31. Andrianov, I.V., Danishevskyy, V.V., Topol, H. and Rogerson, G. 2016. Propagation of Floquet-Bloch shear waves in viscoelastic composites: analysis and comparison of interface/interphase models for imperfect bonding. Acta Mech. 228:1177–1196. 32. Andrianov, I.V., Danishevskyy, V.V. and Weichert, D. 2010. Continuous model of 2D discrete media based on composite equations. Acoust. Phys. 56(6):807–810. 33. Andrianov, I.V., Danishevskyy, V.V. and Weichert, D. 2008. Simple estimations on effective transport properties of a random composite material with cylindrical fibres. ZAMP 59(5):889–903. 34. Andrianov, I.V., Lesnichaya, V.A. and Manevitch, L.I. 1985. Homogenization Methods in Statics and Dynamics of Ribbed Shells. Moscow: Nauka (in Russian). 35. Andrianov, I.V. and Manevitch, L.I. 2002. Asymptotology: Ideas, Methods, and Applications. Dordrecht: Kluwer Academic Publishers. 36. Andrianov, I. and Mityushev, V. 2018. Exact and “exact” formulae in the theory of composites. In: Modern Problems in Applied Analysis. Dryga´s, P., Rogosin, S. (eds.). Birkh¨auser, pp. 15–34.

References

209

37. Andrianov, I., Starushenko, G., Kvitka, S. and Khajiyeva, L. 2019. The Verhulst-Like equations: Integrable O∆E and ODE with chaotic behavior. Symmetry 11:1446. 38. Arvin, H. and Bakhtiari-Nejad, F. 2013. Nonlinear modal interaction in rotating composite Timoshenko beams. Compos. Struct. 96:121–134. 39. Askar, A. 1985. Lattice Dynamical Foundations of Continuum Theories. Elasticity, Piezoelectricity, Viscoelasticity, Plasticity. Singapore: World Scientific. 40. Askes, H. and Aifantis, E.C. 2011. Gradient elasticity in statics and dynamics: An overview of formulations, length scale identification procedures, finite element implementations and new results. Int. J. Solids Struct. 48(13):1962–1990. 41. Askes, H. and Sluys, L.J. 2002. Explicit and implicit gradient series in damage mechanics. Eur. J. Mech. A/Sol. 21:379–390. 42. Askes, H. and Metrikine, A.V. 2002. One-dimensional dynamically consistent gradient elasticity models derived from a discrete microstructure. Part 2: Static and dynamic response. Eur. J. Mech. A/Sol. 21:573–588. 43. Askes, H., Metrikine, A.V., Pichugin, A.V. and Bennett, T. 2008. Four simplified gradient elasticity models for the simulation of dispersive wave propagation. Phil. Mag. 88(28-29):3415–3443. 44. Aubry, S. 1995. Anti-integrability in dynamical and variational problems. Physica D. 86:284–296. 45. Auffray, N., Le Quang, H. and He Q.C. 2013. Matrix representations for 3D straingradient elasticity. J. Mech. Phys. Sol. 61(5):1202–1223. 46. Bacca, M., Bigoni, D., Dal Corso, F. and Veber, D. 2013. Mindlin second-gradient elastic properties from dilute two-phase Cauchy-elastic composites. Part II: Higherorder constitutive properties. Int. J. Solids Struct. 50:4020–4029. 47. Baker, G.A. jr. and Graves-Morris, P. 1996. Pad´e Approximants (2nd ed.). Cambridge, NY: Cambridge University Press. 48. Bakhvalov, N.S. and Eglit, M.E. 1992. Variational properties of averaged equations for periodic media. Proc. Steklov Inst. Math. 192:3–18. 49. Bakhvalov, N.S. and Eglit, M.E. 1993. Averaging of the equations of the dynamics of composites of slightly compressible elastic components. Comput. Math. Math. Phys. 33(7):939–952. 50. Bakhvalov, N.S. and Eglit, M.E. 1993. Homogenization of dynamic problems singularly depending on small parameters. Proc. Second Workshop on Composite Media and Homogenization Theory, Trieste, pp. 17–35. 51. Bakhvalov, N.S. and Eglit, M.E. 1994. An estimate of the error of averaging the dynamics of small perturbations of very inhomogeneous mixtures. Comput. Math. Math. Phys. 34(3):333–349. 52. Bakhvalov, N.S. and Eglit, M.E. 1995. The limiting behaviour of periodic media with soft-modular inclusions. Comput. Math. Math. Phys. 35(6):719–729. 53. Bakhvalov, N.S. and Eglit, M.E. 2000. Long-wave asymptotics with dispersion for wave propagation in stratified media. I. Waves orthogonal to the layers. Russ. J. Num. Anal. Math. Modell. 15(1):3–18. 54. Bakhvalov, N.S. and M.E. Eglit. 2000. Long-wave asymptotics with dispersion for wave propagation in stratified media. II. Waves in arbitrary directions. Russ. J. Num. Anal. and Math. Modell. 15(3-4):225–236. 55. Bakhvalov, N. and Panasenko, G. 1989. Averaging Processes in Periodic Media. Mathematical Problems in Mechanics of Composite Materials. Dordrecht: Kluwer.

210

References

56. Bakhvalov, N.S., Sandrakov, G.V. and Eglit, M.E. 1996. Mathematical study of sound waves propagation progress in mixtures. Moscow Univ. Math. Bull. 51(6):5–7. 57. Bardzokas, D.I., Filshtinsky, M.L. and Filshtinsky, L.A. 2007. Mathematical Methods in Electro-Magneto-Elasticity. Springer, Berlin. 58. Bauman, T., Ben Dhia, H., Elkhodja, N., Oden, J.T. and Prudhomme, S. 2008. On the application of the Arlequin method to the coupling of particle and continuum models. Comp. Mech. 42:511–530. 59. Bedford, A. and Drumheller, D.S. 1983. Theories of immiscible and structured mixtures. Int. J. Eng. Sci. 21:863–960. 60. Bedford, A. and Drumheller, D.S. 1994. Introduction to Elastic Wave Propagation. New York: Wiley. 61. Bedford, A and Stern, M. 1971. Toward a diffusing continuum theory of composite materials. J. Appl. Mech. 38:8–14. 62. Belashov, Yu.V. and Vladimirov, S.V. 2005. Solitary Waves in Dispersive Complex Media. Berlin: Springer. 63. Belyaev, A. 2011. On implicit image derivatives and their applications. In: Proceedings of the British Machine Vision Conference. Hoey, J., McKenna, St., Trucco, E. (eds.). BMVA Press, pp. 72.1–72.12. 64. Ben Dhia, H. 2006. Global-local approaches: the Arlequin framework. Europ. J. Comp. Mech. 15:67–80. 65. Ben Dhia, H. 2008. Further insights by theoretical investigations of the multiscale Arlequin method. Int. J. Multisc. Comp. Eng. 6:215–232. 66. Ben Dhia, H. and Rateau, G. 2005. The Arlequin method as a flexible engineering design tool. Int. J. Numer. Met. Eng. 62:1442–1462. 67. Benaroya, H. 1997. Waves in periodic structures with imperfections. Compos. B. 28:143–152. 68. Bender, C.M. and Tovbis, A. 1997. Continuum limit of lattice approximation schemes. J. Math. Phys. 38:3700–3717. 69. Benilov, E.S., Grimshaw, R. and Kuznetsova, E.P. 1993. The generation of radiating waves in a singularly-perturbed KdV equation. Phys. D. 69:270–278. 70. Bensoussan, A., Lions, J.-L. and Papanicolaou, G. 1978. Asymptotic Analysis for Periodic Structures. Amsterdam: North-Holland. 71. Benveniste, Y. 1985. The effective mechanical behavior of composite materials with imperfect contact between constituents. Mech. Mater. 4:197–208. 72. Benjamin, T.B., Bona, J.G. and Mahoney, J.J. 1972. Model equations for long waves in nonlinear dispersive systems. Phil. Trans. Roy. Soc. A. 272:47–78. 73. Beran, M.J. 1968. Statistical Continuum Theories. New York: Wiley Interscience. 74. Berezovski, A., Engelbrecht, J. and Berezovski, M. 2011. Waves in microstructured solids: a unified viewpoint of modeling. Acta Mech. 220:349–363. 75. Berlyand, L. and Mityushev, V. 2001. Generalized Clausius-Mossotti formula for random composite with circular fibres. J. Stat. Phys. 102:115–145. 76. Berlyand, L. and Mityushev, V. 2005. Increase and decrease of the effective conductivity of two phase composites due to polydispersity. J. Stat. Phys. 118:481–509. 77. Bhatnagar, P.I. 1979. Nonlinear Waves in One-Dimensional Dispersive Systems. Oxford: Clarendon Press. 78. Bigoni, D. and Drugan, W.J. 2007. Analitical derivation of Cosserat moduli via homogenization of heterogeneous elastic materials. J. Appl. Mech. 74:741–753. 79. Bishop, R.E.D. 1952. Longitudinal waves in beams. Aeronaut. Quart. 3(4):280–293.

References

211

80. Blanc, X., Le Bris, C. and Lions, P.-L. 2002. From molecular models to continuum mechanics. Arch. Rational Mech. Anal. 164, 341–381. 81. Blanc, X., Le Bris, C. and Lions, P.L. 2007. Atomistic to continuum limits for computational material science. ESAIM: Math. Mod. Num. Anal. 41(2):391–426. ¨ die Quantenmechanik der Elektronen in Kristallgittern. Z. Phys. 82. Bloch, F. 1928. Uber 52:555–600. 83. Bobrovnitskii, Yu.V. 2011. Features of normal wave dispersion in periodic structures. Acoust. Phys. 57(4):442–446. 84. Boertjens, G.J. and van Horssen, W.T. 1998. On mode interactions for a weakly nonlinear beam equation. Nonlin. Dyn. 17:23–40. 85. Boertjens, G.J. and van Horssen, W.T. 2000. An asymptotic theory for a weakly nonlinear beam equation with a quadratic perturbation. SIAM J. Appl. Math. 60:602–632. 86. Born, M. and Huang, K. 1988. Dynamical Theory of Crystal Lattices. Oxford: Oxford Univ. Press. 87. Born, M. and Wolf, E. 1964. Principles of Optics: Electromagnetic Theory of Propagation, Interference and Diffraction of Light. Oxford: Pergamon Press. 88. Boussinesq, J.V. 1872. Th´eorie des ondes et des remous qui se propagent le long d’un canal rectangulaire horizontal, en communiquant au liquide contenu dans ce canal des vitesses sensiblement pareilles de la surface au fond. J. Math. Pures Appl. 17:55–108. 89. Boutin, C. 1995. Microstructural influence on heat conduction. Int. J. Heat Mass Transf. 38:3181–3195. 90. Boutin, C. 1996. Microstructural effects in elastic composites. Int. J. Sol. Struct. 33:1023–1051. 91. Boutin, C. 2000. Study of permeability by periodic and self-consistent homogenization. Eur. J. Mech. A/Sol. 19:603–632. 92. Boutin, C. and Auriault, J.L. 1993. Rayleigh scattering in elastic composite materials. Int. J. Eng. Sci. 31:1669–1689. 93. Bowen, R.M. 1976. Theory of mixtures. In: Continuum Physics: Mixtures and EM Field Theories. Eringen, A.C. (ed.) New York: Academic Press, pp. 2–129. 94. Braides, A. 2000. Non-local variational limits of discrete systems. Commun. Contemp. Math. 2:285–297. 95. Braun, O.M. and Kivshar, Y.S. 2004. The Frenkel-Kontorova Model: Concepts, Methods, and Applications. Berlin, Heidelberg: Springer-Verlag. 96. Brezinski, C. 2004. Extrapolation algorithms for filtering series of functions, and treating the Gibbs phenomenon. Numer. Algor. 36:309–329. 97. Brillouin, L. 1960. Wave Propagation and Group Velocity. New York: Academic Press. 98. Brillouin, L. 2003. Wave Propagation in Periodic Structures: Electric Filters and Crystal Lattices, 2nd edn. Mineola, New York: Dover Publications. 99. Brocchini, M. 2013. A reasoned overview on Boussinesq-type models: the interplay between physics, mathematics and numerics. Proc. R. Soc. A. 469:20130496. 100. Bryant, J.D., David, T., Gaskell, P.H., King, S. and Lond, G. 1989. Rheology of bovine bone marrow. Proc. Inst. Mech. Eng. 203:71–75. 101. Bykov, V.G. 2015. Nonlinear waves and solitons in models of fault block geological media. Russ. Geol. Geophys. 56(5):793–803. 102. Cai, C.W., Chan, H.C. and Cheung, Y.K. 1997. Localized modes in periodic systems with a nonlinear disorders. J. Appl. Mech. 64:940–945. 103. Cai, C.W., Chan, H.C. and Cheung, Y.K. 2000. Localized modes in a two-degreecoupling periodic system with a nonlinear disordered subsystem. Chaos, Solitons & Fractals. 11:1481–1492.

212

References

104. Cai, C.W., Cheung, Y.K. and Chan, H.C. 1995. Mode localization phenomena in nearly periodic systems. J. Appl. Mech. 62:141–149. 105. Cai, G.Q. and Lin, Y.K. 1990. Localization of wave propagation in disordered periodic structures. AIAA J. 29:450–456. 106. Cai, C.W., Liu, J.K. and Chan, H.C. 2003. Exact analysis of localized modes in biperiodic mono-coupled mass-spring systems with a single disorder. J. Sound Vib. 262:1133–1152. 107. Cao, W. and Qi, W. 1995. Multisource excitations in a stratified biphase structure. J. Appl. Phys. 78:4640–4646. 108. Cao, W. and Qi, W. 1995. Plane wave propagation in finite 2-2 composites. J. Appl. Phys. 78:4627–4632. 109. Carta, G. and Brun, M. 2012. A dispersive homogenization model based on lattice approximation for the prediction of wave motion in laminates. J. Appl. Mech. 79(2):021019-1–021019-8. 110. Carta, G., Brun, M., Movchan, A.B., Movchan, N.V. and Jones, I.S. 2014. Dispersion properties of vortex-type monatomic lattices. Int. J. Sol. Struct. 51:2213–2225. 111. Catheline, S., Gennisson, J.-L. and Fink, M. 2003. Measurement of elastic nonlinearity of soft solid with transient elastography. JASA 114:3087–3091. 112. Cattani, C. and Rushchitsky, J., 2007. Wavelet and Wave Analysis as Applied to Materials with Micro or Nanostructure. Singapore: World Scientific. 113. Cencini, M., Cecconi, F. and Vulpiani, A. 2009. Chaos: From Simple Models to Complex Systems. Singapore: World Scientific. 114. Chakraborty, G. and Mallik, A.K. 2001. Dynamics of a weakly non-linear periodic chain. Int. J. Non-Lin. Mech. 36:375–389. 115. Chang, C.S., Askes, H. and Sluys, L.J. 2002. Higher-order strain/higher-order stress gradient models derived from a discrete microstructure, with application to fracture. Engn. Fract. Mech. 69:1907–1924. 116. Charlotte, M. and Truskinovsky, L. 2008. Towards multi-scale continuum elasticity theory. Continuum Mech. Thermodyn. 20:133. 117. Charlotte, M. and Truskinovsky, L. 2012. Lattice dynamics from a continuum viewpoint. J. Mech. Phys. Sol. 60(8):1508–1544. 118. Chechin, G.M. and Sakhnenko, V.P. 1998. Interactions between normal modes in nonlinear dynamical systems with discrete symmetry. Exact results. Physica D 117:43–76. 119. Chechin, G.M. and Dzhelauhova, G.S. 2009. Discrete breathers and nonlinear normal modes in monoatomic chains. J. Sound Vib. 322:490–512. 120. Chen, W. and Fish, J. 2001. A dispersive model for wave propagation in periodic heterogeneous media based on homogenization with multiple spatial and temporal scales. J. Appl. Mech. 68:153–161. 121. Cherednichenko, K.D. and Smyshlyaev, V.P. 2004. On full two-scale expansion of the solutions of nonlinear periodic rapidly oscillating problems and higher-order homogenised variational problems. Arch. Rat. Mech. Anal. 174:385–442. 122. Cherkaev, E. and Ou, M.-J.Y. 2008. Dehomogenization: reconstruction of moments of the spectral measure of the composite. Inver. Probl. 24:065008. 123. Christensen, R.M. 2005. Mechanics of Composite Materials, 2nd edn. Mineola, New York: Dover Publications. 124. Claude, Ch., Kivshar, Yu.S., Kluth, O. and Spatschek, K.H. 1993. Moving localized modes in nonlinear lattices. Phys. Rev. B. 47(21):14228–14233.

References

213

125. Collins, M.A. 1981. A quasi-continuum approximation for solitons in an atomic chain. Chem. Phys. Lett. 77(2):342–347. 126. Colquitt, D.J., Danishevskyy, V.V. and Kaplunov, J. 2019. Composite dynamic models for periodically heterogeneous media. Math. Mech. Sol. 24(9):2663–2693. 127. Colquitt, D.J., Jones, I.S., Movchan, N.V. and Movchan, A.B. 2011. Dispersion and localization of elastic waves in materials with microstructure. Proc. R. Soc. A 467:2874– 2895. 128. Conca, C. and Lund, F. 1999. Fourier homogenization method and the propagation of acoustic waves through a periodic vortex array. SIAM J. Appl. Math. 59(5):1573–1581. 129. Cosserat, E. and Cosserat, F. 1909. Th´eorie des Corps D´eformables. Paris: Libraire Scientifique A. Hermann et Fils. 130. Craster, R.V., Kaplunov, J. and Pichugin, A.V. 2010. High frequency homogenization for periodic media. Proc. R. Soc. A. 466:2341–2362. 131. Craster, R.V., Kaplunov, J. and Postnova, J. 2010. High-frequency asymptotics, homogenization and localization for lattices. Q.J. Mech. Appl. Math. 63(4):497–520. 132. Dal Maso, G. 1993. An Introduction to Γ-Convergence. Boston: Birkh¨auser. 133. Daya, E.M. and Potier-Ferry, M. 2001. Vibrations of long repetitive structures by a double scale asymptotic method. Struct. Eng. Mech. 12:215–230. 134. Dauxois, T. 1991. Dynamics of breather modes in a nonlinear “helicoidal” model of DNA. Phys. Lett. A 159:390–395. 135. Deift, P. and McLaughlin, K.T.R. 1998. A Continuum Limit of the Toda Lattice. Providence: AMS. 136. Del Piero, G. and Truskinovsky, L. 1998. A one-dimensional model for localized and distributed failure. J. de Physique IY France 8(82):199–210. 137. Deymier, P.A. (ed.) 2013. Acoustic Metamaterials and Phononic Crystals. Berlin: Springer-Verlag. 138. Dirac, P.A.M. 1929. Quantum Mechanics of many-electron systems. Proc. R. Soc. London A. 123(729):714–733. 139. Dodd, R.K., Eilbeck, J.C., Gibbon, J.D. and Morris, H.C. 1982. Solitons and Nonlinear Wave Equations. London: Academic Press. 140. Dreiden, G.V., Khusnutdinova, K.R., Samsonov, A.M. and Semenova, I.V. 2010. Splitting induced generation of soliton trains in layered waveguides. J. Appl. Phys. 107:034909. 141. Dreiden, G.V., Porubov, A.V., Samsonov, A.M., Semenova, I.V. and Sokurinskaya, E.V. 1995. Experiments in the propagation of longitudinal strain solitons in a nonlinearly elastic rod. Tech. Phys. Lett. 21:415–417. 142. Dreiden, G.V., Samsonov, A.M. and Semenova, I.V. 2014. Observation of bulk strain solitons in layered bars of different materials. Tech. Phys. Lett. 40(12):1140–1141. 143. Driscoll, T. and Fornberg, B. 2001. A Pad´e-based algorithm for overcoming the Gibbs phenomenon. Numer. Algorithm. 26:77–92. 144. Drumheller, D.S. and Bedford, A. 1974. Wave propagation in elastic laminates using a second order microstructure theory. Int. J. Sol. Struct. 10:61–76. 145. Drumheller, D.S. and Sutherland, H.J. 1973. A lattice model for stress wave propagation in composite materials. J. Appl. Mech. 40:157–164. 146. Drygas, P., Mityushev, V., Gluzman, S. and Nawalaniec, W. 2020. Applied Analysis of Composite Media: Analytical and Computational Approaches for Materials Scientists and Engineers. New York: Elsevier.

214

References

147. Dykhne, A.M. 1971. Conductivity of a two-dimensional two-phase system. Sov. Phys. JETP 32:63–65. 148. Egle, D.M. and Bray, D.T. 1976. Measurement of acoustoelastic and third-order elastic constants for rail steel. JASA 60:741–744. 149. Eglit, M.E. 1998. New models arising in the averaged description of microinhomogeneous media. Proc. Steklov Inst. Math. 223:94–104. 150. Eglit, M.E. 2010. Dispersion of elastic waves in microinhomogeneous media and structures (A review). Acoust. Phys. 56(6):989–995. 151. Ehrlacher, V., Ortner, C. and Shapeev, A.V. 2015. Analysis of boundary conditions for crystal defect atomistic simulations. arXiv:1306. 5334v3. 152. Engelbrecht, J. 1997. Nonlinear Wave Dynamics: Complexity and Simplicity. Dordrecht, Boston: Kluwer. 153. Engelbrecht, J. and Braun, M. 1998. Nonlinear waves in nonlocal media. Appl. Mech. Rev. 51:475–488. 154. Eremeyev, V.A. and Sharma, B.L. 2019. Anti-plane surface waves in media with surface structure: Discrete vs. continuum model. Int. J. Eng. Sci. 143:33–38. 155. Eringen, A.C. 1987. Theory of nonlocal elasticity and some applications. Res. Mech. 21:313–342. 156. Eringen, A.C. 1992. Vistas on nonlocal continuum Physics. Int. J. Eng. Sci. 30(10):1551–1565. 157. Eringen, A.C. 1999. Microcontinuum Field Theories. I. Foundations and Solids. New York: Springer-Verlag. 158. Erofeev, V.I. 2003. Wave Processes in Solids with Microstructure. Singapore: World Scientific. 159. Espinosa, H.D., Dwivedi, S.K. and Lu, H.-C. 2000. Modelling impact induced delamination of woven fibre reinforced composites with contact/cohesive laws. Comput. Meth. Appl. Mech. Eng. 183:259–290. 160. Espinosa, H.D., Zavattieri, P.D. and Dwivedi, S.K. 1998. A finite deformation continuum/discrete model for the description of fragmentation and damage in brittle materials. J. Mech. Phys. Sol. 46:1909–1942. 161. Fanga, X.-Q., Liua, J.-X., Niea, G.-Q. and Hub, Ch. 2010. Propagation of flexural waves and localized vibrations in the strip plate with a layer using Hamilton system. Eur. J. Mech. A/Sol. 29:152–157. 162. Feng, B.F. and Kawahara, T. 2007. Discrete breathers in two-dimensional nonlinear lattices. Wave Motion 45(1-2):68–82. 163. Feng, B.F., Doi, Y. and Kawahara, T. 2004. Quasi-continuum approximation for intrinsic localized modes in Fermi-Pasta-Ulam lattices. J. Phys. Soc. Jpn. 73:2100–2111. 164. Feng, B.F., Doi, Y. and Kawahara, T. 2006. A regularized model equation for discrete breathers in anharmonic lattices with symmetric nearest-neighbor potentials. Phys. D 214:33–41. 165. Filimonov, A.M. 1992. Some unexpected results on the classical problem of the string with N beads. The case of multiple frequencies. C. R. Acad. Sci. Paris 1(315): 957–961. 166. Filimonov, A.M. 1996. Continuous approximations of difference operators. J. Difference Eq. Appl. 2(4):411–422. 167. Filimonov, A.M. and Myshkis, A.D. 1998. Asymptotic estimate of solution of one mixed difference-differential equation of oscillations theory. J. Difference Eq. Appl. 4:13–16.

References

215

168. Filimonov, A.M., Mao, X. and Maslov, S. 2000. Splash effect and ergodic properties of solution of the classic difference - differential equation. J. Difference Eq. Appl. 6:319– 328. 169. Findlin, A.Ya. 2007. Peculiarities of the use of computational methods in applied mathematics (on global computerization and common sense). In: Blekhman, I.I., Myshkis, A.D., Ya.G. Panovko. 2007. Applied Mathematics: Subject, Logic, Peculiarities of Approaches. With Examples from Mechanics. Moscow, URSS: 350–358 (in Russian). 170. Fish, J. and Chen, W. 2001. Higher-order homogenization of initial/boundary-value problem. J. Eng. Mech. 127:1223–1230. 171. Fish, J. and Chen W. 2004. Space-time multiscale model for wave propagation in heterogeneous media. Comput. Meth. Appl. Mech. Eng. 193:4837–4856. 172. Flach, S. and Kladko, K. 1996. Perturbation analysis of weakly discrete kinks. Phys. Rev. E 54:2912–2916. 173. Flach, S. and Willis, C.R. 1993. Asymptotic behavior of onedimensional nonlinear discrete kink-bearing systems in the continuum limit: Problem of nonuniform convergence. Phys. Rev. E 47:4447–4456. 174. Fleck, N.A. and Hutchinson, J.W. 1993. A phenomenological theory for gradient effects in plasticity. J. Mech. Phys. Sol. 41:1825–1857. 175. Fletcher, C.A.J. 1984. Computational Galerkin Methods. Berlin: Springer. 176. Floquet, G. 1883. Sur les e´ quations diff´erentielles lin´eaires a´ coefficients p´eriodiques. ´ Ann. sc. l’Ecole Norm. Sup´er., S´er 2. 12:47–88. 177. Fl¨ugge, W. 1975. Viscoelasticity. New York: Springer. 178. Franzevich, I.N., Voronov, F.F. and Bakuta, S.A. 1982. Elastic Constants and Modules of Elasticity of Metals and Nonmetals. Reference Book. Kiev: Naukova Dumka (in Russian). 179. Frederickson, P., Kaplan, J.L., Yorke, E.D. and Yorke, J.A. 1983. The Liapunov dimension of strange attractors. J. Differ. Eq. 49:185–207. 180. Galka, A., Telega, J.J. and Tokarzewski, S. 1999. A contribution to evaluation of effective moduli of trabecular bone with rod-like microstructure. J. Theor. Appl. Mech. 37:707–727. 181. Gambin, B. and Kr¨oner, E. 1989. High order terms in the homogenized stressstrain relation of periodic elastic media. Phys. Stat. Sol. 151:513–519. 182. Gao, Q., Wu, F., Zhang, H.W., Zhong, W.X., Howson, W.P. and Williams, F.W. 2012. Exact solutions for dynamic response of a periodic spring and mass structure. J. Sound Vib. 331(5):1183–1190. 183. Ghavanloo, E., Fazelzadeh, S.A. and Rafii-Tabar, H. 2020. Formulation of an efficient continuum mechanics-based model to study wave propagation in one-dimensional diatomic lattices. Mech. Res. Comm. 103:103467. 184. Giannoulis, J. and Mielke, A. 2004. The nonlinear Schr¨odinger equation as a macroscopic limit for an oscillator chain with cubic nonlinearities. Nonlinearity 17:551–565. 185. Gibson, J.L. and Ashby, M.P. 1988. Cellular Solids: Structure and Properties. New York: Pergamon Press. 186. Gleik, J. 1987. Chaos: Making a New Science. New York: Viking Penguin. 187. Golub, M.V., Fomenko, S.I., Bui, T.Q., Zhang, Ch. and Wang, Y.-S. 2012. Transmission and band gaps of elastic SH waves in functionally graded periodic laminates. Int. J. Sol. Struct. 49:344–354. 188. Golub, M.V., Zhang, Ch. and Wang, Y.-S. 2012. SH-wave propagation and scattering in periodically layered composites with a damaged layer. J. Sound Vib. 331:1829–1843.

216

References

189. Goupillaud, P.L. 1961. An approach to inverse filtering of near-surface layer effectc from seismic records. Geophysics 26(6):754–760. 190. Grigolyuk, E.I. and Selezov, I.I. 1973. Nonclassical Theories of Vibrations of Beams, Plates and Shells. Moscow: VINITI (in Russian). 191. Guckenheimer, J. 1998. Computer simulation and beyond for the 21st century. Notices AMS 45:1120–1123. 192. Guckenheimer, J. 1998. Numerical computation in the information age. SIAM NEWS 31(5). 193. Guenneau, S., Poulton, C.G. and Movchan, A.B. 2003. Oblique propagation of electromagnetic and elastic waves for an array of cylindrical fibres. Proc. R. Soc. Lond. A. 459:2215–2263. 194. Guo, X.E. 2001. Mechanical properties of cortical bone and cancellous bone tissue. In: Cowin, S.C. (ed.) Bone Mechanics Handbook. Boca Raton: CRC Press, pp. 10-1–1023. 195. Gusev, A.I., Rempel, A.A. and Magerl, A.J. 2001. Disorder and Order in Strongly Nonstoichiometric Compounds: Transition, Metal Carbides, Nitrides, and Oxides. Berlin, New York: Springer. 196. Guz, A.N. and Nemish, Yu.N. 1987. Perturbation of boundary shape in continuum mechanics. Sov. Appl. Mech. 23(9):799–822. 197. Guz, A.N. and Shulga, N.A. 1992. Dynamics of laminated and fibrous composites. Appl. Mech. Rev. 45:35–60. 198. Hadjesfandiari, A.R. and Dargush, G.F. 2011. Couple stress theory for solids. Int. J. Sol. Struct. 48:2496–2510. 199. Hadjesfandiari, A.R. and Dargush, G.F. 2013. Fundamental solutions for isotropic sizedependent couple stress elasticity. Int. J. Solids Struct. 50:1253–1265. 200. Hamming, R.W. 1973. Numerical Methods for Scientists and Engineers, 2nd ed. New York: McGraw Hill. 201. Hao, H.-Y. and Maris, H.J. 2001. Experiments with acoustic solitons in crystalline solids. Phys. Rev. B. 64:064302. 202. Hashin, Z. 2002. Thin interphase/imperfect interface in elasticity with application to coated fibre composites. J. Mech. Phys. Sol. 50:2509– 2537. 203. Hegemier, G., Gurtman, G.A. and Nayfeh, A.H. 1973. A continuum mixture theory of wave propagation in laminated and fibre reinforced composites. Int. J. Sol. Struct. 9:395–414. 204. Hellinger, E. 1914. Die allgemeinen Ans¨atze der Mechanik der Kontinua. Enz. Mat. Wiss. 4(4):602–694. 205. Herbst, B.M. and Ablowitz, M.J. 1993. Numerical chaos, symplectic intergators, and exponentially small splitting distances. J. Comput. Phys. 105:122–132. 206. Hermann, G., Kaul, R.K. and Delph, T.G. 1978. On continuum modelling of the dynamic behaviour of layered composites. Archiv. Mech. 28(3):405–421. 207. Hersch, J. 1961. Propri´et´es de convexit´e du type de Weye pour des probl´emes de vibration ou d’´equilibre. ZAMP 12: 298–322. 208. Hobart, R. 1965. Peierls stress dependence on dislocation width. J. Appl. Phys. 36:1944–1948. 209. Hodges, C.H. and Woodhouse, J. 1986. Theories of noise and vibration transmission in complex structures. Rep. Prog. Phys. 49:107–170. 210. Hollister, S.J., Fyhire, D.P., Jepsen, K.J. and Goldstein, S.A. 1991. Application of homogenization theory to the study of trabecular bone mechanics. J. Biomech. 24:825– 839.

References

217

211. Hoppensteadt, F.C. and Hyman, J.M. 1977. Periodic solutions of a logistic difference equation. SIAM J. Appl. Math. 32:73–81. 212. Hu, H., Damil N. and Potier-Ferry, M. 2011. A bridging technique to analyze the influence of boundary conditions on instability patterns. J. Comp. Phys. 230:3753–3764. 213. Huang, H.H., Sun, C.T. and Huang, G.L. 2009. On the negative effective mass density in acoustic metamaterials. Int. J. Eng. Sci. 47:610–617. 214. Huges, D.S. and Kelly, I.L. 1953. Second-order elastic deformation of solids. Phys. Rev. 92:1145–1156. 215. Hughes, E.R., Leighton, T.G., Petley, G.M., White, P.R. and Chivers, R.C. 2003. Estimation of critical and viscous frequencies for Biot theory in cancellous bone. Ultrasonics 41:365–368. 216. Hussein, M.I., Hulbert, G.M. and Scott, R.A. 2006. Dispersive elastodynamics of 1D banded materials and structures: analysis. J. Sound Vib. 289:779–806. 217. Hussein, M.I., Leamy, M.J. and Ruzzene, M. 2014. Dynamics of phononic materials and structures: historical origins, recent progress, and future outlook. Appl. Mech. Rev. 66:040802. 218. Indeitsev, D.A., Kuznetsov, N.G., Motygin, O.V. and Mochalova,Yu.A. 2007. Localization of Linear Waves. St. Petersburg: St. Petersburg University (in Russian). 219. Jee, W.S.S. 2001. Integrated bone tissue physiology: anatomy and physiology. In: Cowin, S.C. (ed.) Bone Mechanics Handbook, Boca Raton: CRC, pp. 51-68. 220. Jerri, A.J. 2011. Advances in the Gibbs Phenomenon. New York: ∑ Sampling Publishing. 221. Jiang, M., Shen, Yi. and Liao, X. 2006. Stability, bifurcation and a new chaos in the logistic differential equation with delay. Phys. Lett. A 350:221–227. 222. Joukowsky, N.E. 1937. The work of continuous and non-continuous traction devices in pulling a train from its position and at the beginning of its motion. In: Joukowsky, N.E. Kotelnikov, A.P. (Ed.) Complete Collected Works, 8: Theory of Elasticity. Railways. Automobiles, Moscow: ONTI, pp. 221–255 (in Russian). 223. Kafesaki, M. and Economou, E.N. 1999. Multiple-scattering theory for threedimensional periodic acoustic composites. Phys. Rev. B 60:11993–12001. 224. Kalamkarov, A.L., Andrianov, I.V. and Danishevs’kyy, V.V. 2009. Asymptotic homogenization of composite materials and structures. Appl. Mech. Rev. 62:030802. 225. Kanaun, S.K. and Levin, V.M. 2003. Self-consistent methods in the problem of axial elastic shear wave propagation through fibre composites. Arch. Appl. Mech. 73:105– 130. 226. Kanaun, S.K. and Levin, V.M. 2008. Self-Consistent Methods for Composites. Vol.2: Wave Propagation in Heterogeneous Materials. New York: Springer. 227. Kanaun, S.K. and Levin, V.M. 2005. Propagation of shear elastic waves in composites with a random set of spherical inclusions (effective field approach). Int. J. Sol. Struct. 42:3971–3997. 228. Kanaun, S.K., Levin, V.M. and Sabina F.J. 2004. Propagation of elastic waves in composites with random set of spherical inclusions (effective medium approach). Wave Motion 40:69–88. 229. Kantorovich, L.V. and Krylov, V.I. 1958. Approximate Methods of Higher Analysis. Groningen: P. Noordhoff. 230. Kaplunov, J.D., Kossovich, L.Ya. and Nolde, E.V. 1998. Dynamics of Thin Walled Elastic Bodies. San Diego: Academic Press.

218

References

231. Kaplunov, J. and A. Pichugin. 2009. On rational boundary conditions for higher-order long-wave models. In: Borodich, F. (eds.) IUTAM Symposium on Scaling in Solid Mechanics. Iutam Bookseries 10, Dordrecht: Springer, pp. 81–90. 232. Karpov, S.Yu. and Stolyarov, S.N. 1993. Propagation and transformation of electromagnetic waves in one-dimensional periodic structures. Physics-Uspekhi 36(1):1–22. 233. Kasra, M. and Grynpas, M.D. 1998. Static and dynamic finite element analyses of an idealized structurel model of vertebral trabecular bone. Trans. ASME J. Biomech. Eng. 120:267–272. 234. Kawarai, S. 2002. Exact discretization of differential equations by s-z transform. In: Proceedings of the 2002 IEEE International Symposium on Circuits and Systems, Phoenix-Scottsdale, AZ, USA, 26-29 May, pp. 461–464. 235. Keller, J.B. 1964. A theorem on the conductivity of a composite medium. J. Math. Phys. 5(4):548–549. 236. Kevrekidis, P.G. 2011. Non-linear waves in lattices: past, present, future. IMA J. Appl. Math. 76(3): 389–423. 237. Kevrekidis, P.G. and Kevrekidis, I.G. 2001. Heterogeneous versus discrete mapping problem. Phys. Rev. E. 64:056624-1 – 056624-8. 238. Kevrekidis, P.G., Kevrekidis, I.G., Bishop, A.R. and Titi, E.S. 2002. Continuum approach to discreteness. Phys. Rev. E. 65(4):46613-1 – 46613-13. 239. Khusnutdinova, K.R. and Samsonov, A.M. 2008. Fission of a longitudinal strain solitary wave in a delaminated bar. Phys. Rev. E. 77:066603. 240. Kissel, G.J. 1988. Localization in Disordered Periodic Structures. Massachusetts: Massachusetts Institute of Technology. 241. Kittel, C. 2005. Introduction to Solid State Physics. (8th ed.) Hoboken, New York: Wiley. 242. Kivshar, Yu.S. and Salerno, M. 1994. Modulation instabilities in the discrete deformable nonlinear Schr¨odinger equation. Phys. Rev. E. 49(4):3543–3546. 243. Kliakhandler, I.L., Porubov, A. and Velarde, M.G. 2000. Localized finite-amplitude disturbance and selection of solitary waves. Phys. Rev. E 62:4959–4962. 244. Kochmann, D.M. and Bertoldi, K. 2017. Exploiting microstructural instabilities in solids and structures: from metamaterials to structural transitions. Appl. Mech. Rev. 69:050801. 245. Korn, G.A. and Korn, T.M. 2000. Mathematical Handbook for Scientists and Engineers: Definitions, Theorems, and Formulas for Reference and Review. Mineola, New York: Dover. 246. Korteweg, D.J. and de Vries, G. 1895. On the change of the form of long waves advancing in a rectangular channel and on a new type of long stationary waves. Phil. Mag. 5:422–443. 247. Kosevich, A.M. 2005. The Crystal Lattice: Phonons, Solitons, Dislocations, Superlattices. Berlin: Wiley. 248. Kosevich, A.M. and Kovalev, A.S. 1975. Self-localization of vibrations in a onedimensional anharmonic chain. Sov. Phys.-JETP. 40(5):891–896. 249. Kosevich, A.M. and Savotchenko, S.E. 1999. Peculiarities of dynamics of onedimensional discrete systems with interaction extending beyond nearest neighbors, and the role of higher dispersion in soliton dynamics. Low Temp. Phys. 25(7):550–557. 250. Kosevich, Yu.A. 2003. Nonlinear envelope-function equation and strongly localized vibrational modes in anharmonic lattices. Phys. Rev. B. 47:3138–3152.

References

219

251. Kovalev, A.S. and Kosevich, A.M. 1975. Self-localization of vibrations in a onedimensional anharmonic chain. Sov. Phys. JETP 40:891–896. 252. Kozlov, S.M. 1989. Geometrical aspects of averaging. Russ. Math. Surv. 44:91–144. 253. Kozlov, S.M. 1987. Averagind of difference schemes. Math. USSR-Sb. 57(2):351–369. 254. Kozyrenko, V.N., Kumpanenko, I.V. and Mikhailov, I.D. 1977. Green’s function analysis of the vibrational spectra of polymer chain. I. Several approaches to the problem. J. Polymer Sci. 15:1721–1738. 255. Krivtsov, A.M. 2007. Deformation and Destruction of Microstructured Solids. Moscow: Fizmatlit (in Russian). 256. Kruzik, J.J. 2009. Predicting fatigue failures. Science 325:156–157. 257. Kunin, I.A. 1966. Model of an elastic medium of simple structure with threedimensional dispersion. J. Appl. Math. Mech. 30(3):642–652. 258. Kunin, I.A. 1982. Elastic Media with Microstructure. 1. One-Dimensional Models. Berlin: Springer. 259. Kunin, I.A. 1983. Elastic Media with Microstructure. 2. Three-dimensional Models. Berlin: Springer. 260. Kurchanov, P.F., Myshkis, A.D. and Filimonov, A.M. 1991. Some unexpected results in the classical problem of vibrations of the string with n beads when n is large. C.R. Acad. Sci. Paris 1313:961–965. 261. Kurchanov, P.F., Myshkis, A.D. and Filimonov, A.M. 1991. Vibrations of rolling stock and a theorem of Kronecker. J. Appl. Math. Mech. 55(6):870–876. 262. Kushwaha, M.S. 1997. Stop-bands for periodic metallic rods: sculptures that can filter the noise. Appl. Phys. Lett. 70:3218–3220. 263. Kushwaha, M.S. and Halevi, P. 1994. Band-gap engineering in periodic elastic composites. Appl. Phys. Lett. 64:1085–1087. 264. Kushwaha, M.S. and Halevi, P. 1996. Giant acoustic stop bands in twodimensional periodic arrays of liquid cylinders. Appl. Phys. Lett. 69:31–33. 265. Kushwaha, M.S., Halevi, P., Dobrzynski, L. and Djafari-Rouhani, B. 1993. Acoustic band structure of periodic elastic composites. Phys. Rev. Lett. 71:2022–2025. 266. Kushwaha, M.S., Halevi, P., Martinez, G., Dobrzynski, L. and Djafari-Rouhani, B. 1994. Theory of acoustic band structure of periodic elastic composites. Phys. Rev. B. 49:2313–2322. 267. Lagrange, J.L. 1997. Analytical Mechanics. Berlin: Springer Nature. 268. Lakes, R.S. 1982. Dynamical study of couple stress effects in human compact bone. Trans. ASME J. Biomech. Eng. 104:6–11. 269. Lamacz, A. 2011. Dispersive effective models for waves in heterogeneous media. Math. Model. Meth. Appl. Sci. 21(9):1871–1899. 270. Landa, P.S. 1996. Nonlinear Oscillations and Waves in Dynamical Systems. Dordrecht: Kluwer. 271. Landa, P.S., 2001. Regular and Chaotic Oscillations. Berlin, New York: SpringerVerlag. 272. Landa, P.S. and Marchenko, V.F. 1991. On the linear theory of waves in media with periodic structures. Sov. Phys. Usp. 34(9):830–834. 273. Lazar, M., Maugin, G.A. and Aifantis, E.C. 2006. On a theory of nonlocal elasticity of bi-Helmholtz type and some applications. Int. J. Sol. Struct. 43:1404–1421. ´ ´ 274. Le Roux, M.J. 1911. Etude g´eom´etrique torsion. Annales scientifiques de L’Ecole Normale Sup´erieur 28, 523–579.

220

References

275. Lebedev, L.P. and Vorovich, I.I. 2002. Functional Analysis in Mechanics. New York: Springer. 276. Lenci, S. and Menditto, G. 2000. Weak interface in long fibre composites. Int. J. Sol. Struct. 37:4239–4260. 277. Levy, A.J. and Dong, Z. 1998. Effective transverse response of fibre composites with nonlinear interface. J. Mech. Phys. Sol. 46:1279–1300. 278. Levy, A.J. 1996. The effective dilatational response of fibre reinforced composites with nonlinear interface. J. Appl. Mech. 63:357–364. 279. Levy, A.J. 2000. The fibre composite with nonlinear interface. Part I: Axial tension. J. Appl. Mech. 67:727–732. 280. Li, D. and H. Benaroya. 1992. Dynamics of periodic and near-periodic structures. Appl. Mech. Rev. 45(11):447–459. 281. Li, D. and Benaroya, H. 1996. Vibration localization in multi-coupled and multidimensional near-periodic structures. Wave Motion 23:67–82. 282. Liang, B., Yuan, B. and Chen, J.-C. 2009. Acoustic diode: rectification of acoustic energy flux in one-dimensional systems. Phys. Rev. Let. 103:104301. 283. Lin, Y.K. 1996. Dynamics of disordered periodic structures. Appl. Mech. Rev. 49:57– 64. 284. Liu, Z., Chan, C.T., Sheng, P., Goertzen, A.L. and Page, J.H. 2000. Elastic wave scattering by periodic structures of spherical objects: theory and experiment. Phys. Rev. B 62:2446–2457. 285. Love, A.E.H. 1927. A Treatise on the Mathematical Theory of Elasticity, 4th edn. Cambridge: Cambridge University Press. 286. Lubin, G. 2014. Handbook of Composites. Berlin: Springer. 287. Lubineau, G., Azdoud, Y., Han, F., Rey, C. and Askari, A. 2012. A morphing strategy to couple non-local to local continuum mechanics. J. Mech. Phys. Sol. 60:1088–1102. 288. Lucia, U. 2016. Macroscopic irreversibility and microscopic paradox: A Constructal law analysis of atoms as open systems. Sci. Rep. 6:35796. 289. Lur’e, A.I. 1951. Operational Calculus and its Applications to the Problems of Mechanics. Moscow: GITTL (in Russian). 290. Lur’e, A.I. 1990. Nonlinear Theory of Elasticity. Amsterdam: North-Holland. 291. Malyi, V.I. 1971. About nonlocal theory of elasticity. In: IV All-Union Conference on Strength and Plasticity. Moscow: Nauka, pp. 74–78 (in Russian). 292. Malyi, V. 2021. Theoretical determination of the five physical constants of the ToupinMindlin gradient elasticity for polycrystalline materials. In: Nonlinear Dynamics of Discrete and Continuous Systems, Cham: Springer Nature. 145–154. Abramian, A.K.,Andrianov, I.V., Gaiko, V.A. (eds). Advanced Structured Matherials 139. 293. Manevich, A.I. and Manevitch, L.I. 2005. The Mechanics of Nonlinear Systems with Internal Resonances. Singapore: World Scientific. 294. Manevitch, L.I. and Gendelman, O.V. 2011. Tractable Models of Solid Mechanics. Formulation, Analysis and Interpretation. Berlin, Heidelberg, London, New York: Springer. 295. Manevitch, L.I. and Pilipchuk, V.N. 1985. Localized vibrations in linear and nonlinear lattices. Adv. Mech. 13:107–134 (in Russian). 296. Manevitch, L.I. and Smirnov, V.V. 2008. Solitons in Macromolecular Systems. New York: Nova Science Publishers. 297. Manevitch, L.I., Kovaleva, A.S., Smirnov, V.V. and Starosvetsky, Yu. 2017. Nonstationary Resonant Dynamics of Oscillatory Chains and Nanostructures. Singapore: Springer.

References

221

298. Manevitch, L.I., Mikhlin, Yu.V. and Pilipchuk, V.N. 1989. Method of Normal Vibrations for Essentially Nonlinear Systems. Moscow: Nauka (in Russian). 299. Maradudin, A.A. 1965. Some effects of point defects on the vibrations of crystal lattices. Rep. Prog. Phys. 28:331–380. 300. Maradudin, A.A. 2003. Lattice dynamics. Ann. Rev. Phys. Chem. 14(1):89–116. 301. Maradudin, A.A., Montroll, E.W. and Weiss, G.H. 1971. Theory of Lattice Dynamics in the Harmonic Approximation. New York: Academic Press. 302. Martowicz, A., Roemer, J., Staszewski, W.J., Ruzzene, M. and Uhl, T. 2019. Solving partial differential equations in computational mechanics via nonlocal numerical approaches. ZAMM 99(4):e201800342. 303. Maslov, V.P. 1976. Operational Methods. Moscow: Mir. 304. Maslov, V.P. and Mosolov, P.P. 2000. Nonlinear Wave Equations Perturbed by Viscous Terms. Berlin, New York: de Gruyter. 305. Maslov, V.P. and Omelyanov, G.A. 2001. Geometric Asymptotic for Nonlinear PDE. I. Providence: AMS. 306. Maugin, G.A. 1999. Nonlinear Waves in Elastic Crystals. Oxford: Oxford University Press. 307. Maugin, G.A. 1999. From Piola’s manifold to Cosserats’ structure. In: Geometry, Continua and Microstructure, Maugin, G.A. (Ed.) Paris: Hermann, pp. 113–120. 308. Maugin, G.A. 2013. Continuum Mechanics Through the Twentieth Century. A Concise Historical Perspective. Dordrecht: Springer. 309. May, R. 1976. Simple mathematical models with very complicated dynamics. Nature 261:459–467. 310. McPhedran, R.C. and McKenzie, D.R. 1978. The conductivity of lattices of spheres. I. The simple cubic lattice. Proc. Roy. Soc. London A359:45–63. 311. McPhedran, R.C., Poladian, L. and Milton, G.W. 1988. Asymptotic studies of closely spaced, highly conducting cylinders. Proc. Roy. Soc. London A415:185–196. 312. Mencik, J.M. and Ichchou, M.N. 2005. Multi-mode propagation and diffusion in structures through finite elements. Eur. J. Mech. A/Solids 24(5):877–898. 313. Meng, S. and Guzina, B.B. 2018. On the dynamic homogenization of periodic media: Willis’ approach versus two-scale paradigm. Proc. R. Soc. A 474:20170638. 314. Metrikine, A.V. 2006. On causality of the gradient elasticity models. J. Sound Vib. 297:727–742. 315. Metrikine, A.V. and Askes, H. 2002. One-dimensional dynamically consistent gradient elasticity models derived from a discrete microstructure. Part 1: Generic formulation. Eur. J. Mech. A /Sol. 21:555–572. 316. Metrikine, A.V. and Askes, H. 2008. An isotropic dynamically consistent gradient elasticity model derived from a 2D lattice. Phil. Mag. 86(21):3259–3268. 317. Maldovan, M. 2013. Sound and heat revolution in phononics. Nature 503:209–217. 318. Mindlin, R.D. 1964. Micro-structure in linear elasticity. Arch. Rat. Mech. Anal. 16:51– 78. 319. Mindlin, R.D. and Herrmann, G. 1952. A one-dimensional theory of compressional waves in an elastic rod. Proc. First U.S. Nat. Congr. Appl. Mech., ASME 187–191. 320. Montero de Espinosa, F.R., Jim´enez E. and Torres, M. 1998. Ultrasonic band gap in a periodic two-dimensional composite. Phys. Rev. Lett. 80:1208–1211. 321. Moon, F.C. 1987. Chaotic Vibrations. An Introduction for Applied Scientists and Engineers. Ithaca: Cornell University. 322. Mortell, M.P. and Seymour, R.B. 1972. Pulse propagation in a nonlinear viscoelastic rod of finite length. SIAM J. Appl. Math. 22:209–224.

222

References

323. Mortell, M.P. and Varley, E. 1970. Finite amplitude waves in bounded media: nonlinear free vibrations of an elastic panel. Proc. Roy. Soc. A 318:169–196. 324. Movchan, A.B. and Slepyan, L.I. 2007. Band gap Green’s functions and localized oscillations. Proc. R. Soc. A. 463:2709–2727. 325. Movchan, A.B., Movchan, N.V., Jones, I.S. and Colquitt, D.J. 2018. Mathematical Modelling of Waves in Multi-Scale Structured Media. London: Taylor and Francis. 326. Movchan, A.B., Movchan, N.V. and Poulton, C.G. 2002. Asymptotic Models of Fields in Dilute and Densely Packed Composites. London: Imperial College Press. 327. Munkhammar, J. 2013. Chaos in fractional order logistic equation. Fract. Calc. Appl. Anal. 16:511–519. 328. Murnaghan, F.D. 1951. Finite Deformation of an Elastic Solid. New York: Wiley. 329. Myshkis, A.D. 2005. Mixed functional differential equations. J. Math. Sc. 129(5):4111–4226. 330. Nayfeh, A.H. 2000. Perturbation Methods. New York: Wiley. 331. Nayfeh, A.H. and Mook, D.T. 1979. Nonlinear Oscillations. New York: Wiley. 332. Needleman, A. 1990. An analysis of tensile decohesion along an interface. J. Mech. Phys. Sol. 38:289–324. 333. Needleman, A. 1992. Micromechanical modelling of interfacial decohesion. Ultramicroscopy 40:203–214. 334. Nemat-Nasser, S. and Srivastava, A. 2011. Overall dynamic constitutive relations of layered elastic composites. J. Mech. Phys. 59:1953–2258. 335. Nesterenko, V.F. 2018. Waves in strongly nonlinear discrete systems. Phil. Trans. R. Soc. A 376:20170130. 336. Nie, S. and C. Basaran. 2005. A micromechanical model for effective elastic properties of particulate composites with imperfect interfacial bonds. Int. J. Sol. Struct. 42:4179– 4191. 337. Ogden, R.W. 1997. Nonlinear Elastic Deformations. New York: Dover. 338. Oleynik, O.A., Shamaev, A.S. and Yosifian, G.A. 1992. Mathematical Problems in Elasticity and Homogenization. Amsterdam: North-Holland. 339. Osharovich, G.G. and Ayzenberg-Stepanenk, M.V. 2012. Wave localization in stratified square-cell lattices: The antiplane problem. J. Sound Vib. 331:1378–1397. 340. Pagano, S. and Paroni, R. 2003. A simple model for phase transition: from the discrete to the continuum problem. Q. Appl. Math. 61:89–109. 341. Pal, R.K., Rimoli, J.J. and Ruzzene, M. 2016. Effect of large deformation pre-loads on the wave properties of hexagonal lattices. Smart Mater. Struct. 25:054010. 342. Pal, R.K., Ruzzene, M. and Rimoli, J.J. 2016. A continuum model for nonlinear lattices under large deformations. Int. J. Sol. Struct. 96:300–319. 343. Palmov. V.A. 1967. Propagation of vibrations in a nonlinear dissipative medium. J. Appl. Math. Mech. 31:763–769. 344. Palmov, V.A. 2014. Vibrations of Elasto-Plastic Bodies. Berlin: Springer. 345. Panasenko, G.P. 2005. Multi-Scale Modeling for Structures and Composites. Berlin: Springer. 346. Parks, M.L., Bochev, P.B. and Lehoucq, R.B. 2008. Connecting atomistic-tocontinuum coupling and domain decomposition. Multisc. Mod. Simul. 7:362–380. 347. Parnell, W.J. 2007. Effective wave propagation in a prestressed nonlinear elastic composite bar. IMA J. Appl. Math. 72:223–244. 348. Parnell, W.J. 2012. Nonlinear pre-stress for cloaking from antiplane elastic waves. Proc. R. Soc. A. 468:563–580.

References

223

349. Parnell, W.J. and Abrahams, I.D. 2006. Dynamic homogenization in periodic fibre reinforced media. Quasi-static limit for SH waves. Wave Motion 43:474–498. 350. Parnell, W.J. and Abrahams, I.D. 2008. Homogenization for wave propagation in periodic fibre-reinforced media with complex microstructure. I-Theory. J. Mech. Phys. Sol. 56:2521–2540. 351. Parnell, W.J. and Abrahams, I.D. 2011. The effective wavenumber of a pre-stressed nonlinear microvoided composite. J. Phys.: Conf. Ser. 269:012007. 352. Parnell, W.J. and Grimal, Q. 2009. The influence of mesoscale porosity on cortical bone anisotropy. Investigations via asymptotic homogenization. J. Roy. Soc. Interf. 6:97– 109. 353. Paroni, R. 2003. From discrete to continuum: a Young measure approach. ZAMP 54(2):328–348. 354. Pasternak, E. and M¨uhlhaus H.-B. 2005. Generalized homogenization procedure for granular material. J. Eng. Math. 52:199–229. 355. Pavlov, I.S. and Potapov, A.I. 2008. Structural models in mechanics of nanocrystalline media. Dokl. Phys. 53(7):408–412. 356. Peerlings, R.H.J., Geers, M.G.D., de Borst, R. and Brekelmans, W.A.M. 2001. A critical comparison of nonlocal and gradient-enhanced softening continua. Int. J. Sol. Struct. 38:7723–7746. 357. Peregrin, D.H. 1966. Calculation of the development of an undular bore. Fluid Mech. 25:321–330. 358. Perrins, W.T, McKenzie, D.R. and McPhedran R.C. 1979. Transport properties of regular arrays of cylinders. Proc. Roy. Soc. A369:207–225. 359. Petropoulou, E.N. 2010. A discrete equivalent of the logistic equation. Adv. Differ. Eq. 2010:457073. 360. Pfaller, G., Possart, P., Steinmann, M., Rahimi, F., M¨uller-Plathe and B¨ohm, M.C. 2012. Acomparison of staggered solution schemes for coupled particle-continuum systems modeled with the Arlequin method. Comp. Mech. 49:565–579. 361. Pichugin, A.V., Askes, H. and Tyas, A. 2008. Asymptotic equivalence of homogenization procedures and fine-tuning of continuum theories. J. Sound Vib. 313:858–874. 362. Picu, R.C. 2002. On the functional form of non-local elasticity kernels. J. Mech. Phys. Sol. 50:1923–1939. 363. Pierre, C. and Dowell, E.H. 1987. Localization of vibrations by structural irregularity. J. Sound Vib. 114:549–564. 364. Pierre, Ch., Castanier, M. and Joe, C.W. 1996. Wave localization in multi-coupled periodic structures. Application to truss beams. Appl. Mech. Rev. 49:65–86. 365. Pilipchuk, V.N. and Starushenko, G.A. 1997. A version of non-smooth transformations of variables for one-dimensional elastic systems of periodic structures. J. Appl. Math. Mech. 61(2):265–274. 366. Pilipchuk, V.N., Andrianov, I.V. and Markert, B. 2016. Analysis of micro-structural effects on phononic waves in layered elastic media with periodic nonsmooth coordinates. Wave Motion 63:149–169. 367. Platts, S.B., Movchan, N.V., McPhedran, R.C. and Movchan, A.B. 2002. Twodimensional phononic crystals and scattering of elastic waves by an array of voids. Proc. R. Soc. Lond. A. 458:2327–2347. 368. Platts, S.B., Movchan, N.V., McPhedran, R.C., Movchan, A.B. 2003. Band gaps and elastic waves in disordered stacks: normal incidence. Proc. R. Soc. Lond. A. 459:221– 240.

224

References

369. Porubov, A.V. 2003. Amplification of Nonlinear Strain Waves in Solids. Singapore: World Scientific. 370. Porubov, A.V. 2009. Localization of Nonlinear Strain Waves. Moscow: FIZMATLIT (in Russian). 371. Porubov, A.V. and Andrianov, I.V. 2013. Nonlinear waves in diatomic crystals. Wave Motion 50:1153–1160. 372. Porubov, A.V. and Velarde, M.G. 2002. Strain kinks in an elastic rod embedded in a viscoelastic medium. Wave Motion 35:189–204. 373. Porubov, A.V., Osokina, A.E. and Antonov, I.D. 2020. Nonlinear dynamics of twodimensional lattices with complex structure. Nonlinear Wave Dynamics of Materials and Structures. Springer Nature: Cham, 309–334. 374. Potapov, A.I., Pavlov, I.S. and Lisina, S.A. 2009. Acoustic identification of nanocrystalline media. J. Sound Vib. 322:564–580. 375. Potapov, A.I., Pavlov, I.S. and Maugin, G.A. 2006. A 2D granular medium with rotating particles. Int. J. Solids Str. 43(20):6194–6207. 376. Poulton, C.G., Movchan, A.B., McPhedran, R.C., Nicorovici, N.A. and Antipov, Y.A. 2000. Eigenvalue problems for doubly periodic structures and phononic band gaps. Proc. R. Soc. Lond. A. 456:2543–2559. 377. Prudnikov, A.P., Brichkov, Yu.A. and Marichev, O.I. 1986. Integrals and Series. Vol. 1. Elementary Functions. New York: Gordon & Breach. 378. Psarobas, I.E., Stefanou, N. and Modinos, A. 2000. Scattering of elastic waves by periodic arrays of spherical bodies. Phys. Rev. B 62:278–291. 379. Rayleigh, J.W.S. 1877–1888. The Theory of Sound, 1-2. London: Macmillan and Co. 380. Rayleigh, Lord Sec. R.S. 1892. On the influence of obstacles arranged in rectangular order upon the properties of a medium. The London, Edinburgh, and Dublin Phil. Mag. J. Sci. 34(211):481–502. 381. Rednikov, A.Ye., Velarde, M.G., Ryazantsev, Yu.S., Nepomnyashchy, A.A. and Kurdyumov, V.N. 1995. Cnoidal wave trains and solitary waves in a dissipation modified Korteweg - de Vries equation. Acta Appl. Math. 39:457–475. 382. Remoissenet, M. 1986. Low-amplitude breather and envelope solitons in quasi-onedimensional physical models. Phys. Rev B 33:2386–2392. 383. Ribeiro, P. and Petyt, M. 1999. Non-linear vibration of beams with internal resonances by the hierarchical finite-element method. J. Sound Vib. 224:591–624. 384. Rogers, R.C. and Truskinovsky, L. 1997. Discretization and hysteresis. Physica B 233:370–375. 385. Rosenau, Ph. 1986. Dynamics of nonlinear mass-spring chains near the continuum limit. Phys. Lett. A 118(5): 222–227. 386. Rosenau, Ph. 1987. Dynamics of dense lattices. Phys. Rev. B 36(11):5868–5876. 387. Rosenau, Ph. 1988. Dynamics of dense discrete systems. Prog. Theor. Phys. 89(5):1028–1042. 388. Rosenau, Ph. 1989. Extending hydrodynamics via the regularization of the ChapmanEnskog expansion. Phys. Rev. A 40(12):7193–7196. 389. Rosenau, Ph. 2003. Hamiltonian dynamics of dense chains and lattices: or how to correct the continuum. Phys. Lett. A 311(5):39–52. 390. Rudenko, O.V. 2006. Giant nonlinearities in structurally inhomogeneous media and the fundamentals of nonlinear acoustic diagnostic techniques. Phys. Uspek. 49:69–87. 391. Rushchitsky, J.J. 1999. Interaction of waves in solid mixtures. Appl. Mech. Rev. 52:35– 74.

References

225

392. Rushchitsky, J. 2014. Nonlinear Elastic Waves in Materials. Berlin: Springer. 393. Sachdev, P.L. 1987. Nonlinear Diffusive Waves. Cambridge: Cambridge University Press. 394. Sakuma, Y., Pa¨ıdoussis, M.P. and Price, S.J. 2010. Mode localization phenomena and stability of disordered trains and train-like articulated systems travelling in confined fluid. J. Sound Vib. 329:5501–5519. 395. Salupere, A., Engelbrecht, J. and Maugin, G.A. 2001. Solitonic structures in KdVbased higher-order systems. Wave Motion 34:51–61. 396. Salupere, A., Maugin, G.A. and Engelbrecht, J. 1994. Korteweg-de Vries soliton detection from a harmonic input. Phys. Lett. A 192:5–8. 397. Samarskii, A.A. and Mikhailov, A.P. 2002. Principles of Mathematical Modeling. Ideas, Methods, Examples. London: Taylor and Francis. 398. Samsonov, A.M. 2001. Strain Solitons in Solids and How to Construct Them. Boca Raton: CRC Press. 399. Santosa, F. and Symes, W. 1991. A dispersive effective medium for wave propagation in periodic composites. SIAM J. Appl. Math. 51:984–1005. 400. Schr¨odinger, E. 1914. Zur Dynamik elastisch gekoppelter Punktsysteme. Annalen der Physik 349(14):916–934. 401. Scott, A. 2003. Nonlinear Science: Emergence and Dynamics of Coherent Structures. New York: Oxford University Press. 402. Seeger, A. 2010. On the simulation of dispersive wave propagation by elasticity models. Philos. Mag. 90(9):1101–1104. 403. Sen, A. and Mukherjee, D. 2009. Chaos in the delay logistic equation with discontinuous delays. Chaos Soliton Fract. 40:2126–2132. 404. Seymour, R.B. and Varley, E. 1970. High frequency, periodic disturbances in dissipative systems. I. Small amplitude, finite rate theory. Proc. Roy. Soc. A 314:387–415. 405. Shamrovskyi, A.D. 2004. Discrete Approaches in Economics. Zaporozhye: Zaporozhye State Engineering Academy (in Russian). 406. Shodja, H.M., Zaheri, A. and Tehranchi, A. 2013. Ab initio calculations of characteristic lengths of crystalline materials in first strain gradient elasticity. Mech. Mater. 61:73–78. 407. Shokin, Y.I. 1983. The Method of Differential Approximation. Berlin: Springer. 408. Shulga, N.A. 2003. Propagation of elastic waves in periodically inhomogeneous media. Int. Appl. Mech. 39:763–796. 409. Shulga, N.A. 2003. Propagation of coupled waves interacting with an electromagnetic field in periodically inhomogeneous media. Int. Appl. Mech. 39:1146–1172. 410. Sievers, A.J. and Page, J.B. 1995. Unusual local mode systems. In: Dynamical Properties of Solids, Vol 7. Phonon Physics the Cutting Edge, Horton, G.K., Maradudin, A.A. (eds.), pp. 137–256. 411. Sigalas, M.M. and Economou, E.N. 1992. Elastic and acoustic wave band structure. J. Sound Vib. 158:377–382. 412. Sigalas, M.M. and Economou, E.N. 1993. Band structure of elastic waves in two dimensional systems. Sol. Stat. Comm. 86:141–143. 413. Sigalas, M.M. and Economou, E.N. 1994. Elastic waves in plates with periodically place inclusions. J. Appl. Phys. 75:2845–2850. 414. Sigalas, M.M. and Economou, E.N. 1996. Attenuation of multiple-scattered sound. Europhys. Lett. 36:241–246.

226

References

415. Slepyan, L.I. 1972. Non-steady-state Elastic Waves. Leningrad: Sudostroyenie (in Russian). 416. Slepyan, L.I. 1981. Crack propagation in high-frequency lattice vibration. Sov. Phys. Dokl. 26:900–902. 417. Slepyan, L.I. 1981. Dynamics of a crack in a lattice. Sov. Phys. Dokl. 26:538–540. 418. Slepyan, L.I. 1982. The relation between the solutions of mixed dynamic problems for a continuous elastic medium and a lattice. Sov. Phys. Dokl. 27:771–772. 419. Slepyan, L.I. 1984. Dynamics of brittle fracture in media with a structure. Mech. Sol. 19(6):114–115. 420. Slepyan, L.I. and Troyankina, L.V. 1984. Fracture wave in a chain structure. J. Appl. Mech. Techn. Phys. 25(6):921–927. 421. Slepyan, L.I. and Troyankina, L.V. 1988. Impact waves in a nonlinear chain. In: Plasticity and Fracture of Solids, Gol’dstein, R.V. (ed.) Moscow: Nauka, pp. 175–186 (in Russian). 422. Smith, B., Bjorstad, P. and Gropp, W. 1996. Domain Decomposition. Cambridge: Cambridge University Press. 423. Smyshlyaev, V.P. 2009. Propagation and localization of elastic waves in highly anisotropic periodic composites via two-scale homogenization. Mech. Mat. 41:434– 447. 424. Strogatz, S.H. 2018. Nonlinear Dynamics and Chaos with Applications to Physics, Biology, Chemistry, and Engineering. Boca Raton: CRC Press. 425. Sun, C.T., Achenbach, J.D., Herrmann, G. 1968. Continuum theory for a laminated media. J. Appl. Mech. 35:467–475. 426. Tadmor, E.B., Ortiz, M. and Phillips, R. 1996. Quasicontinuum analysis of defects in crystals. Phil. Mag. A 73:1529–1563. 427. Tamura, S., Shields, J.A. and Wolfe, J.P. 1991. Lattice dynamics and elastic phonon scattering in silicon. Phys. Rev. B 44:3001–3011. 428. Tan, H., Liu, C., Huang, Y. and Geubelle, P.H. 2005. The cohesive law for the particle/matrix interfaces in high explosives. J. Mech. Phys. Sol. 53:1892–1917. 429. Tarasov, V.E. 2017. Discrete wave equation with infinite differences. Appl. Math. Inf. Sci. Lett. 5(2):41–44. 430. Tarasova, V.V. and Tarasov, V.E. 2017. Logistic map with memory from economic model. Chaos Solit. Fract. 95:84–91. 431. Ting, T.C.T. 1980. Dynamic response of composites. Appl. Mech. Rev. 33:1629–1635. 432. Tokarzewski, S., Telega, J.J. and Galka, A. 2000. Prediction of torsional rigidities of bone filled with marrow: The application of multipoint Pad´e approximants. Acta Bioeng. Biomech. 2:560–566. 433. Torres, M., Montero de Espinosa, F.R., Garcia-Pablos, D., Garcia, N. 1999. Sonic band gaps in finite elastic media: surface states and localization phenomena in linear and point defects. Phys. Rev. Lett. 82:3054–3057. 434. Toupin, R.A. 1964. Theories of elasticity with couple-stresses. Arch. Ration. Mech. Anal. 17(2):85–112. 435. Truskinovsky, L. and Vainchtein, A. 2005. Quasicontinuum modelling of short-wave instabilities in crystal lattices. Phil. Mag. 85(33-35):4055–4065. 436. Tvergaard, V. 1995. Fibre debonding and breakage in a whisker reinforced metal. Mater. Sci. Eng. A 90:215–222. 437. Tvergaard, V. and Hutchinson, J.W. 1993. The influence of plasticity on mixed-mode interface toughness. J. Mech. Phys. Sol. 41:1119–1135.

References

227

438. Tzirakis, N. and Kevrekidis, P.G. 2005. On the collapse arresting effects of discreteness. Math. Comput. Simul. 69:553–566. 439. Ulam, S.M. 1960. A Collection of Mathematical Problems. New York: Interscience Publishers. 440. Vakakis, A.F., King, M.E. and Pearlstein, A.J. 1994. Forced localization in a periodic chain of nonlinear oscillators. Int. J. Non-Lin. Mech. 29:429–447. 441. Vakakis, A.F., Manevitch, L.I., Mikhlin, Yu.V., Pilipchuk, V.N. and Zevin, A.A. 1996. Normal Modes and Localization in Nonlinear Systems. New York: Wiley. 442. Vakakis, A.F., Nayfeh, A.H. and King, M.E. 1993. A multiple scales analysis of nonlinear localized modes in a cyclic periodic system. J. Appl. Mech. 60:388–397. 443. Van Dyke, M. 1975. Perturbation Methods. Stanford: The Parabolic Press. 444. Van Rietbergen, B. and Huiskes, R. 2001. Elastic constants of cancellous bone. In: Cowin, S.C. (ed.) Bone Mechanics Handbook. Boca Raton: CRC Press, 15-1 – 15-24. 445. Varley, E. and Rogers, T.G. 1967. The propagation of high frequency, finite acceleration pulses and shocks in viscoelastic materials. Proc. Roy. Soc. A 296:498–518. 446. Vasiliev, V.V. and Lurie, S.A. 2016. Correct nonlocal generalized theories of elasticity. Phys. Mesomech. 19(3):269–281. 447. Vasiliev, A.A., Dmitriev, S.V. and Miroshnichenko, A.E. 2010. Multi-field approach in mechanics of structural solids. Int. J. Sol. Struct. 47:510–525. 448. Vedenova, E.G., Manevich, L.I. and Pilipchuk, V.N. 1985. Normal oscillations of a string with concentrated masses on non-linearly elastic supports. Appl. Math. Mech. 49:153–159. 449. Verhulst, P.F. 1845. Recherches math´ematiques sur la loi d’accroissement de la population. Nouv. M´em. del’ Acad´emie Royale des Sci. et Belles-Lett. de Brux., 18:1–42. 450. Verhulst, P.F. 1847. Deuxi´eme m´emoire sur la loi d’accroissement de la population. M´em. de l’Acad´emie Royale des Sci. des Lett. et des Beaux-Arts de Belg. 20:1–32. 451. Vishik, M.I. and Lyusternik, L.A. 1960. The asymptotic behaviour of solutions of linear differential equations with large or quickly changing coefficients and boundary conditions. Russ. Math. Surv. 15(4):23–91. 452. Wagner, G.J. and Liu, WK. 2003. Coupling of atomistic and continuum simulations using a bridging scale decomposition. J. Comput. Phys. 190:249–274. 453. Wattis, J.A.D. 1993. Approximations to solitary waves on lattices, II: quasi-continuum approximations for fast and slow waves. J. Phys. A: Math. Gen. 26:1193–1209. 454. Wattis, J.A.D. 2000. Quasi-continuum approximations to lattice equations arising from discrete nonlinear telegraph equation. J. Phys. A: Math. Gen. 33:5925–5944. 455. Weinan, E. and Engquist, B. 2003. The heterogeneous multiscale methods. Comm. Math. Sci. 1(1):87–132. 456. Weissert, T.P. 1997. The Genesis of Simulations in Dynamics: Pursuing the FermiPasta-Ulam Problem. Berlin: Springer. 457. Wilcox, D.C. 1995. Perturbation Methods in the Computer Age. La Canada, Ca.: DCW Industries Inc. 458. Williams, J.L. and Lewis, J.L. 1982. Properties and an anisotropic model of cancellous bone from the proximal tibial epiphysis. Trans. ASME J. Biomech. Eng. 104(1):50–56. 459. Willis, J.R. 2009. Exact effective relations for dynamics of a laminated body. Mech. Mater. 41:385–393. 460. Willis, J.R. 2011. Effective constitutive relations for waves in composites and metamaterials. Proc. R. Soc. A 467(2131):1865–1879.

228

References

461. Willis, J.R. 2012. A comparison of two formulations for effective relations for waves in a composite. Mech. Mater. 47:51–60. 462. Wolfe, J.P. 1998. Imaging Phonons: Acoustic Wave Propagation in Solids. Cambridge: Cambridge University Press. 463. Xiao, S.P. and Belytschko, T. 2004. A bridging domain method for coupling continua with molecular dynamics. Comp. Met. Appl. Mech. Eng. 193:1645–1669. 464. Yan, Z.-Z. and Zhang, Ch. 2012. Band structures and localization properties of aperiodic layered phononic crystals. Phys. B: Phys. Condens. Matter. 407:1014–1019. 465. Yan, Z.-Z., Zhang, Ch. and Wang, Y.-S. 2009. Analysis of wave propagation and localization in periodic/disordered layered composite structures by a mass-spring model. Appl. Phys. Lett. 94:161909. 466. Yan, Z.-Z., Zhang, Ch. and Wang, Y.-S. 2010. Wave propagation and localization in randomly disordered layered composites with local resonances. Wave Motion 47:409– 420. 467. Zabusky, N.J. and Deem, G.S. 1967. Dynamics of nonlinear lattices. I. Localized optical excitations, acoustic radiation, and strong nonlinear behavior. J. Comput. Phys. 2:126–153. 468. Zabusky, N.J. and Kruskal, M.D. 1965. Interaction of “solitons” in a collisionless plasma and the recurrence of initial states. Phys. Rev. Lett. 15:240–243. 469. Zaitsev, V.Yu., Nazarov, V.E. and Talanov, V.I. 2006. @Nonclassical” manifestations of microstructure-induced nonlinearities: new prospects for acoustic diagnostics. Phys. Usp. 49:89–94. 470. Zakharov, V.E. 1974. On stochastization of one-dimensional chains of nonlinear oscillators. Sov. Phys. JETP 38(1):108–110. 471. Zakharov. Yu. 2019. On physical principles and mathematical mechanisms of the phenomenon of irreversibility. Phys. A: Statist. Mech. Appl. 525:1289–1295. 472. Zalipaev, V.V., Movchan, A.B., Poulton, C.G., McPhedran, R.C. 2002. Elastic waves and homogenization in oblique periodic structures. Proc. R. Soc. Lond. A. 458:1887– 1912. 473. Zevin, A.A. 1991. Symmetrization of functionals and its applications in mechanics problems. Mech. Sol. 26(5):109–118. 474. Zevin, A.A. 1996. Localization of periodic oscillations in discrete non-linear systems. J. Sound Vib. 193(4):847–862. 475. Zevin, A.A. 1998. Estimates of eigenvalue of self-adjont boundary-value problems with periodic coefficients. Ukr. Math. J. 50(5):719–722. 476. Zheludev, N.I. and Kivshar, Yu.S. 2012. From metamaterials to metadevices. Nat. Mater. 11:917–924. 477. Zhikov, V.V. 1991. Estimates for the averaged matrix and the averaged tensor. Russ. Math. Surv. 46(3):65–136. 478. Zivieri, R., Garesci, F., Azzerboni, B., Chiappini, M. and Finocchio, G. 2019. Nonlinear dispersion relation in anharmonic periodic massspring and mass-in-mass systems. J. Sound Vib. 462:114929

Index acoustic branch, 34, 35, 37, 49, 50, 71, defect, xiii, 123, 130, 133–135, 137, 139, 72, 93, 186 140, 189 asymptotic approaches, xii, 20, 136, 142, deterministic system, xiv, 196, 201 149 discrete attenuation approximation, 125, 175, 184 coefficient, 23, 33–35, 37, 116, 117, Cauchy problem, 195 121, 127, 128, 148, 152, 177 equation, 194, 195, 201 effect, xii, 33 kink, 153, 181 factor, 123, 129, 134, 135, 137, 139, lattice, 112, 125, 163 140 media, xiv, 172, 173, 189 model, xiii, 115, 154, 157, 161, 165, Bloch-Floquet 180–182, 189, 195 approach, 1, 29 problem, 153, 157, 158, 167 method, xii, 2, 23, 29, 39, 46 wave filter, 60 waves, 130 discretization, xiv, 145, 153, 190, 193– 195, 201 Cauchy-Green dispersion, xi, xii, 1–6, 8, 18, 23, 24, 28, deformation tensor, 63 29, 31–34, 36, 45, 49–51, 53, strain tensor, 4, 63, 143, 151 59–62, 70, 78, 79, 90, 93, 99, chaotic 109, 115, 116, 127, 128, 132– behavior, 195, 196, 199, 201 134, 136, 137, 139, 142, 144– continualization, xiv 146, 153, 154, 165, 166, 177, dynamical systems, xiv, 201 178, 186 oscillations, 198, 201 dissipation, xii, 1–3, 21, 70, 78, 141, 142, regime, 3, 195 144, 148, 150, 152, 154, 186 solution, 195 double-dispersive equation, 146 continualization, xiv, 111, 114, 123, 127, 153, 155, 160–163, 167, 169, elastic 170, 183, 186, 190, 191, 195, coefficient, 70, 77, 97, 143–145 196 composite material, xiii, 130 algorithm, 193 couplings, 155, 171 procedure, xiv, 184, 187, 193 deformation, 2, 63, 65, 79, 83, 99, transform, 201 107, 169 continuous energy density, 155, 170 approximation, xiii, 103, 112, 114, force, 155 121, 123–126, 153, 157, 159, foundation, 112 165, 167, 172, 173, 175, 176, interaction, 190 181 material, 58, 141 model, xiii, xiv, 79, 111, 121, 122, matrix, 52 154, 161, 164, 181, 184, 189, medium, 142, 153, 155, 170 196 moduli, 3, 9, 12, 28, 64, 65, 90, 170 potential, 4, 64, 143, 151 229

230

properties, 64, 83 solids, 189 spring, 142, 183, 186 waves localization, 130 waves propagation, xii, 23, 39, 79, 81 waves strain, xi energy transfer, xiv, 2, 141, 142, 147–149, 151, 152, 164, 186 equations algebraic, 2, 30, 47, 61, 139 differential, 2, 6, 160, 161, 188, 193 double-dispersive, 146, 153, 176, 178 equilibrium, 8, 11 higher order, 18, 187 integro-differential, 153, 171, 173, 174 Lagrange, 160 logistic, 195 ordinary difference, xiv ordinary differential (ODE), xiv, 20, 21, 146, 152, 160, 161, 181, 193–197, 201 partial differential (PDE), xiv, 14, 20, 21, 65, 67, 167, 178, 179, 181, 186 periodicity, 11 triple-dispersive, 176, 178 Fermi-Pasta-Ulam lattice, 153, 184 fibre composite, xii, xiii, 39, 46, 81, 85, 137, 138 Fourier analysis, 20, 21 expansion, 2, 9, 146, 152 method, 167 series, xiii, 7, 20, 39, 46–48, 50, 60, 102, 104–106, 138 space, 20 transform, 20, 164, 179 Fourier-Pad´e approximation, xiii, 101, 103–106

INDEX

Gibbs-Wilbraham effects, 101, 103 phenomenon, xiv, 104 gradient model, 146, 153, 178 modules, 155, 169, 170 term, 5, 144 theory, 170 Green function, 112, 153, 176 theory, 55 hard nonlinearity, xiii, 66, 70, 74–77, 81, 83, 93, 95–99, 127, 128, 145 heterogeneous bone, 53, 60 material, xi, 21, 50, 129 media, 146 medium, 7, 8, 20, 52, 131, 137, 138 rod, 186 solid, 141–143, 145, 151 structure, xi, 8, 9, 154 homogenization, 155, 170, 186, 191 approaches, 1 higher order, xii, 6, 24, 40 method, xii–xiv, 2, 5, 6, 8, 18, 20, 21, 23, 31, 34, 39, 49, 50, 53, 63, 66, 69, 84, 99 problem, 21 procedure, 14, 22, 25 theory, 1, 20, 51 two-scale, 130 imperfect bonding, xiii, xiv, 81, 83, 84 contact, 81–83 intermediate continuous model, 153, 162– 164, 172 internal resonance, xiv, 141, 142, 148, 186 layered composite, xiii, xiv, 2, 23, 24, 28, 63, 65, 68, 101, 130–133, 136 viscoelastic solid, 141

INDEX

local

231

media, 5, 6, 146 approximation, 172 modulus, 66, 91 destruction, xi phenomena, 5 displacements, 41 problem, 19, 86 functionals, 20 properties, 82 model, 153, 176, 189 regime, 76 operator, 21, 155, 190 spring, 179, 183 perturbation, 111, 129 stiffness, 83, 106 reflection, 28, 53, 70 theory, xiii, 63 stresses, 57, 84, 89, 90 vibration, xiii, 123, 142, 146, 186 variation, 53 nonlinearity, xi, 3, 6, 70, 72, 74, 76– vibration, 67, 104 78, 83, 90, 92, 94, 97, 99, 106, localization, xi, 112, 113, 121, 123, 124, 109, 111, 126, 127, 144, 145, 130, 135 147, 149, 152, 154, 186, 190 effect, 111, 118, 139 Duffing-type, xiii frequency, 113, 119, 129, 133–135, effect, xiii, 2, 126, 128 137, 139, 140 geometrical, xiii, 4, 63, 66, 143, 151 of vibration, xiii, 111, 112, 119, 130 physical, xiii, 4, 63, 64, 151 logistic structural, xiii, 4, 81 DDE, 193, 194 nonlocal equation, 201 interaction, xiv, 172 map, 195 model, 153, 176 model, 193, 195 operator, 155, 164, 190 ODE, 195, 196, 201 scheme, 190 Lyapunov theory, 50, 170 dimension, xiv, 199, 200 numerical exponents, xiv, 199, 200, 203–205 algorithm, 19 stability, 156 analysis, xiii, 19, 193 approaches, xii, xv, 142, 154 molecular calculation, 51, 54 biology, 153 computation, 20, 107 chain, 79, 107 homogenization, xv dynamics, xiv, 153, 154, 189 integration, 7, 89, 106, 149, 150, 197 nonhomogeneous investigations, 159 material, xii, 5, 70 methods, 7, 101 media, 40, 66, 70 modeling, 7, 19, 106 medium, xi, 1, 2, 23 procedure, 101 structure, xi simulation, xiv, 149, 152, 163, 189 nonlinear effect, xi, 3, 70, 76, 79, 90, 99, 127 optical elastic moduli, 3 mode, 161 elastic support, 124 motion, 185 lattice, xiii, 112, 125, 126, 180 waveguide, 154 material, 66, 70

232

Pad´e approximation, xiv, 103, 115, 125, 153, 164, 190, 193, 195–197 Pad´e approximation, xii, xiv pass band, xiii, 2, 4, 23, 32–34, 36, 38, 48, 60, 62, 71, 72, 126, 127, 133 polarization, xii, 8, 16 pseudo-spectral method, xiii, xiv, 7, 101, 103 refraction, xi, 23 solution analytical, xiii, xv, 1, 5–7, 12, 19, 26, 72, 73, 78, 81, 85, 89, 92, 99, 108, 109, 136, 163 numerical, xv, 1, 18–20, 71, 108, 109, 130, 150, 198–200, 202 wave, 181, 188 stop band, xiii, 2, 4, 23, 29, 32–34, 36, 38, 46, 48, 50, 60, 62, 71, 72, 113, 117, 121, 127, 130, 133– 135, 139, 140, 179 tension impulse, xiii, 101, 109, 110 Toda lattice, 153, 179, 181 wave acoustic, 53 antiplane shear, xiii, 51, 59, 129, 137 dispersion, 153 equation, xii, 5, 29, 40, 46, 52, 55, 66, 70, 72, 82, 92, 101–103, 106, 131, 137 evolution, xii filter, 2, 23 filtering, 47 harmonic, 2, 28, 29, 45, 52, 58, 76, 91, 132 linear, 71, 79 localization, xiii, 97, 105–108, 129, 130, 133–137, 139, 140 long, 21, 29, 40, 59, 62, 70, 99, 159, 177, 179, 180, 185

INDEX

longitudinal, 23, 66 macroscopic, xiii, 41, 44, 55, 59, 66, 69, 71, 81, 84, 91, 141 microscopic, xiii, 26, 28 non-dimensional, 177 nonlinear, 6, 69, 77, 78, 86, 98, 103, 108 nonstationary, 101 plane, 129, 138 profile, 72, 92, 101 propagation, xi–xiv, 1, 2, 6, 39, 45, 46, 48, 59, 70, 75, 76, 92, 97, 99, 101, 116, 138, 146, 153, 154, 175, 177, 178 properties, 138 scattering, 28 shock, 97 standing, 2, 33 stationary, 72, 92 travelling, 179 vector, 45, 46, 58, 91, 92, 138 velocity, 46, 78, 95, 99